# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_ZnFeF5Htaz
_database_code_depnum_ccdc_archive 'CCDC 1527796'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 F5 Fe1.06 N3 Zn0.94'
_chemical_formula_weight         281.72
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Zn Zn 0.284 1.430 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.346 0.844 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.0753(2)
_cell_length_b                   7.44521(17)
_cell_length_c                   9.4607(2)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     639.24(3)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5582
_pd_meas_2theta_range_min        5.11700
_pd_meas_2theta_range_max        99.99400
_pd_meas_2theta_range_inc        0.017001

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        1.1122
_pd_proc_ls_prof_wR_factor       1.5317
_pd_proc_ls_prof_wR_expected     1.0782

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       11.8900
_pd_proc_ls_prof_cwR_factor      7.2729
_pd_proc_ls_prof_cwR_expected    5.1198

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            2.0180
_pd_proc_ls_prof_echi2           2.1286
_refine_ls_goodness_of_fit_all   1.4206

#  Items related to LS refinement

_refine_ls_R_I_factor            4.0239
_refine_ls_number_reflns         413
_refine_ls_number_parameters     52
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        5.0537
_pd_proc_2theta_range_max        99.9307
_pd_proc_2theta_range_inc        0.017001
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Zn1 0.75000 0.75000 0.75000 0.0278(5) 0.94000 Uiso Zn
Fe1 0.75000 0.75000 0.75000 0.0278(5) 0.06000 Uiso Fe
Fe2 0.50000 0.50000 0.50000 0.0236(7) 1.00000 Uiso Fe
F1 0.50000 0.75000 0.4240(4) 0.0308(9) 1.00000 Uiso F
F2 0.6476(2) 0.5583(3) 0.63418(19) 0.0308(9) 1.00000 Uiso F
N1 0.9241(4) 0.75000 0.5818(4) 0.01267 1.00000 Uiso N
N2 1.00000 0.75000 0.3686(6) 0.01267 1.00000 Uiso N
C1 0.8778(6) 0.75000 0.4500(5) 0.01267 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn1 F2 2.025(2) 1_555 ?
Zn1 F2 2.025(2) 3_656 ?
Zn1 F2 2.025(2) 13_666 ?
Zn1 F2 2.025(2) 15_565 ?
Zn1 N1 2.242(4) 1_555 ?
Zn1 N1 3.359(4) 2_466 ?
Zn1 N1 2.242(4) 3_656 ?
Zn1 N1 3.359(4) 4_765 ?
Zn1 C1 3.066(5) 1_555 ?
Zn1 C1 3.066(5) 3_656 ?
Fe1 F2 2.025(2) 1_555 ?
Fe1 F2 2.025(2) 3_656 ?
Fe1 F2 2.025(2) 13_666 ?
Fe1 F2 2.025(2) 15_565 ?
Fe1 N1 2.242(4) 1_555 ?
Fe1 N1 3.359(4) 2_466 ?
Fe1 N1 2.242(4) 3_656 ?
Fe1 N1 3.359(4) 4_765 ?
Fe1 C1 3.066(5) 1_555 ?
Fe1 C1 3.066(5) 3_656 ?
Fe2 F1 1.9954(14) 1_555 ?
Fe2 F1 1.9954(14) 5_666 ?
Fe2 F2 1.8958(18) 1_555 ?
Fe2 F2 1.8958(18) 5_666 ?
Fe2 F2 1.8958(18) 10_566 ?
Fe2 F2 1.8958(18) 14_655 ?
F1 Fe2 1.9954(14) 1_555 ?
F1 Fe2 1.9954(14) 4_665 ?
F1 F2 2.790(3) 1_555 ?
F1 F2 2.790(3) 4_665 ?
F1 F2 2.714(2) 5_666 ?
F1 F2 2.714(2) 8_556 ?
F1 F2 2.714(2) 10_566 ?
F1 F2 2.714(2) 11_656 ?
F1 F2 2.790(3) 14_655 ?
F1 F2 2.790(3) 15_565 ?
F1 N2 2.768(7) 2_465 ?
F1 C1 3.437(5) 1_555 ?
F1 C1 3.437(5) 4_665 ?
F2 Zn1 2.025(2) 1_555 ?
F2 Fe1 2.025(2) 1_555 ?
F2 Fe2 1.8958(18) 1_555 ?
F2 F1 2.790(3) 1_555 ?
F2 F1 2.714(2) 5_666 ?
F2 F2 2.874(3) 3_656 ?
F2 F2 2.683(3) 10_566 ?
F2 F2 2.679(3) 14_655 ?
F2 F2 2.854(3) 15_565 ?
F2 N1 2.929(4) 1_555 ?
F2 N1 3.111(4) 3_656 ?
F2 N2 3.461(4) 6_645 ?
F2 C1 3.072(5) 1_555 ?
F2 C1 3.204(4) 8_546 ?
N1 Zn1 2.242(4) 1_555 ?
N1 Zn1 3.359(4) 2_566 ?
N1 Fe1 2.242(4) 1_555 ?
N1 Fe1 3.359(4) 2_566 ?
N1 F2 2.929(4) 1_555 ?
N1 F2 3.111(4) 3_656 ?
N1 F2 3.111(4) 13_666 ?
N1 F2 2.929(4) 15_565 ?
N1 N1 1.378(5) 4_765 ?
N1 N2 2.131(7) 1_555 ?
N1 C1 1.316(6) 1_555 ?
N1 C1 2.188(6) 4_765 ?
N2 F1 2.768(7) 2_565 ?
N2 F2 3.461(4) 6_654 ?
N2 F2 3.461(4) 7_564 ?
N2 F2 3.461(4) 9_554 ?
N2 F2 3.461(4) 12_664 ?
N2 N1 2.131(7) 1_555 ?
N2 N1 2.131(7) 4_765 ?
N2 C1 1.350(6) 1_555 ?
N2 C1 1.350(6) 4_765 ?
C1 Zn1 3.066(5) 1_555 ?
C1 Fe1 3.066(5) 1_555 ?
C1 F1 3.437(5) 1_555 ?
C1 F2 3.072(5) 1_555 ?
C1 F2 3.204(4) 8_556 ?
C1 F2 3.204(4) 10_566 ?
C1 F2 3.072(5) 15_565 ?
C1 N1 1.316(6) 1_555 ?
C1 N1 2.188(6) 4_765 ?
C1 N2 1.350(6) 1_555 ?
C1 C1 2.218(8) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Zn1 F2 90.38(13) 1_555 3_656 ?
F2 Zn1 F2 180.00(18) 1_555 13_666 ?
F2 Zn1 F2 89.62(15) 1_555 15_565 ?
F2 Zn1 N1 86.52(18) 1_555 1_555 ?
F2 Zn1 N1 81.50(15) 1_555 2_466 ?
F2 Zn1 N1 93.48(19) 1_555 3_656 ?
F2 Zn1 N1 98.50(16) 1_555 4_765 ?
F2 Zn1 C1 70.90(18) 1_555 1_555 ?
F2 Zn1 C1 109.1(2) 1_555 3_656 ?
F2 Zn1 F2 89.62(15) 3_656 13_666 ?
F2 Zn1 F2 180.00(18) 3_656 15_565 ?
F2 Zn1 N1 93.48(19) 3_656 1_555 ?
F2 Zn1 N1 98.50(16) 3_656 2_466 ?
F2 Zn1 N1 86.52(18) 3_656 3_656 ?
F2 Zn1 N1 81.50(15) 3_656 4_765 ?
F2 Zn1 C1 109.1(2) 3_656 1_555 ?
F2 Zn1 C1 70.90(18) 3_656 3_656 ?
F2 Zn1 F2 90.38(13) 13_666 15_565 ?
F2 Zn1 N1 93.48(19) 13_666 1_555 ?
F2 Zn1 N1 98.50(16) 13_666 2_466 ?
F2 Zn1 N1 86.52(18) 13_666 3_656 ?
F2 Zn1 N1 81.50(15) 13_666 4_765 ?
F2 Zn1 C1 109.1(2) 13_666 1_555 ?
F2 Zn1 C1 70.90(18) 13_666 3_656 ?
F2 Zn1 N1 86.52(18) 15_565 1_555 ?
F2 Zn1 N1 81.50(15) 15_565 2_466 ?
F2 Zn1 N1 93.48(19) 15_565 3_656 ?
F2 Zn1 N1 98.50(16) 15_565 4_765 ?
F2 Zn1 C1 70.90(18) 15_565 1_555 ?
F2 Zn1 C1 109.1(2) 15_565 3_656 ?
N1 Zn1 N1 163.1(2) 1_555 2_466 ?
N1 Zn1 N1 180.0(3) 1_555 3_656 ?
N1 Zn1 C1 157.4(3) 1_555 3_656 ?
N1 Zn1 N1 180.00(20) 2_466 4_765 ?
N1 Zn1 C1 140.5(2) 2_466 1_555 ?
N1 Zn1 N1 163.1(2) 3_656 4_765 ?
N1 Zn1 C1 157.4(3) 3_656 1_555 ?
N1 Zn1 C1 140.5(2) 4_765 3_656 ?
C1 Zn1 C1 180.0(3) 1_555 3_656 ?
F2 Fe1 F2 90.38(13) 1_555 3_656 ?
F2 Fe1 F2 180.00(18) 1_555 13_666 ?
F2 Fe1 F2 89.62(15) 1_555 15_565 ?
F2 Fe1 N1 86.52(18) 1_555 1_555 ?
F2 Fe1 N1 81.50(15) 1_555 2_466 ?
F2 Fe1 N1 93.48(19) 1_555 3_656 ?
F2 Fe1 N1 98.50(16) 1_555 4_765 ?
F2 Fe1 C1 70.90(18) 1_555 1_555 ?
F2 Fe1 C1 109.1(2) 1_555 3_656 ?
F2 Fe1 F2 89.62(15) 3_656 13_666 ?
F2 Fe1 F2 180.00(18) 3_656 15_565 ?
F2 Fe1 N1 93.48(19) 3_656 1_555 ?
F2 Fe1 N1 98.50(16) 3_656 2_466 ?
F2 Fe1 N1 86.52(18) 3_656 3_656 ?
F2 Fe1 N1 81.50(15) 3_656 4_765 ?
F2 Fe1 C1 109.1(2) 3_656 1_555 ?
F2 Fe1 C1 70.90(18) 3_656 3_656 ?
F2 Fe1 F2 90.38(13) 13_666 15_565 ?
F2 Fe1 N1 93.48(19) 13_666 1_555 ?
F2 Fe1 N1 98.50(16) 13_666 2_466 ?
F2 Fe1 N1 86.52(18) 13_666 3_656 ?
F2 Fe1 N1 81.50(15) 13_666 4_765 ?
F2 Fe1 C1 109.1(2) 13_666 1_555 ?
F2 Fe1 C1 70.90(18) 13_666 3_656 ?
F2 Fe1 N1 86.52(18) 15_565 1_555 ?
F2 Fe1 N1 81.50(15) 15_565 2_466 ?
F2 Fe1 N1 93.48(19) 15_565 3_656 ?
F2 Fe1 N1 98.50(16) 15_565 4_765 ?
F2 Fe1 C1 70.90(18) 15_565 1_555 ?
F2 Fe1 C1 109.1(2) 15_565 3_656 ?
N1 Fe1 N1 163.1(2) 1_555 2_466 ?
N1 Fe1 N1 180.0(3) 1_555 3_656 ?
N1 Fe1 C1 157.4(3) 1_555 3_656 ?
N1 Fe1 N1 180.00(20) 2_466 4_765 ?
N1 Fe1 C1 140.5(2) 2_466 1_555 ?
N1 Fe1 N1 163.1(2) 3_656 4_765 ?
N1 Fe1 C1 157.4(3) 3_656 1_555 ?
N1 Fe1 C1 140.5(2) 4_765 3_656 ?
C1 Fe1 C1 180.0(3) 1_555 3_656 ?
F1 Fe2 F1 180.00(12) 1_555 5_666 ?
F1 Fe2 F2 91.59(16) 1_555 1_555 ?
F1 Fe2 F2 88.41(11) 1_555 5_666 ?
F1 Fe2 F2 88.41(11) 1_555 10_566 ?
F1 Fe2 F2 91.59(16) 1_555 14_655 ?
F1 Fe2 F2 88.41(11) 5_666 1_555 ?
F1 Fe2 F2 91.59(16) 5_666 5_666 ?
F1 Fe2 F2 91.59(16) 5_666 10_566 ?
F1 Fe2 F2 88.41(11) 5_666 14_655 ?
F2 Fe2 F2 180.00(18) 1_555 5_666 ?
F2 Fe2 F2 90.09(14) 1_555 10_566 ?
F2 Fe2 F2 89.91(13) 1_555 14_655 ?
F2 Fe2 F2 89.91(13) 5_666 10_566 ?
F2 Fe2 F2 90.09(14) 5_666 14_655 ?
F2 Fe2 F2 180.00(18) 10_566 14_655 ?
Fe2 F1 Fe2 137.76(6) 1_555 4_665 ?
Fe2 F1 F2 102.73(11) 1_555 4_665 ?
Fe2 F1 F2 149.54(12) 1_555 8_556 ?
Fe2 F1 F2 149.54(12) 1_555 11_656 ?
Fe2 F1 F2 102.73(11) 1_555 15_565 ?
Fe2 F1 N2 111.1(3) 1_555 2_465 ?
Fe2 F1 C1 88.52(4) 1_555 1_555 ?
Fe2 F1 C1 88.52(19) 1_555 4_665 ?
Fe2 F1 F2 102.73(11) 4_665 1_555 ?
Fe2 F1 F2 149.54(12) 4_665 5_666 ?
Fe2 F1 F2 149.54(12) 4_665 10_566 ?
Fe2 F1 F2 102.73(11) 4_665 14_655 ?
Fe2 F1 N2 111.1(3) 4_665 2_465 ?
Fe2 F1 C1 88.52(19) 4_665 1_555 ?
Fe2 F1 C1 88.52(19) 4_665 4_665 ?
F2 F1 F2 89.10(13) 1_555 4_665 ?
F2 F1 F2 87.07(11) 1_555 5_666 ?
F2 F1 F2 109.89(13) 1_555 8_556 ?
F2 F1 F2 58.33(10) 1_555 10_566 ?
F2 F1 F2 144.50(14) 1_555 11_656 ?
F2 F1 F2 57.38(11) 1_555 14_655 ?
F2 F1 F2 61.53(12) 1_555 15_565 ?
F2 F1 N2 135.5(3) 1_555 2_465 ?
F2 F1 C1 58.01(15) 1_555 1_555 ?
F2 F1 C1 115.3(2) 1_555 4_665 ?
F2 F1 F2 109.89(13) 4_665 5_666 ?
F2 F1 F2 87.07(11) 4_665 8_556 ?
F2 F1 F2 144.50(14) 4_665 10_566 ?
F2 F1 F2 58.33(10) 4_665 11_656 ?
F2 F1 F2 61.53(12) 4_665 14_655 ?
F2 F1 F2 57.38(11) 4_665 15_565 ?
F2 F1 N2 135.5(3) 4_665 2_465 ?
F2 F1 C1 115.3(2) 4_665 1_555 ?
F2 F1 C1 58.01(15) 4_665 4_665 ?
F2 F1 F2 156.60(14) 5_666 8_556 ?
F2 F1 F2 59.15(9) 5_666 10_566 ?
F2 F1 F2 115.50(13) 5_666 11_656 ?
F2 F1 F2 58.33(10) 5_666 14_655 ?
F2 F1 F2 144.50(14) 5_666 15_565 ?
F2 F1 N2 78.30(19) 5_666 2_465 ?
F2 F1 C1 120.5(2) 5_666 1_555 ?
F2 F1 C1 61.46(13) 5_666 4_665 ?
F2 F1 F2 115.50(13) 8_556 10_566 ?
F2 F1 F2 59.15(9) 8_556 11_656 ?
F2 F1 F2 144.50(14) 8_556 14_655 ?
F2 F1 F2 58.33(10) 8_556 15_565 ?
F2 F1 N2 78.30(19) 8_556 2_465 ?
F2 F1 C1 61.46(13) 8_556 1_555 ?
F2 F1 C1 120.5(2) 8_556 4_665 ?
F2 F1 F2 156.60(14) 10_566 11_656 ?
F2 F1 F2 87.07(11) 10_566 14_655 ?
F2 F1 F2 109.89(13) 10_566 15_565 ?
F2 F1 N2 78.30(19) 10_566 2_465 ?
F2 F1 C1 61.46(13) 10_566 1_555 ?
F2 F1 C1 120.5(2) 10_566 4_665 ?
F2 F1 F2 109.89(13) 11_656 14_655 ?
F2 F1 F2 87.07(11) 11_656 15_565 ?
F2 F1 N2 78.30(19) 11_656 2_465 ?
F2 F1 C1 120.5(2) 11_656 1_555 ?
F2 F1 C1 61.46(13) 11_656 4_665 ?
F2 F1 F2 89.10(13) 14_655 15_565 ?
F2 F1 N2 135.5(3) 14_655 2_465 ?
F2 F1 C1 115.3(2) 14_655 1_555 ?
F2 F1 C1 58.01(15) 14_655 4_665 ?
F2 F1 N2 135.5(3) 15_565 2_465 ?
F2 F1 C1 58.01(15) 15_565 1_555 ?
F2 F1 C1 115.3(2) 15_565 4_665 ?
N2 F1 C1 94.1(2) 2_465 1_555 ?
N2 F1 C1 94.1(2) 2_465 4_665 ?
C1 F1 C1 171.8(3) 1_555 4_665 ?
Zn1 F2 Fe2 147.98(8) 1_555 1_555 ?
Zn1 F2 F1 104.20(15) 1_555 1_555 ?
Zn1 F2 F1 158.79(10) 1_555 5_666 ?
Zn1 F2 F2 137.73(12) 1_555 10_566 ?
Zn1 F2 F2 117.31(11) 1_555 14_655 ?
Zn1 F2 F2 45.19(9) 1_555 15_565 ?
Zn1 F2 N1 49.83(12) 1_555 1_555 ?
Zn1 F2 N1 46.01(12) 1_555 3_656 ?
Zn1 F2 N2 107.35(10) 1_555 6_645 ?
Zn1 F2 C1 70.57(17) 1_555 1_555 ?
Zn1 F2 C1 109.89(14) 1_555 8_546 ?
Fe1 F2 Fe2 147.98(8) 1_555 1_555 ?
Fe1 F2 F1 104.20(15) 1_555 1_555 ?
Fe1 F2 F1 158.79(10) 1_555 5_666 ?
Fe1 F2 F2 137.73(12) 1_555 10_566 ?
Fe1 F2 F2 117.31(11) 1_555 14_655 ?
Fe1 F2 F2 45.19(9) 1_555 15_565 ?
Fe1 F2 N1 49.83(12) 1_555 1_555 ?
Fe1 F2 N1 46.01(12) 1_555 3_656 ?
Fe1 F2 N2 107.35(10) 1_555 6_645 ?
Fe1 F2 C1 70.57(17) 1_555 1_555 ?
Fe1 F2 C1 109.89(14) 1_555 8_546 ?
Fe2 F2 F1 45.63(9) 1_555 1_555 ?
Fe2 F2 F1 47.30(8) 1_555 5_666 ?
Fe2 F2 F2 165.39(12) 1_555 3_656 ?
Fe2 F2 F2 45.04(9) 1_555 14_655 ?
Fe2 F2 F2 103.24(12) 1_555 15_565 ?
Fe2 F2 N1 127.13(17) 1_555 1_555 ?
Fe2 F2 N1 122.38(17) 1_555 3_656 ?
Fe2 F2 N2 90.22(19) 1_555 6_645 ?
Fe2 F2 C1 102.0(2) 1_555 1_555 ?
Fe2 F2 C1 97.5(2) 1_555 8_546 ?
F1 F2 F1 92.93(10) 1_555 5_666 ?
F1 F2 F2 148.65(16) 1_555 3_656 ?
F1 F2 F2 59.41(10) 1_555 10_566 ?
F1 F2 F2 61.31(11) 1_555 14_655 ?
F1 F2 F2 59.23(11) 1_555 15_565 ?
F1 F2 N1 92.38(15) 1_555 1_555 ?
F1 F2 N1 106.28(19) 1_555 3_656 ?
F1 F2 N2 127.59(20) 1_555 6_645 ?
F1 F2 C1 71.62(17) 1_555 1_555 ?
F1 F2 C1 120.15(16) 1_555 8_546 ?
F1 F2 F2 118.29(12) 5_666 3_656 ?
F1 F2 F2 62.26(10) 5_666 10_566 ?
F1 F2 F2 60.43(9) 5_666 14_655 ?
F1 F2 F2 147.75(12) 5_666 15_565 ?
F1 F2 N1 143.19(13) 5_666 1_555 ?
F1 F2 N1 117.38(15) 5_666 3_656 ?
F1 F2 N2 51.55(14) 5_666 6_645 ?
F1 F2 C1 127.84(17) 5_666 1_555 ?
F1 F2 C1 70.46(15) 5_666 8_546 ?
F2 F2 F2 136.19(12) 3_656 10_566 ?
F2 F2 F2 130.30(12) 3_656 14_655 ?
F2 F2 F2 90.00(11) 3_656 15_565 ?
F2 F2 N1 64.84(12) 3_656 1_555 ?
F2 F2 N1 58.44(11) 3_656 3_656 ?
F2 F2 N2 76.21(10) 3_656 6_645 ?
F2 F2 C1 89.58(17) 3_656 1_555 ?
F2 F2 C1 76.58(14) 3_656 8_546 ?
F2 F2 F2 90.00(11) 10_566 14_655 ?
F2 F2 F2 108.88(13) 10_566 15_565 ?
F2 F2 N1 89.86(14) 10_566 1_555 ?
F2 F2 N1 164.92(18) 10_566 3_656 ?
F2 F2 N2 113.06(20) 10_566 6_645 ?
F2 F2 C1 67.27(14) 10_566 1_555 ?
F2 F2 C1 62.16(14) 10_566 8_546 ?
F2 F2 F2 90.00(12) 14_655 15_565 ?
F2 F2 N1 148.95(18) 14_655 1_555 ?
F2 F2 N1 77.93(13) 14_655 3_656 ?
F2 F2 N2 67.23(13) 14_655 6_645 ?
F2 F2 C1 132.8(2) 14_655 1_555 ?
F2 F2 C1 130.7(2) 14_655 8_546 ?
F2 F2 N1 60.84(12) 15_565 1_555 ?
F2 F2 N1 62.70(12) 15_565 3_656 ?
F2 F2 N2 131.54(14) 15_565 6_645 ?
F2 F2 C1 62.32(15) 15_565 1_555 ?
F2 F2 C1 135.75(15) 15_565 8_546 ?
N1 F2 N1 95.84(18) 1_555 3_656 ?
N1 F2 N2 139.73(16) 1_555 6_645 ?
N1 F2 C1 75.43(11) 1_555 8_546 ?
N1 F2 N2 70.73(10) 3_656 6_645 ?
N1 F2 C1 114.8(2) 3_656 1_555 ?
N1 F2 C1 132.81(19) 3_656 8_546 ?
N2 F2 C1 159.2(2) 6_645 1_555 ?
N2 F2 C1 86.36(18) 6_645 8_546 ?
C1 F2 C1 75.43(13) 1_555 8_546 ?
Zn1 N1 Zn1 106.51(11) 1_555 2_566 ?
Zn1 N1 Fe1 106.51(11) 1_555 2_566 ?
Zn1 N1 N1 134.8(3) 1_555 4_765 ?
Zn1 N1 N2 154.1(3) 1_555 1_555 ?
Zn1 N1 C1 116.6(4) 1_555 1_555 ?
Zn1 N1 C1 169.5(3) 1_555 4_765 ?
Zn1 N1 Fe1 106.51(11) 2_566 1_555 ?
Zn1 N1 F2 132.40(11) 2_566 1_555 ?
Zn1 N1 F2 77.00(10) 2_566 3_656 ?
Zn1 N1 F2 77.00(10) 2_566 13_666 ?
Zn1 N1 F2 132.40(11) 2_566 15_565 ?
Zn1 N1 N2 99.4(2) 2_566 1_555 ?
Zn1 N1 C1 136.9(4) 2_566 1_555 ?
Zn1 N1 C1 63.0(2) 2_566 4_765 ?
Fe1 N1 Fe1 106.51(11) 1_555 2_566 ?
Fe1 N1 N1 134.8(3) 1_555 4_765 ?
Fe1 N1 N2 154.1(3) 1_555 1_555 ?
Fe1 N1 C1 116.6(4) 1_555 1_555 ?
Fe1 N1 C1 169.5(3) 1_555 4_765 ?
Fe1 N1 F2 132.40(11) 2_566 1_555 ?
Fe1 N1 F2 77.00(10) 2_566 3_656 ?
Fe1 N1 F2 77.00(10) 2_566 13_666 ?
Fe1 N1 F2 132.40(11) 2_566 15_565 ?
Fe1 N1 N2 99.4(2) 2_566 1_555 ?
Fe1 N1 C1 136.9(4) 2_566 1_555 ?
Fe1 N1 C1 63.0(2) 2_566 4_765 ?
F2 N1 F2 56.72(11) 1_555 3_656 ?
F2 N1 F2 84.16(13) 1_555 13_666 ?
F2 N1 F2 58.32(12) 1_555 15_565 ?
F2 N1 N1 148.9(3) 1_555 4_765 ?
F2 N1 N2 115.9(2) 1_555 1_555 ?
F2 N1 C1 83.5(4) 1_555 1_555 ?
F2 N1 C1 143.2(3) 1_555 4_765 ?
F2 N1 F2 54.61(11) 3_656 13_666 ?
F2 N1 F2 84.16(13) 3_656 15_565 ?
F2 N1 N1 102.1(3) 3_656 4_765 ?
F2 N1 N2 152.2(3) 3_656 1_555 ?
F2 N1 C1 138.7(4) 3_656 1_555 ?
F2 N1 C1 131.6(3) 3_656 4_765 ?
F2 N1 F2 56.72(11) 13_666 15_565 ?
F2 N1 N1 102.1(3) 13_666 4_765 ?
F2 N1 N2 152.2(3) 13_666 1_555 ?
F2 N1 C1 138.7(4) 13_666 1_555 ?
F2 N1 C1 131.6(3) 13_666 4_765 ?
F2 N1 N1 148.9(3) 15_565 4_765 ?
F2 N1 N2 115.9(2) 15_565 1_555 ?
F2 N1 C1 83.5(4) 15_565 1_555 ?
F2 N1 C1 143.2(3) 15_565 4_765 ?
N1 N1 N2 71.1(4) 4_765 1_555 ?
N1 N1 C1 108.6(6) 4_765 1_555 ?
C1 N1 C1 73.9(5) 1_555 4_765 ?
F1 N2 F2 50.16(16) 2_565 6_654 ?
F1 N2 F2 50.16(16) 2_565 7_564 ?
F1 N2 F2 50.16(16) 2_565 9_554 ?
F1 N2 F2 50.16(16) 2_565 12_664 ?
F1 N2 N1 161.1(3) 2_565 1_555 ?
F1 N2 N1 161.1(3) 2_565 4_765 ?
F1 N2 C1 124.8(5) 2_565 1_555 ?
F1 N2 C1 124.8(5) 2_565 4_765 ?
F2 N2 F2 100.31(12) 6_654 7_564 ?
F2 N2 F2 45.53(10) 6_654 9_554 ?
F2 N2 F2 83.08(12) 6_654 12_664 ?
F2 N2 N1 118.8(2) 6_654 1_555 ?
F2 N2 N1 137.0(2) 6_654 4_765 ?
F2 N2 C1 92.7(3) 6_654 1_555 ?
F2 N2 C1 133.1(4) 6_654 4_765 ?
F2 N2 F2 83.08(12) 7_564 9_554 ?
F2 N2 F2 45.53(10) 7_564 12_664 ?
F2 N2 N1 137.0(2) 7_564 1_555 ?
F2 N2 N1 118.8(2) 7_564 4_765 ?
F2 N2 C1 133.1(4) 7_564 1_555 ?
F2 N2 C1 92.7(3) 7_564 4_765 ?
F2 N2 F2 100.31(12) 9_554 12_664 ?
F2 N2 N1 137.0(2) 9_554 1_555 ?
F2 N2 N1 118.8(2) 9_554 4_765 ?
F2 N2 C1 133.1(4) 9_554 1_555 ?
F2 N2 C1 92.7(3) 9_554 4_765 ?
F2 N2 N1 118.8(2) 12_664 1_555 ?
F2 N2 N1 137.0(2) 12_664 4_765 ?
F2 N2 C1 92.7(3) 12_664 1_555 ?
F2 N2 C1 133.1(4) 12_664 4_765 ?
N1 N2 C1 74.1(4) 1_555 4_765 ?
N1 N2 C1 74.1(4) 4_765 1_555 ?
C1 N2 C1 110.4(7) 1_555 4_765 ?
Zn1 C1 F1 71.88(14) 1_555 1_555 ?
Zn1 C1 F2 89.05(13) 1_555 8_556 ?
Zn1 C1 F2 89.05(13) 1_555 10_566 ?
Zn1 C1 N1 77.5(2) 1_555 4_765 ?
Zn1 C1 N2 147.0(4) 1_555 1_555 ?
Zn1 C1 C1 112.2(3) 1_555 4_765 ?
Fe1 C1 F1 71.88(14) 1_555 1_555 ?
Fe1 C1 F2 89.05(13) 1_555 8_556 ?
Fe1 C1 F2 89.05(13) 1_555 10_566 ?
Fe1 C1 N1 77.5(2) 1_555 4_765 ?
Fe1 C1 N2 147.0(4) 1_555 1_555 ?
Fe1 C1 C1 112.2(3) 1_555 4_765 ?
F1 C1 F2 50.38(14) 1_555 1_555 ?
F1 C1 F2 48.08(12) 1_555 8_556 ?
F1 C1 F2 48.08(12) 1_555 10_566 ?
F1 C1 F2 50.38(14) 1_555 15_565 ?
F1 C1 N1 112.7(3) 1_555 1_555 ?
F1 C1 N1 149.4(2) 1_555 4_765 ?
F1 C1 N2 141.1(3) 1_555 1_555 ?
F1 C1 C1 175.9(3) 1_555 4_765 ?
F2 C1 F2 91.74(14) 1_555 8_556 ?
F2 C1 F2 50.57(13) 1_555 10_566 ?
F2 C1 F2 55.37(14) 1_555 15_565 ?
F2 C1 N1 71.3(3) 1_555 1_555 ?
F2 C1 N1 103.6(2) 1_555 4_765 ?
F2 C1 N2 151.90(9) 1_555 1_555 ?
F2 C1 C1 132.8(3) 1_555 4_765 ?
F2 C1 F2 91.51(13) 8_556 10_566 ?
F2 C1 F2 50.57(13) 8_556 15_565 ?
F2 C1 N1 116.3(3) 8_556 1_555 ?
F2 C1 N1 132.6(2) 8_556 4_765 ?
F2 C1 N2 113.2(3) 8_556 1_555 ?
F2 C1 C1 130.7(3) 8_556 4_765 ?
F2 C1 F2 91.74(14) 10_566 15_565 ?
F2 C1 N1 116.3(3) 10_566 1_555 ?
F2 C1 N1 132.6(2) 10_566 4_765 ?
F2 C1 N2 113.2(3) 10_566 1_555 ?
F2 C1 C1 130.7(3) 10_566 4_765 ?
F2 C1 N1 71.3(3) 15_565 1_555 ?
F2 C1 N1 103.6(2) 15_565 4_765 ?
F2 C1 N2 151.9(4) 15_565 1_555 ?
F2 C1 C1 132.8(3) 15_565 4_765 ?
N1 C1 N2 106.2(6) 1_555 1_555 ?
N1 C1 C1 71.4(4) 1_555 4_765 ?
N1 C1 N2 69.5(4) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_CoGaF5Htaz
_database_code_depnum_ccdc_archive 'CCDC 1527728'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 Co F5 Ga N3'
_chemical_formula_weight         289.7
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.349 0.972 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.231 1.608 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.0193(4)
_cell_length_b                   7.3421(3)
_cell_length_c                   9.3901(4)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     621.82(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5582
_pd_meas_2theta_range_min        5.11700
_pd_meas_2theta_range_max        99.99400
_pd_meas_2theta_range_inc        0.017001

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.7247
_pd_proc_ls_prof_wR_factor       0.9884
_pd_proc_ls_prof_wR_expected     0.7054

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       18.4947
_pd_proc_ls_prof_cwR_factor      9.1477
_pd_proc_ls_prof_cwR_expected    6.5282

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            1.9635
_pd_proc_ls_prof_echi2           2.1091
_refine_ls_goodness_of_fit_all   1.4012

#  Items related to LS refinement

_refine_ls_R_I_factor            5.6598
_refine_ls_number_reflns         412
_refine_ls_number_parameters     56
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        5.1795
_pd_proc_2theta_range_max        100.0565
_pd_proc_2theta_range_inc        0.017001
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Co1 0.75000 0.75000 0.75000 0.0195(10) 1.00000 Uiso Co
Ga1 0.50000 0.50000 0.50000 0.0173(9) 1.00000 Uiso Ga
F1 0.50000 0.75000 0.4255(6) 0.0183(14) 1.00000 Uiso F
F2 0.6489(3) 0.5496(4) 0.6346(3) 0.0183(14) 1.00000 Uiso F
N1 0.9289(7) 0.75000 0.5776(6) 0.01267 1.00000 Uiso N
N2 1.00000 0.75000 0.3666(10) 0.01267 1.00000 Uiso N
C1 0.8819(9) 0.75000 0.4547(9) 0.01267 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Co1 F2 2.042(3) 1_555 ?
Co1 F2 2.042(3) 3_656 ?
Co1 F2 2.042(3) 13_666 ?
Co1 F2 2.042(3) 15_565 ?
Co1 N1 2.286(6) 1_555 ?
Co1 N1 3.318(6) 2_466 ?
Co1 N1 2.286(6) 3_656 ?
Co1 N1 3.318(6) 4_765 ?
Co1 C1 3.017(8) 1_555 ?
Co1 C1 3.017(8) 3_656 ?
Ga1 F1 1.964(2) 1_555 ?
Ga1 F1 1.964(2) 5_666 ?
Ga1 F2 1.880(3) 1_555 ?
Ga1 F2 1.880(3) 5_666 ?
Ga1 F2 1.880(3) 10_566 ?
Ga1 F2 1.880(3) 14_655 ?
F1 Ga1 1.964(2) 1_555 ?
F1 Ga1 1.964(2) 4_665 ?
F1 F2 2.797(5) 1_555 ?
F1 F2 2.797(5) 4_665 ?
F1 F2 2.638(3) 5_666 ?
F1 F2 2.638(3) 8_556 ?
F1 F2 2.638(3) 10_566 ?
F1 F2 2.638(3) 11_656 ?
F1 F2 2.797(5) 14_655 ?
F1 F2 2.797(5) 15_565 ?
F1 N2 2.743(11) 2_465 ?
F1 C1 3.455(8) 1_555 ?
F1 C1 3.455(8) 4_665 ?
F2 Co1 2.042(3) 1_555 ?
F2 Ga1 1.880(3) 1_555 ?
F2 F1 2.797(5) 1_555 ?
F2 F1 2.638(3) 5_666 ?
F2 F2 2.832(4) 3_656 ?
F2 F2 2.631(4) 10_566 ?
F2 F2 2.686(4) 14_655 ?
F2 F2 2.943(4) 15_565 ?
F2 N1 2.971(6) 1_555 ?
F2 N1 3.156(6) 3_656 ?
F2 N2 3.375(7) 6_645 ?
F2 C1 3.072(8) 1_555 ?
F2 C1 3.156(7) 8_546 ?
N1 Co1 2.286(6) 1_555 ?
N1 Co1 3.318(6) 2_566 ?
N1 F2 2.971(6) 1_555 ?
N1 F2 3.156(6) 3_656 ?
N1 F2 3.156(6) 13_666 ?
N1 F2 2.971(6) 15_565 ?
N1 N1 1.283(9) 4_765 ?
N1 N2 2.083(11) 1_555 ?
N1 C1 1.229(10) 1_555 ?
N1 C1 2.060(10) 4_765 ?
N2 F1 2.743(11) 2_565 ?
N2 F2 3.375(7) 6_654 ?
N2 F2 3.375(7) 7_564 ?
N2 F2 3.375(7) 9_554 ?
N2 F2 3.375(7) 12_664 ?
N2 N1 2.083(11) 1_555 ?
N2 N1 2.083(11) 4_765 ?
N2 C1 1.349(10) 1_555 ?
N2 C1 1.349(10) 4_765 ?
C1 Co1 3.017(8) 1_555 ?
C1 F1 3.455(8) 1_555 ?
C1 F2 3.072(8) 1_555 ?
C1 F2 3.156(7) 8_556 ?
C1 F2 3.156(7) 10_566 ?
C1 F2 3.072(8) 15_565 ?
C1 N1 1.229(10) 1_555 ?
C1 N1 2.060(10) 4_765 ?
C1 N2 1.349(10) 1_555 ?
C1 C1 2.130(11) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Co1 F2 87.81(19) 1_555 3_656 ?
F2 Co1 F2 180.0(3) 1_555 13_666 ?
F2 Co1 F2 92.2(2) 1_555 15_565 ?
F2 Co1 N1 86.53(13) 1_555 1_555 ?
F2 Co1 N1 82.5(2) 1_555 2_466 ?
F2 Co1 N1 93.5(3) 1_555 3_656 ?
F2 Co1 N1 97.5(3) 1_555 4_765 ?
F2 Co1 C1 71.85(13) 1_555 1_555 ?
F2 Co1 C1 108.2(4) 1_555 3_656 ?
F2 Co1 F2 92.2(2) 3_656 13_666 ?
F2 Co1 F2 180.0(3) 3_656 15_565 ?
F2 Co1 N1 93.5(3) 3_656 1_555 ?
F2 Co1 N1 97.5(3) 3_656 2_466 ?
F2 Co1 N1 86.5(3) 3_656 3_656 ?
F2 Co1 N1 82.5(2) 3_656 4_765 ?
F2 Co1 C1 108.2(4) 3_656 1_555 ?
F2 Co1 C1 71.8(3) 3_656 3_656 ?
F2 Co1 F2 87.81(19) 13_666 15_565 ?
F2 Co1 N1 93.5(3) 13_666 1_555 ?
F2 Co1 N1 97.5(3) 13_666 2_466 ?
F2 Co1 N1 86.5(3) 13_666 3_656 ?
F2 Co1 N1 82.5(2) 13_666 4_765 ?
F2 Co1 C1 108.2(4) 13_666 1_555 ?
F2 Co1 C1 71.8(3) 13_666 3_656 ?
F2 Co1 N1 86.5(3) 15_565 1_555 ?
F2 Co1 N1 82.5(2) 15_565 2_466 ?
F2 Co1 N1 93.5(3) 15_565 3_656 ?
F2 Co1 N1 97.5(3) 15_565 4_765 ?
F2 Co1 C1 71.8(3) 15_565 1_555 ?
F2 Co1 C1 108.2(4) 15_565 3_656 ?
N1 Co1 N1 164.1(4) 1_555 2_466 ?
N1 Co1 N1 180.0(5) 1_555 3_656 ?
N1 Co1 C1 158.3(5) 1_555 3_656 ?
N1 Co1 N1 180.0(3) 2_466 4_765 ?
N1 Co1 C1 142.4(4) 2_466 1_555 ?
N1 Co1 N1 164.1(4) 3_656 4_765 ?
N1 Co1 C1 158.3(5) 3_656 1_555 ?
N1 Co1 C1 142.4(4) 4_765 3_656 ?
C1 Co1 C1 180.0(5) 1_555 3_656 ?
F1 Ga1 F1 180.00(19) 1_555 5_666 ?
F1 Ga1 F2 93.3(2) 1_555 1_555 ?
F1 Ga1 F2 86.65(16) 1_555 5_666 ?
F1 Ga1 F2 86.65(16) 1_555 10_566 ?
F1 Ga1 F2 93.3(2) 1_555 14_655 ?
F1 Ga1 F2 86.65(16) 5_666 1_555 ?
F1 Ga1 F2 93.3(2) 5_666 5_666 ?
F1 Ga1 F2 93.3(2) 5_666 10_566 ?
F1 Ga1 F2 86.65(16) 5_666 14_655 ?
F2 Ga1 F2 180.0(3) 1_555 5_666 ?
F2 Ga1 F2 88.8(2) 1_555 10_566 ?
F2 Ga1 F2 91.2(2) 1_555 14_655 ?
F2 Ga1 F2 91.2(2) 5_666 10_566 ?
F2 Ga1 F2 88.8(2) 5_666 14_655 ?
F2 Ga1 F2 180.0(3) 10_566 14_655 ?
Ga1 F1 Ga1 138.27(8) 1_555 4_665 ?
Ga1 F1 F2 103.98(16) 1_555 4_665 ?
Ga1 F1 F2 45.34(11) 1_555 5_666 ?
Ga1 F1 F2 148.79(17) 1_555 8_556 ?
Ga1 F1 F2 45.34(11) 1_555 10_566 ?
Ga1 F1 F2 148.79(17) 1_555 11_656 ?
Ga1 F1 F2 103.98(16) 1_555 15_565 ?
Ga1 F1 N2 110.9(4) 1_555 2_465 ?
Ga1 F1 C1 88.38(7) 1_555 1_555 ?
Ga1 F1 C1 88.38(7) 1_555 4_665 ?
Ga1 F1 F2 103.98(16) 4_665 1_555 ?
Ga1 F1 F2 148.79(17) 4_665 5_666 ?
Ga1 F1 F2 45.34(11) 4_665 8_556 ?
Ga1 F1 F2 148.79(17) 4_665 10_566 ?
Ga1 F1 F2 45.34(11) 4_665 11_656 ?
Ga1 F1 F2 103.98(16) 4_665 14_655 ?
Ga1 F1 N2 110.9(4) 4_665 2_465 ?
Ga1 F1 C1 88.38(7) 4_665 1_555 ?
Ga1 F1 C1 88.38(7) 4_665 4_665 ?
F2 F1 F2 90.83(18) 1_555 4_665 ?
F2 F1 F2 87.48(17) 1_555 5_666 ?
F2 F1 F2 110.14(19) 1_555 8_556 ?
F2 F1 F2 57.80(15) 1_555 10_566 ?
F2 F1 F2 146.4(2) 1_555 11_656 ?
F2 F1 F2 57.39(16) 1_555 14_655 ?
F2 F1 F2 63.48(17) 1_555 15_565 ?
F2 F1 N2 134.6(4) 1_555 2_465 ?
F2 F1 C1 57.7(2) 1_555 1_555 ?
F2 F1 C1 115.0(3) 1_555 4_665 ?
F2 F1 F2 110.14(19) 4_665 5_666 ?
F2 F1 F2 87.48(17) 4_665 8_556 ?
F2 F1 F2 146.4(2) 4_665 10_566 ?
F2 F1 F2 57.80(15) 4_665 11_656 ?
F2 F1 F2 63.48(17) 4_665 14_655 ?
F2 F1 F2 57.39(16) 4_665 15_565 ?
F2 F1 N2 134.6(4) 4_665 2_465 ?
F2 F1 C1 115.0(3) 4_665 1_555 ?
F2 F1 C1 57.7(2) 4_665 4_665 ?
F2 F1 F2 155.30(20) 5_666 8_556 ?
F2 F1 F2 61.20(13) 5_666 10_566 ?
F2 F1 F2 112.97(18) 5_666 11_656 ?
F2 F1 F2 57.80(15) 5_666 14_655 ?
F2 F1 F2 146.4(2) 5_666 15_565 ?
F2 F1 N2 77.6(3) 5_666 2_465 ?
F2 F1 C1 121.6(3) 5_666 1_555 ?
F2 F1 C1 60.63(20) 5_666 4_665 ?
F2 F1 F2 112.97(18) 8_556 10_566 ?
F2 F1 F2 61.20(13) 8_556 11_656 ?
F2 F1 F2 146.4(2) 8_556 14_655 ?
F2 F1 F2 57.80(15) 8_556 15_565 ?
F2 F1 N2 77.6(3) 8_556 2_465 ?
F2 F1 C1 60.63(20) 8_556 1_555 ?
F2 F1 C1 121.6(3) 8_556 4_665 ?
F2 F1 F2 155.30(20) 10_566 11_656 ?
F2 F1 F2 87.48(17) 10_566 14_655 ?
F2 F1 F2 110.14(19) 10_566 15_565 ?
F2 F1 N2 77.6(3) 10_566 2_465 ?
F2 F1 C1 60.63(20) 10_566 1_555 ?
F2 F1 C1 121.6(3) 10_566 4_665 ?
F2 F1 F2 110.14(19) 11_656 14_655 ?
F2 F1 F2 87.48(17) 11_656 15_565 ?
F2 F1 N2 77.6(3) 11_656 2_465 ?
F2 F1 C1 121.6(3) 11_656 1_555 ?
F2 F1 C1 60.63(20) 11_656 4_665 ?
F2 F1 F2 90.83(18) 14_655 15_565 ?
F2 F1 N2 134.6(4) 14_655 2_465 ?
F2 F1 C1 115.0(3) 14_655 1_555 ?
F2 F1 C1 57.7(2) 14_655 4_665 ?
F2 F1 N2 134.6(4) 15_565 2_465 ?
F2 F1 C1 57.7(2) 15_565 1_555 ?
F2 F1 C1 115.0(3) 15_565 4_665 ?
N2 F1 C1 94.6(4) 2_465 1_555 ?
N2 F1 C1 94.6(4) 2_465 4_665 ?
C1 F1 C1 170.9(4) 1_555 4_665 ?
Co1 F2 Ga1 144.62(12) 1_555 1_555 ?
Co1 F2 F1 102.0(2) 1_555 1_555 ?
Co1 F2 F1 160.30(14) 1_555 5_666 ?
Co1 F2 F2 46.09(13) 1_555 3_656 ?
Co1 F2 F2 135.18(18) 1_555 10_566 ?
Co1 F2 F2 116.52(16) 1_555 14_655 ?
Co1 F2 N1 50.16(19) 1_555 1_555 ?
Co1 F2 N1 46.29(18) 1_555 3_656 ?
Co1 F2 N2 107.75(16) 1_555 6_645 ?
Co1 F2 C1 69.0(3) 1_555 1_555 ?
Co1 F2 C1 110.2(2) 1_555 8_546 ?
Ga1 F2 F1 48.01(12) 1_555 5_666 ?
Ga1 F2 F2 167.02(18) 1_555 3_656 ?
Ga1 F2 F2 45.60(14) 1_555 10_566 ?
Ga1 F2 F2 101.17(16) 1_555 15_565 ?
Ga1 F2 N1 125.6(3) 1_555 1_555 ?
Ga1 F2 N1 120.5(3) 1_555 3_656 ?
Ga1 F2 N2 91.3(3) 1_555 6_645 ?
Ga1 F2 C1 102.2(3) 1_555 1_555 ?
Ga1 F2 C1 99.3(3) 1_555 8_546 ?
F1 F2 F1 92.52(15) 1_555 5_666 ?
F1 F2 F2 147.8(2) 1_555 3_656 ?
F1 F2 F2 58.07(15) 1_555 10_566 ?
F1 F2 F2 61.31(17) 1_555 14_655 ?
F1 F2 F2 58.26(16) 1_555 15_565 ?
F1 F2 N1 91.2(2) 1_555 1_555 ?
F1 F2 N1 104.4(3) 1_555 3_656 ?
F1 F2 N2 127.2(3) 1_555 6_645 ?
F1 F2 C1 72.0(3) 1_555 1_555 ?
F1 F2 C1 120.0(2) 1_555 8_546 ?
F1 F2 F2 119.43(19) 5_666 3_656 ?
F1 F2 F2 64.13(16) 5_666 10_566 ?
F1 F2 F2 59.40(13) 5_666 14_655 ?
F1 F2 F2 146.49(16) 5_666 15_565 ?
F1 F2 N1 143.8(2) 5_666 1_555 ?
F1 F2 N1 117.3(2) 5_666 3_656 ?
F1 F2 N2 52.6(2) 5_666 6_645 ?
F1 F2 C1 129.1(3) 5_666 1_555 ?
F1 F2 C1 72.6(2) 5_666 8_546 ?
F2 F2 F2 137.33(20) 3_656 10_566 ?
F2 F2 F2 130.08(18) 3_656 14_655 ?
F2 F2 F2 90.00(16) 3_656 15_565 ?
F2 F2 N1 65.83(19) 3_656 1_555 ?
F2 F2 N1 59.20(18) 3_656 3_656 ?
F2 F2 N2 76.25(15) 3_656 6_645 ?
F2 F2 C1 88.9(3) 3_656 1_555 ?
F2 F2 C1 77.0(2) 3_656 8_546 ?
F2 F2 F2 90.00(17) 10_566 14_655 ?
F2 F2 F2 106.07(18) 10_566 15_565 ?
F2 F2 N1 87.9(2) 10_566 1_555 ?
F2 F2 N1 162.2(3) 10_566 3_656 ?
F2 F2 N2 116.1(3) 10_566 6_645 ?
F2 F2 C1 66.7(2) 10_566 1_555 ?
F2 F2 C1 63.4(2) 10_566 8_546 ?
F2 F2 F2 90.00(16) 14_655 15_565 ?
F2 F2 N1 148.2(3) 14_655 1_555 ?
F2 F2 N1 77.2(2) 14_655 3_656 ?
F2 F2 N2 66.5(2) 14_655 6_645 ?
F2 F2 C1 133.2(3) 14_655 1_555 ?
F2 F2 C1 131.8(3) 14_655 8_546 ?
F2 F2 N1 60.32(19) 15_565 1_555 ?
F2 F2 N1 62.21(17) 15_565 3_656 ?
F2 F2 N2 130.7(2) 15_565 6_645 ?
F2 F2 C1 61.4(2) 15_565 1_555 ?
F2 F2 C1 134.2(2) 15_565 8_546 ?
N1 F2 N1 96.5(3) 1_555 3_656 ?
N1 F2 N2 141.0(3) 1_555 6_645 ?
N1 F2 C1 74.41(17) 1_555 8_546 ?
N1 F2 N2 70.28(16) 3_656 6_645 ?
N1 F2 C1 113.6(4) 3_656 1_555 ?
N1 F2 C1 134.5(3) 3_656 8_546 ?
N2 F2 C1 160.0(4) 6_645 1_555 ?
N2 F2 C1 89.0(3) 6_645 8_546 ?
C1 F2 C1 74.46(20) 1_555 8_546 ?
Co1 N1 Co1 105.70(18) 1_555 2_566 ?
Co1 N1 N1 134.9(6) 1_555 4_765 ?
Co1 N1 N2 153.0(5) 1_555 1_555 ?
Co1 N1 C1 114.9(7) 1_555 1_555 ?
Co1 N1 C1 169.0(5) 1_555 4_765 ?
Co1 N1 F2 130.84(18) 2_566 1_555 ?
Co1 N1 F2 77.07(16) 2_566 3_656 ?
Co1 N1 F2 77.07(16) 2_566 13_666 ?
Co1 N1 F2 130.84(18) 2_566 15_565 ?
Co1 N1 N2 101.3(4) 2_566 1_555 ?
Co1 N1 C1 139.4(7) 2_566 1_555 ?
Co1 N1 C1 63.3(4) 2_566 4_765 ?
F2 N1 F2 54.97(17) 1_555 3_656 ?
F2 N1 F2 83.55(19) 1_555 13_666 ?
F2 N1 F2 59.36(18) 1_555 15_565 ?
F2 N1 N1 148.2(6) 1_555 4_765 ?
F2 N1 N2 115.7(4) 1_555 1_555 ?
F2 N1 C1 82.9(6) 1_555 1_555 ?
F2 N1 C1 143.6(5) 1_555 4_765 ?
F2 N1 F2 55.58(16) 3_656 13_666 ?
F2 N1 F2 83.55(19) 3_656 15_565 ?
F2 N1 N1 102.8(5) 3_656 4_765 ?
F2 N1 N2 152.0(5) 3_656 1_555 ?
F2 N1 C1 136.6(7) 3_656 1_555 ?
F2 N1 C1 131.6(5) 3_656 4_765 ?
F2 N1 F2 54.97(17) 13_666 15_565 ?
F2 N1 N1 102.8(5) 13_666 4_765 ?
F2 N1 N2 152.0(5) 13_666 1_555 ?
F2 N1 C1 136.6(7) 13_666 1_555 ?
F2 N1 C1 131.6(5) 13_666 4_765 ?
F2 N1 N1 148.2(6) 15_565 4_765 ?
F2 N1 N2 115.7(4) 15_565 1_555 ?
F2 N1 C1 82.9(6) 15_565 1_555 ?
F2 N1 C1 143.6(5) 15_565 4_765 ?
N1 N1 N2 72.1(7) 4_765 1_555 ?
N1 N1 C1 110.2(10) 4_765 1_555 ?
C1 N1 C1 76.1(8) 1_555 4_765 ?
F1 N2 F2 49.8(3) 2_565 6_654 ?
F1 N2 F2 49.8(3) 2_565 7_564 ?
F1 N2 F2 49.8(3) 2_565 9_554 ?
F1 N2 F2 49.8(3) 2_565 12_664 ?
F1 N2 N1 162.1(5) 2_565 1_555 ?
F1 N2 N1 162.1(5) 2_565 4_765 ?
F1 N2 C1 127.8(8) 2_565 1_555 ?
F1 N2 C1 127.8(8) 2_565 4_765 ?
F2 N2 F2 99.59(19) 6_654 7_564 ?
F2 N2 F2 46.90(17) 6_654 9_554 ?
F2 N2 F2 81.36(19) 6_654 12_664 ?
F2 N2 N1 119.4(4) 6_654 1_555 ?
F2 N2 N1 137.5(4) 6_654 4_765 ?
F2 N2 C1 94.7(6) 6_654 1_555 ?
F2 N2 C1 135.3(6) 6_654 4_765 ?
F2 N2 F2 81.36(19) 7_564 9_554 ?
F2 N2 F2 46.90(17) 7_564 12_664 ?
F2 N2 N1 137.5(4) 7_564 1_555 ?
F2 N2 N1 119.4(4) 7_564 4_765 ?
F2 N2 C1 135.3(6) 7_564 1_555 ?
F2 N2 C1 94.7(6) 7_564 4_765 ?
F2 N2 F2 99.59(19) 9_554 12_664 ?
F2 N2 N1 137.5(4) 9_554 1_555 ?
F2 N2 N1 119.4(4) 9_554 4_765 ?
F2 N2 C1 135.3(6) 9_554 1_555 ?
F2 N2 C1 94.7(6) 9_554 4_765 ?
F2 N2 N1 119.4(4) 12_664 1_555 ?
F2 N2 N1 137.5(4) 12_664 4_765 ?
F2 N2 C1 94.7(6) 12_664 1_555 ?
F2 N2 C1 135.3(6) 12_664 4_765 ?
N1 N2 C1 70.1(7) 1_555 4_765 ?
N1 N2 C1 70.1(7) 4_765 1_555 ?
C1 N2 C1 104.3(10) 1_555 4_765 ?
Co1 C1 F1 71.3(2) 1_555 1_555 ?
Co1 C1 F2 88.9(2) 1_555 8_556 ?
Co1 C1 F2 88.9(2) 1_555 10_566 ?
Co1 C1 N1 79.2(4) 1_555 4_765 ?
Co1 C1 N2 151.1(7) 1_555 1_555 ?
Co1 C1 C1 113.2(5) 1_555 4_765 ?
F1 C1 F2 50.3(2) 1_555 1_555 ?
F1 C1 F2 46.77(18) 1_555 8_556 ?
F1 C1 F2 46.77(18) 1_555 10_566 ?
F1 C1 F2 50.3(2) 1_555 15_565 ?
F1 C1 N1 114.7(6) 1_555 1_555 ?
F1 C1 N1 150.5(4) 1_555 4_765 ?
F1 C1 N2 137.6(5) 1_555 1_555 ?
F1 C1 C1 175.4(5) 1_555 4_765 ?
F2 C1 F2 91.4(2) 1_555 8_556 ?
F2 C1 F2 49.96(20) 1_555 10_566 ?
F2 C1 F2 57.2(2) 1_555 15_565 ?
F2 C1 N1 73.7(6) 1_555 1_555 ?
F2 C1 N1 105.0(4) 1_555 4_765 ?
F2 C1 N2 151.36(9) 1_555 1_555 ?
F2 C1 C1 133.2(5) 1_555 4_765 ?
F2 C1 F2 88.38(20) 8_556 10_566 ?
F2 C1 F2 49.96(20) 8_556 15_565 ?
F2 C1 N1 118.6(6) 8_556 1_555 ?
F2 C1 N1 134.5(4) 8_556 4_765 ?
F2 C1 N2 111.3(5) 8_556 1_555 ?
F2 C1 C1 131.8(5) 8_556 4_765 ?
F2 C1 F2 91.4(2) 10_566 15_565 ?
F2 C1 N1 118.6(6) 10_566 1_555 ?
F2 C1 N1 134.5(4) 10_566 4_765 ?
F2 C1 N2 111.3(5) 10_566 1_555 ?
F2 C1 C1 131.8(5) 10_566 4_765 ?
F2 C1 N1 73.7(6) 15_565 1_555 ?
F2 C1 N1 105.0(4) 15_565 4_765 ?
F2 C1 N2 151.4(6) 15_565 1_555 ?
F2 C1 C1 133.2(5) 15_565 4_765 ?
N1 C1 N2 107.7(10) 1_555 1_555 ?
N1 C1 C1 69.8(7) 1_555 4_765 ?
N1 C1 N2 71.9(7) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_CoFeF5Htaz
_database_code_depnum_ccdc_archive 'CCDC 1527799'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 Co0.93 F5 Fe1.07 N3'
_chemical_formula_weight         275.61
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.349 0.972 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.346 0.844 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.0882(5)
_cell_length_b                   7.4479(4)
_cell_length_c                   9.4689(5)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     640.93(6)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5582
_pd_meas_2theta_range_min        5.11700
_pd_meas_2theta_range_max        99.99400
_pd_meas_2theta_range_inc        0.017001

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.5718
_pd_proc_ls_prof_wR_factor       0.7308
_pd_proc_ls_prof_wR_expected     0.7326

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       27.1042
_pd_proc_ls_prof_cwR_factor      10.4083
_pd_proc_ls_prof_cwR_expected    10.4341

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            0.9951
_pd_proc_ls_prof_echi2           1.0298
_refine_ls_goodness_of_fit_all   0.9975

#  Items related to LS refinement

_refine_ls_R_I_factor            6.3982
_refine_ls_number_reflns         415
_refine_ls_number_parameters     56
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        5.0520
_pd_proc_2theta_range_max        99.9290
_pd_proc_2theta_range_inc        0.017001
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Co1 0.75000 0.75000 0.75000 0.0290(13) 0.93000 Uiso Co
Fe1 0.75000 0.75000 0.75000 0.0290(13) 0.07000 Uiso Fe
Fe2 0.50000 0.50000 0.50000 0.0217(14) 1.00000 Uiso Fe
F1 0.50000 0.75000 0.4246(7) 0.0256(16) 1.00000 Uiso F
F2 0.6487(4) 0.5567(5) 0.6355(3) 0.0256(16) 1.00000 Uiso F
N1 0.9240(8) 0.75000 0.5838(8) 0.025(3) 1.00000 Uiso N
N2 1.00000 0.75000 0.3676(11) 0.025(3) 1.00000 Uiso N
C1 0.8791(10) 0.75000 0.4510(11) 0.025(3) 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Co1 F2 2.024(3) 1_555 ?
Co1 F2 2.024(3) 3_656 ?
Co1 F2 2.024(3) 13_666 ?
Co1 F2 2.024(3) 15_565 ?
Co1 N1 2.231(7) 1_555 ?
Co1 N1 3.355(7) 2_466 ?
Co1 N1 2.231(7) 3_656 ?
Co1 N1 3.355(7) 4_765 ?
Co1 C1 3.065(10) 1_555 ?
Co1 C1 3.065(10) 3_656 ?
Fe1 F2 2.024(3) 1_555 ?
Fe1 F2 2.024(3) 3_656 ?
Fe1 F2 2.024(3) 13_666 ?
Fe1 F2 2.024(3) 15_565 ?
Fe1 N1 2.231(7) 1_555 ?
Fe1 N1 3.355(7) 2_466 ?
Fe1 N1 2.231(7) 3_656 ?
Fe1 N1 3.355(7) 4_765 ?
Fe1 C1 3.065(10) 1_555 ?
Fe1 C1 3.065(10) 3_656 ?
Fe2 F1 1.994(2) 1_555 ?
Fe2 F1 1.994(2) 5_666 ?
Fe2 F2 1.911(3) 1_555 ?
Fe2 F2 1.911(3) 5_666 ?
Fe2 F2 1.911(3) 10_566 ?
Fe2 F2 1.911(3) 14_655 ?
F1 Fe2 1.994(2) 1_555 ?
F1 Fe2 1.994(2) 4_665 ?
F1 F2 2.808(6) 1_555 ?
F1 F2 2.808(6) 4_665 ?
F1 F2 2.714(4) 5_666 ?
F1 F2 2.714(4) 8_556 ?
F1 F2 2.714(4) 10_566 ?
F1 F2 2.714(4) 11_656 ?
F1 F2 2.808(6) 14_655 ?
F1 F2 2.808(6) 15_565 ?
F1 N2 2.767(12) 2_465 ?
F1 C1 3.454(9) 1_555 ?
F1 C1 3.454(9) 4_665 ?
F2 Co1 2.024(3) 1_555 ?
F2 Fe1 2.024(3) 1_555 ?
F2 Fe2 1.911(3) 1_555 ?
F2 F1 2.808(6) 1_555 ?
F2 F1 2.714(4) 5_666 ?
F2 F2 2.845(5) 3_656 ?
F2 F2 2.701(4) 10_566 ?
F2 F2 2.703(5) 14_655 ?
F2 F2 2.879(5) 15_565 ?
F2 N1 2.928(7) 1_555 ?
F2 N1 3.094(7) 3_656 ?
F2 N2 3.446(7) 6_645 ?
F2 C1 3.084(9) 1_555 ?
F2 C1 3.205(7) 8_546 ?
N1 Co1 2.231(7) 1_555 ?
N1 Co1 3.355(7) 2_566 ?
N1 Fe1 2.231(7) 1_555 ?
N1 Fe1 3.355(7) 2_566 ?
N1 F2 2.928(7) 1_555 ?
N1 F2 3.094(7) 3_656 ?
N1 F2 3.094(7) 13_666 ?
N1 F2 2.928(7) 15_565 ?
N1 N1 1.381(10) 4_765 ?
N1 N2 2.161(12) 1_555 ?
N1 C1 1.322(13) 1_555 ?
N1 C1 2.187(12) 4_765 ?
N2 F1 2.767(12) 2_565 ?
N2 F2 3.446(7) 6_654 ?
N2 F2 3.446(7) 7_564 ?
N2 F2 3.446(7) 9_554 ?
N2 F2 3.446(7) 12_664 ?
N2 N1 2.161(12) 1_555 ?
N2 N1 2.161(12) 4_765 ?
N2 C1 1.353(11) 1_555 ?
N2 C1 1.353(11) 4_765 ?
C1 Co1 3.065(10) 1_555 ?
C1 Fe1 3.065(10) 1_555 ?
C1 F1 3.454(9) 1_555 ?
C1 F2 3.084(9) 1_555 ?
C1 F2 3.205(7) 8_556 ?
C1 F2 3.205(7) 10_566 ?
C1 F2 3.084(9) 15_565 ?
C1 N1 1.322(13) 1_555 ?
C1 N1 2.187(12) 4_765 ?
C1 N2 1.353(11) 1_555 ?
C1 C1 2.198(13) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Co1 F2 89.3(2) 1_555 3_656 ?
F2 Co1 F2 180.0(3) 1_555 13_666 ?
F2 Co1 F2 90.7(3) 1_555 15_565 ?
F2 Co1 N1 86.8(3) 1_555 1_555 ?
F2 Co1 N1 81.3(3) 1_555 2_466 ?
F2 Co1 N1 93.2(4) 1_555 3_656 ?
F2 Co1 N1 98.7(3) 1_555 4_765 ?
F2 Co1 C1 71.3(3) 1_555 1_555 ?
F2 Co1 C1 108.7(4) 1_555 3_656 ?
F2 Co1 F2 90.7(3) 3_656 13_666 ?
F2 Co1 F2 180.0(3) 3_656 15_565 ?
F2 Co1 N1 93.2(4) 3_656 1_555 ?
F2 Co1 N1 98.7(3) 3_656 2_466 ?
F2 Co1 N1 86.8(3) 3_656 3_656 ?
F2 Co1 N1 81.3(3) 3_656 4_765 ?
F2 Co1 C1 108.7(4) 3_656 1_555 ?
F2 Co1 C1 71.3(3) 3_656 3_656 ?
F2 Co1 F2 89.3(2) 13_666 15_565 ?
F2 Co1 N1 93.2(4) 13_666 1_555 ?
F2 Co1 N1 98.7(3) 13_666 2_466 ?
F2 Co1 N1 86.8(3) 13_666 3_656 ?
F2 Co1 N1 81.3(3) 13_666 4_765 ?
F2 Co1 C1 108.7(4) 13_666 1_555 ?
F2 Co1 C1 71.3(3) 13_666 3_656 ?
F2 Co1 N1 86.8(3) 15_565 1_555 ?
F2 Co1 N1 81.3(3) 15_565 2_466 ?
F2 Co1 N1 93.2(4) 15_565 3_656 ?
F2 Co1 N1 98.7(3) 15_565 4_765 ?
F2 Co1 C1 71.3(3) 15_565 1_555 ?
F2 Co1 C1 108.7(4) 15_565 3_656 ?
N1 Co1 N1 163.1(5) 1_555 2_466 ?
N1 Co1 N1 180.0(6) 1_555 3_656 ?
N1 Co1 C1 157.4(6) 1_555 3_656 ?
N1 Co1 N1 180.0(4) 2_466 4_765 ?
N1 Co1 C1 140.5(5) 2_466 1_555 ?
N1 Co1 N1 163.1(5) 3_656 4_765 ?
N1 Co1 C1 157.4(6) 3_656 1_555 ?
N1 Co1 C1 140.5(5) 4_765 3_656 ?
C1 Co1 C1 180.0(6) 1_555 3_656 ?
F2 Fe1 F2 89.3(2) 1_555 3_656 ?
F2 Fe1 F2 180.0(3) 1_555 13_666 ?
F2 Fe1 F2 90.7(3) 1_555 15_565 ?
F2 Fe1 N1 86.8(3) 1_555 1_555 ?
F2 Fe1 N1 81.3(3) 1_555 2_466 ?
F2 Fe1 N1 93.2(4) 1_555 3_656 ?
F2 Fe1 N1 98.7(3) 1_555 4_765 ?
F2 Fe1 C1 71.3(3) 1_555 1_555 ?
F2 Fe1 C1 108.7(4) 1_555 3_656 ?
F2 Fe1 F2 90.7(3) 3_656 13_666 ?
F2 Fe1 F2 180.0(3) 3_656 15_565 ?
F2 Fe1 N1 93.2(4) 3_656 1_555 ?
F2 Fe1 N1 98.7(3) 3_656 2_466 ?
F2 Fe1 N1 86.8(3) 3_656 3_656 ?
F2 Fe1 N1 81.3(3) 3_656 4_765 ?
F2 Fe1 C1 108.7(4) 3_656 1_555 ?
F2 Fe1 C1 71.3(3) 3_656 3_656 ?
F2 Fe1 F2 89.3(2) 13_666 15_565 ?
F2 Fe1 N1 93.2(4) 13_666 1_555 ?
F2 Fe1 N1 98.7(3) 13_666 2_466 ?
F2 Fe1 N1 86.8(3) 13_666 3_656 ?
F2 Fe1 N1 81.3(3) 13_666 4_765 ?
F2 Fe1 C1 108.7(4) 13_666 1_555 ?
F2 Fe1 C1 71.3(3) 13_666 3_656 ?
F2 Fe1 N1 86.8(3) 15_565 1_555 ?
F2 Fe1 N1 81.3(3) 15_565 2_466 ?
F2 Fe1 N1 93.2(4) 15_565 3_656 ?
F2 Fe1 N1 98.7(3) 15_565 4_765 ?
F2 Fe1 C1 71.3(3) 15_565 1_555 ?
F2 Fe1 C1 108.7(4) 15_565 3_656 ?
N1 Fe1 N1 163.1(5) 1_555 2_466 ?
N1 Fe1 N1 180.0(6) 1_555 3_656 ?
N1 Fe1 C1 157.4(6) 1_555 3_656 ?
N1 Fe1 N1 180.0(4) 2_466 4_765 ?
N1 Fe1 C1 140.5(5) 2_466 1_555 ?
N1 Fe1 N1 163.1(5) 3_656 4_765 ?
N1 Fe1 C1 157.4(6) 3_656 1_555 ?
N1 Fe1 C1 140.5(5) 4_765 3_656 ?
C1 Fe1 C1 180.0(6) 1_555 3_656 ?
F1 Fe2 F1 180.0(2) 1_555 5_666 ?
F1 Fe2 F2 92.0(3) 1_555 1_555 ?
F1 Fe2 F2 88.0(2) 1_555 5_666 ?
F1 Fe2 F2 88.0(2) 1_555 10_566 ?
F1 Fe2 F2 92.0(3) 1_555 14_655 ?
F1 Fe2 F2 88.0(2) 5_666 1_555 ?
F1 Fe2 F2 92.0(3) 5_666 5_666 ?
F1 Fe2 F2 92.0(3) 5_666 10_566 ?
F1 Fe2 F2 88.0(2) 5_666 14_655 ?
F2 Fe2 F2 180.0(3) 1_555 5_666 ?
F2 Fe2 F2 90.0(2) 1_555 10_566 ?
F2 Fe2 F2 90.0(3) 1_555 14_655 ?
F2 Fe2 F2 90.0(3) 5_666 10_566 ?
F2 Fe2 F2 90.0(2) 5_666 14_655 ?
F2 Fe2 F2 180.0(3) 10_566 14_655 ?
Fe2 F1 Fe2 138.04(10) 1_555 4_665 ?
Fe2 F1 F2 102.95(20) 1_555 4_665 ?
Fe2 F1 F2 149.4(2) 1_555 8_556 ?
Fe2 F1 F2 149.4(2) 1_555 11_656 ?
Fe2 F1 F2 102.95(20) 1_555 15_565 ?
Fe2 F1 N2 111.0(5) 1_555 2_465 ?
Fe2 F1 C1 88.52(8) 1_555 1_555 ?
Fe2 F1 C1 88.5(3) 1_555 4_665 ?
Fe2 F1 F2 102.95(20) 4_665 1_555 ?
Fe2 F1 F2 149.4(2) 4_665 5_666 ?
Fe2 F1 F2 149.4(2) 4_665 10_566 ?
Fe2 F1 F2 102.95(20) 4_665 14_655 ?
Fe2 F1 N2 111.0(5) 4_665 2_465 ?
Fe2 F1 C1 88.5(3) 4_665 1_555 ?
Fe2 F1 C1 88.52(8) 4_665 4_665 ?
F2 F1 F2 89.4(2) 1_555 4_665 ?
F2 F1 F2 87.55(20) 1_555 5_666 ?
F2 F1 F2 109.9(2) 1_555 8_556 ?
F2 F1 F2 58.54(17) 1_555 10_566 ?
F2 F1 F2 145.1(2) 1_555 11_656 ?
F2 F1 F2 57.53(19) 1_555 14_655 ?
F2 F1 F2 61.68(20) 1_555 15_565 ?
F2 F1 N2 135.3(5) 1_555 2_465 ?
F2 F1 C1 57.9(3) 1_555 1_555 ?
F2 F1 C1 115.4(4) 1_555 4_665 ?
F2 F1 F2 109.9(2) 4_665 5_666 ?
F2 F1 F2 87.55(20) 4_665 8_556 ?
F2 F1 F2 145.1(2) 4_665 10_566 ?
F2 F1 F2 58.54(17) 4_665 11_656 ?
F2 F1 F2 61.68(20) 4_665 14_655 ?
F2 F1 F2 57.53(19) 4_665 15_565 ?
F2 F1 N2 135.3(5) 4_665 2_465 ?
F2 F1 C1 115.4(4) 4_665 1_555 ?
F2 F1 C1 57.9(3) 4_665 4_665 ?
F2 F1 F2 155.8(2) 5_666 8_556 ?
F2 F1 F2 59.72(16) 5_666 10_566 ?
F2 F1 F2 114.6(2) 5_666 11_656 ?
F2 F1 F2 58.54(17) 5_666 14_655 ?
F2 F1 F2 145.1(2) 5_666 15_565 ?
F2 F1 N2 77.9(3) 5_666 2_465 ?
F2 F1 C1 120.8(3) 5_666 1_555 ?
F2 F1 C1 61.2(2) 5_666 4_665 ?
F2 F1 F2 114.6(2) 8_556 10_566 ?
F2 F1 F2 59.72(16) 8_556 11_656 ?
F2 F1 F2 145.1(2) 8_556 14_655 ?
F2 F1 F2 58.54(17) 8_556 15_565 ?
F2 F1 N2 77.9(3) 8_556 2_465 ?
F2 F1 C1 61.2(2) 8_556 1_555 ?
F2 F1 C1 120.8(3) 8_556 4_665 ?
F2 F1 F2 155.8(2) 10_566 11_656 ?
F2 F1 F2 87.55(20) 10_566 14_655 ?
F2 F1 F2 109.9(2) 10_566 15_565 ?
F2 F1 N2 77.9(3) 10_566 2_465 ?
F2 F1 C1 61.2(2) 10_566 1_555 ?
F2 F1 C1 120.8(3) 10_566 4_665 ?
F2 F1 F2 109.9(2) 11_656 14_655 ?
F2 F1 F2 87.55(20) 11_656 15_565 ?
F2 F1 N2 77.9(3) 11_656 2_465 ?
F2 F1 C1 120.8(3) 11_656 1_555 ?
F2 F1 C1 61.2(2) 11_656 4_665 ?
F2 F1 F2 89.4(2) 14_655 15_565 ?
F2 F1 N2 135.3(5) 14_655 2_465 ?
F2 F1 C1 115.4(4) 14_655 1_555 ?
F2 F1 C1 57.9(3) 14_655 4_665 ?
F2 F1 N2 135.3(5) 15_565 2_465 ?
F2 F1 C1 57.9(3) 15_565 1_555 ?
F2 F1 C1 115.4(4) 15_565 4_665 ?
N2 F1 C1 94.1(4) 2_465 1_555 ?
N2 F1 C1 94.1(4) 2_465 4_665 ?
C1 F1 C1 171.7(5) 1_555 4_665 ?
Co1 F2 Fe2 147.00(14) 1_555 1_555 ?
Co1 F2 F1 103.6(3) 1_555 1_555 ?
Co1 F2 F1 159.63(17) 1_555 5_666 ?
Co1 F2 F2 45.35(15) 1_555 3_656 ?
Co1 F2 F2 136.99(20) 1_555 10_566 ?
Co1 F2 F2 117.1(2) 1_555 14_655 ?
Co1 F2 N1 49.5(2) 1_555 1_555 ?
Co1 F2 N1 46.0(2) 1_555 3_656 ?
Co1 F2 N2 107.96(18) 1_555 6_645 ?
Co1 F2 C1 70.3(3) 1_555 1_555 ?
Co1 F2 C1 110.3(3) 1_555 8_546 ?
Fe1 F2 Fe2 147.00(14) 1_555 1_555 ?
Fe1 F2 F1 103.6(3) 1_555 1_555 ?
Fe1 F2 F1 159.63(17) 1_555 5_666 ?
Fe1 F2 F2 45.35(15) 1_555 3_656 ?
Fe1 F2 F2 136.99(20) 1_555 10_566 ?
Fe1 F2 F2 117.1(2) 1_555 14_655 ?
Fe1 F2 N1 49.5(2) 1_555 1_555 ?
Fe1 F2 N1 46.0(2) 1_555 3_656 ?
Fe1 F2 N2 107.96(18) 1_555 6_645 ?
Fe1 F2 C1 70.3(3) 1_555 1_555 ?
Fe1 F2 C1 110.3(3) 1_555 8_546 ?
Fe2 F2 F1 45.21(16) 1_555 1_555 ?
Fe2 F2 F1 47.24(14) 1_555 5_666 ?
Fe2 F2 F2 165.8(2) 1_555 3_656 ?
Fe2 F2 F2 45.01(15) 1_555 10_566 ?
Fe2 F2 F2 102.8(2) 1_555 15_565 ?
Fe2 F2 N1 126.9(3) 1_555 1_555 ?
Fe2 F2 N1 121.9(3) 1_555 3_656 ?
Fe2 F2 N2 90.3(4) 1_555 6_645 ?
Fe2 F2 C1 101.7(4) 1_555 1_555 ?
Fe2 F2 C1 97.6(3) 1_555 8_546 ?
F1 F2 F1 92.45(18) 1_555 5_666 ?
F1 F2 F2 148.6(3) 1_555 3_656 ?
F1 F2 F2 58.99(17) 1_555 10_566 ?
F1 F2 F2 61.2(2) 1_555 14_655 ?
F1 F2 F2 59.16(19) 1_555 15_565 ?
F1 F2 N1 92.3(3) 1_555 1_555 ?
F1 F2 N1 105.6(4) 1_555 3_656 ?
F1 F2 N2 127.2(4) 1_555 6_645 ?
F1 F2 C1 71.6(3) 1_555 1_555 ?
F1 F2 C1 119.9(3) 1_555 8_546 ?
F1 F2 F2 118.8(2) 5_666 3_656 ?
F1 F2 F2 62.47(17) 5_666 10_566 ?
F1 F2 F2 60.14(16) 5_666 14_655 ?
F1 F2 F2 147.3(2) 5_666 15_565 ?
F1 F2 N1 143.5(3) 5_666 1_555 ?
F1 F2 N1 117.7(3) 5_666 3_656 ?
F1 F2 N2 51.7(3) 5_666 6_645 ?
F1 F2 C1 127.7(3) 5_666 1_555 ?
F1 F2 C1 70.8(3) 5_666 8_546 ?
F2 F2 F2 136.4(2) 3_656 10_566 ?
F2 F2 F2 130.3(2) 3_656 14_655 ?
F2 F2 F2 90.00(20) 3_656 15_565 ?
F2 F2 N1 64.8(2) 3_656 1_555 ?
F2 F2 N1 58.9(2) 3_656 3_656 ?
F2 F2 N2 76.57(18) 3_656 6_645 ?
F2 F2 C1 89.6(3) 3_656 1_555 ?
F2 F2 C1 76.8(3) 3_656 8_546 ?
F2 F2 F2 90.00(20) 10_566 14_655 ?
F2 F2 F2 108.2(2) 10_566 15_565 ?
F2 F2 N1 89.7(3) 10_566 1_555 ?
F2 F2 N1 164.0(3) 10_566 3_656 ?
F2 F2 N2 113.5(4) 10_566 6_645 ?
F2 F2 C1 66.9(3) 10_566 1_555 ?
F2 F2 C1 62.3(2) 10_566 8_546 ?
F2 F2 F2 90.0(2) 14_655 15_565 ?
F2 F2 N1 148.7(4) 14_655 1_555 ?
F2 F2 N1 77.7(3) 14_655 3_656 ?
F2 F2 N2 66.9(2) 14_655 6_645 ?
F2 F2 C1 132.8(4) 14_655 1_555 ?
F2 F2 C1 130.8(4) 14_655 8_546 ?
F2 F2 N1 60.5(2) 15_565 1_555 ?
F2 F2 N1 62.3(2) 15_565 3_656 ?
F2 F2 N2 131.5(2) 15_565 6_645 ?
F2 F2 C1 62.2(3) 15_565 1_555 ?
F2 F2 C1 135.5(2) 15_565 8_546 ?
N1 F2 N1 95.6(4) 1_555 3_656 ?
N1 F2 N2 140.2(3) 1_555 6_645 ?
N1 F2 C1 75.49(20) 1_555 8_546 ?
N1 F2 N2 71.15(19) 3_656 6_645 ?
N1 F2 C1 114.5(4) 3_656 1_555 ?
N1 F2 C1 133.7(4) 3_656 8_546 ?
N2 F2 C1 159.6(4) 6_645 1_555 ?
N2 F2 C1 86.9(3) 6_645 8_546 ?
C1 F2 C1 75.2(2) 1_555 8_546 ?
Co1 N1 Co1 107.2(2) 1_555 2_566 ?
Co1 N1 Fe1 107.2(2) 1_555 2_566 ?
Co1 N1 N1 135.1(7) 1_555 4_765 ?
Co1 N1 N2 153.5(6) 1_555 1_555 ?
Co1 N1 C1 116.9(8) 1_555 1_555 ?
Co1 N1 C1 170.2(6) 1_555 4_765 ?
Co1 N1 Fe1 107.2(2) 2_566 1_555 ?
Co1 N1 F2 132.6(2) 2_566 1_555 ?
Co1 N1 F2 77.6(2) 2_566 3_656 ?
Co1 N1 F2 77.6(2) 2_566 13_666 ?
Co1 N1 F2 132.6(2) 2_566 15_565 ?
Co1 N1 N2 99.3(5) 2_566 1_555 ?
Co1 N1 C1 136.0(8) 2_566 1_555 ?
Co1 N1 C1 63.1(4) 2_566 4_765 ?
Fe1 N1 Fe1 107.2(2) 1_555 2_566 ?
Fe1 N1 N1 135.1(7) 1_555 4_765 ?
Fe1 N1 N2 153.5(6) 1_555 1_555 ?
Fe1 N1 C1 116.9(8) 1_555 1_555 ?
Fe1 N1 C1 170.2(6) 1_555 4_765 ?
Fe1 N1 F2 132.6(2) 2_566 1_555 ?
Fe1 N1 F2 77.6(2) 2_566 3_656 ?
Fe1 N1 F2 77.6(2) 2_566 13_666 ?
Fe1 N1 F2 132.6(2) 2_566 15_565 ?
Fe1 N1 N2 99.3(5) 2_566 1_555 ?
Fe1 N1 C1 136.0(8) 2_566 1_555 ?
Fe1 N1 C1 63.1(4) 2_566 4_765 ?
F2 N1 F2 56.3(2) 1_555 3_656 ?
F2 N1 F2 84.4(2) 1_555 13_666 ?
F2 N1 F2 58.9(2) 1_555 15_565 ?
F2 N1 N1 148.7(6) 1_555 4_765 ?
F2 N1 N2 115.6(5) 1_555 1_555 ?
F2 N1 C1 84.0(7) 1_555 1_555 ?
F2 N1 C1 142.7(5) 1_555 4_765 ?
F2 N1 F2 55.5(2) 3_656 13_666 ?
F2 N1 F2 84.4(2) 3_656 15_565 ?
F2 N1 N1 102.3(6) 3_656 4_765 ?
F2 N1 N2 151.9(6) 3_656 1_555 ?
F2 N1 C1 138.7(8) 3_656 1_555 ?
F2 N1 C1 132.0(5) 3_656 4_765 ?
F2 N1 F2 56.3(2) 13_666 15_565 ?
F2 N1 N1 102.3(6) 13_666 4_765 ?
F2 N1 N2 151.9(6) 13_666 1_555 ?
F2 N1 C1 138.7(8) 13_666 1_555 ?
F2 N1 C1 132.0(5) 13_666 4_765 ?
F2 N1 N1 148.7(6) 15_565 4_765 ?
F2 N1 N2 115.6(5) 15_565 1_555 ?
F2 N1 C1 84.0(7) 15_565 1_555 ?
F2 N1 C1 142.7(5) 15_565 4_765 ?
N1 N1 N2 71.4(7) 4_765 1_555 ?
N1 N1 C1 108.0(11) 4_765 1_555 ?
C1 N1 C1 72.9(8) 1_555 4_765 ?
F1 N2 F2 50.4(3) 2_565 6_654 ?
F1 N2 F2 50.4(3) 2_565 7_564 ?
F1 N2 F2 50.4(3) 2_565 9_554 ?
F1 N2 F2 50.4(3) 2_565 12_664 ?
F1 N2 N1 161.4(6) 2_565 1_555 ?
F1 N2 N1 161.4(6) 2_565 4_765 ?
F1 N2 C1 125.7(9) 2_565 1_555 ?
F1 N2 C1 125.7(9) 2_565 4_765 ?
F2 N2 F2 100.7(2) 6_654 7_564 ?
F2 N2 F2 46.18(19) 6_654 9_554 ?
F2 N2 F2 83.0(2) 6_654 12_664 ?
F2 N2 N1 118.6(4) 6_654 1_555 ?
F2 N2 N1 136.9(5) 6_654 4_765 ?
F2 N2 C1 93.1(6) 6_654 1_555 ?
F2 N2 C1 133.7(7) 6_654 4_765 ?
F2 N2 F2 83.0(2) 7_564 9_554 ?
F2 N2 F2 46.18(19) 7_564 12_664 ?
F2 N2 N1 136.9(5) 7_564 1_555 ?
F2 N2 N1 118.6(4) 7_564 4_765 ?
F2 N2 C1 133.7(7) 7_564 1_555 ?
F2 N2 C1 93.1(6) 7_564 4_765 ?
F2 N2 F2 100.7(2) 9_554 12_664 ?
F2 N2 N1 136.9(5) 9_554 1_555 ?
F2 N2 N1 118.6(4) 9_554 4_765 ?
F2 N2 C1 133.7(7) 9_554 1_555 ?
F2 N2 C1 93.1(6) 9_554 4_765 ?
F2 N2 N1 118.6(4) 12_664 1_555 ?
F2 N2 N1 136.9(5) 12_664 4_765 ?
F2 N2 C1 93.1(6) 12_664 1_555 ?
F2 N2 C1 133.7(7) 12_664 4_765 ?
N1 N2 C1 72.9(8) 1_555 4_765 ?
N1 N2 C1 72.9(8) 4_765 1_555 ?
C1 N2 C1 108.6(11) 1_555 4_765 ?
Co1 C1 F1 71.6(3) 1_555 1_555 ?
Co1 C1 F2 89.2(2) 1_555 8_556 ?
Co1 C1 F2 89.2(2) 1_555 10_566 ?
Co1 C1 N1 77.4(4) 1_555 4_765 ?
Co1 C1 N2 148.2(7) 1_555 1_555 ?
Co1 C1 C1 112.5(5) 1_555 4_765 ?
Fe1 C1 F1 71.6(3) 1_555 1_555 ?
Fe1 C1 F2 89.2(2) 1_555 8_556 ?
Fe1 C1 F2 89.2(2) 1_555 10_566 ?
Fe1 C1 N1 77.4(4) 1_555 4_765 ?
Fe1 C1 N2 148.2(7) 1_555 1_555 ?
Fe1 C1 C1 112.5(5) 1_555 4_765 ?
F1 C1 F2 50.5(2) 1_555 1_555 ?
F1 C1 F2 47.9(2) 1_555 8_556 ?
F1 C1 F2 47.9(2) 1_555 10_566 ?
F1 C1 F2 50.5(2) 1_555 15_565 ?
F1 C1 N1 112.1(7) 1_555 1_555 ?
F1 C1 N1 149.1(5) 1_555 4_765 ?
F1 C1 N2 140.1(5) 1_555 1_555 ?
F1 C1 C1 175.8(5) 1_555 4_765 ?
F2 C1 F2 91.9(3) 1_555 8_556 ?
F2 C1 F2 50.8(2) 1_555 10_566 ?
F2 C1 F2 55.7(3) 1_555 15_565 ?
F2 C1 N1 70.8(7) 1_555 1_555 ?
F2 C1 N1 103.3(5) 1_555 4_765 ?
F2 C1 N2 151.89(14) 1_555 1_555 ?
F2 C1 C1 132.8(5) 1_555 4_765 ?
F2 C1 F2 90.9(2) 8_556 10_566 ?
F2 C1 F2 50.8(2) 8_556 15_565 ?
F2 C1 N1 116.4(7) 8_556 1_555 ?
F2 C1 N1 133.0(5) 8_556 4_765 ?
F2 C1 N2 112.4(5) 8_556 1_555 ?
F2 C1 C1 130.8(5) 8_556 4_765 ?
F2 C1 F2 91.9(3) 10_566 15_565 ?
F2 C1 N1 116.4(7) 10_566 1_555 ?
F2 C1 N1 133.0(5) 10_566 4_765 ?
F2 C1 N2 112.4(5) 10_566 1_555 ?
F2 C1 C1 130.8(5) 10_566 4_765 ?
F2 C1 N1 70.8(7) 15_565 1_555 ?
F2 C1 N1 103.3(5) 15_565 4_765 ?
F2 C1 N2 151.9(7) 15_565 1_555 ?
F2 C1 C1 132.8(5) 15_565 4_765 ?
N1 C1 N2 107.7(11) 1_555 1_555 ?
N1 C1 C1 72.0(8) 1_555 4_765 ?
N1 C1 N2 70.8(8) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_CoVF5Htaz
_database_code_depnum_ccdc_archive 'CCDC 1527754'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 Co F5 N3 V'
_chemical_formula_weight         270.92
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.349 0.972 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.301 0.529 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.0738(4)
_cell_length_b                   7.4627(3)
_cell_length_c                   9.4407(4)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     639.28(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5582
_pd_meas_2theta_range_min        5.11700
_pd_meas_2theta_range_max        99.99400
_pd_meas_2theta_range_inc        0.017001

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.7184
_pd_proc_ls_prof_wR_factor       0.9288
_pd_proc_ls_prof_wR_expected     0.8597

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       21.7689
_pd_proc_ls_prof_cwR_factor      9.6913
_pd_proc_ls_prof_cwR_expected    8.9708

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            1.1671
_pd_proc_ls_prof_echi2           1.2086
_refine_ls_goodness_of_fit_all   1.0803

#  Items related to LS refinement

_refine_ls_R_I_factor            5.6681
_refine_ls_number_reflns         416
_refine_ls_number_parameters     50
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        5.0862
_pd_proc_2theta_range_max        99.9632
_pd_proc_2theta_range_inc        0.017001
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Co1 0.75000 0.75000 0.75000 0.0123(10) 1.00000 Uiso Co
V1 0.50000 0.50000 0.50000 0.0053(13) 1.00000 Uiso V
F1 0.50000 0.75000 0.4231(6) 0.0108(13) 1.00000 Uiso F
F2 0.6480(3) 0.5557(4) 0.6356(3) 0.0108(13) 1.00000 Uiso F
N1 0.9248(6) 0.75000 0.5793(7) 0.01267 1.00000 Uiso N
N2 1.00000 0.75000 0.3658(9) 0.01267 1.00000 Uiso N
C1 0.8777(9) 0.75000 0.4515(8) 0.01267 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Co1 F2 2.031(3) 1_555 ?
Co1 F2 2.031(3) 3_656 ?
Co1 F2 2.031(3) 13_666 ?
Co1 F2 2.031(3) 15_565 ?
Co1 N1 2.261(6) 1_555 ?
Co1 N1 3.362(6) 2_466 ?
Co1 N1 2.261(6) 3_656 ?
Co1 N1 3.362(6) 4_765 ?
Co1 C1 3.047(8) 1_555 ?
Co1 C1 3.047(8) 3_656 ?
V1 F1 2.002(2) 1_555 ?
V1 F1 2.002(2) 5_666 ?
V1 F2 1.901(3) 1_555 ?
V1 F2 1.901(3) 5_666 ?
V1 F2 1.901(3) 10_566 ?
V1 F2 1.901(3) 14_655 ?
F1 V1 2.002(2) 1_555 ?
F1 V1 2.002(2) 4_665 ?
F1 F2 2.816(5) 1_555 ?
F1 F2 2.816(5) 4_665 ?
F1 F2 2.705(3) 5_666 ?
F1 F2 2.705(3) 8_556 ?
F1 F2 2.705(3) 10_566 ?
F1 F2 2.705(3) 11_656 ?
F1 F2 2.816(5) 14_655 ?
F1 F2 2.816(5) 15_565 ?
F1 N2 2.727(10) 2_465 ?
F1 C1 3.438(8) 1_555 ?
F1 C1 3.438(8) 4_665 ?
F2 Co1 2.031(3) 1_555 ?
F2 V1 1.901(3) 1_555 ?
F2 F1 2.816(5) 1_555 ?
F2 F1 2.705(3) 5_666 ?
F2 F2 2.845(4) 3_656 ?
F2 F2 2.692(4) 10_566 ?
F2 F2 2.686(4) 14_655 ?
F2 F2 2.900(4) 15_565 ?
F2 N1 2.948(6) 1_555 ?
F2 N1 3.128(6) 3_656 ?
F2 N2 3.425(6) 6_645 ?
F2 C1 3.077(8) 1_555 ?
F2 C1 3.198(6) 8_546 ?
N1 Co1 2.261(6) 1_555 ?
N1 Co1 3.362(6) 2_566 ?
N1 F2 2.948(6) 1_555 ?
N1 F2 3.128(6) 3_656 ?
N1 F2 3.128(6) 13_666 ?
N1 F2 2.948(6) 15_565 ?
N1 N1 1.365(8) 4_765 ?
N1 N2 2.128(10) 1_555 ?
N1 C1 1.280(10) 1_555 ?
N1 C1 2.160(10) 4_765 ?
N2 F1 2.727(10) 2_565 ?
N2 F2 3.425(6) 6_654 ?
N2 F2 3.425(6) 7_564 ?
N2 F2 3.425(6) 9_554 ?
N2 F2 3.425(6) 12_664 ?
N2 N1 2.128(10) 1_555 ?
N2 N1 2.128(10) 4_765 ?
N2 C1 1.373(9) 1_555 ?
N2 C1 1.373(9) 4_765 ?
C1 Co1 3.047(8) 1_555 ?
C1 F1 3.438(8) 1_555 ?
C1 F2 3.077(8) 1_555 ?
C1 F2 3.198(6) 8_556 ?
C1 F2 3.198(6) 10_566 ?
C1 F2 3.077(8) 15_565 ?
C1 N1 1.280(10) 1_555 ?
C1 N1 2.160(10) 4_765 ?
C1 N2 1.373(9) 1_555 ?
C1 C1 2.219(12) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Co1 F2 88.90(19) 1_555 3_656 ?
F2 Co1 F2 180.0(3) 1_555 13_666 ?
F2 Co1 F2 91.1(2) 1_555 15_565 ?
F2 Co1 N1 86.60(13) 1_555 1_555 ?
F2 Co1 N1 81.7(2) 1_555 2_466 ?
F2 Co1 N1 93.4(3) 1_555 3_656 ?
F2 Co1 N1 98.3(2) 1_555 4_765 ?
F2 Co1 C1 71.43(13) 1_555 1_555 ?
F2 Co1 C1 108.6(3) 1_555 3_656 ?
F2 Co1 F2 91.1(2) 3_656 13_666 ?
F2 Co1 F2 180.0(3) 3_656 15_565 ?
F2 Co1 N1 93.4(3) 3_656 1_555 ?
F2 Co1 N1 98.3(2) 3_656 2_466 ?
F2 Co1 N1 86.6(3) 3_656 3_656 ?
F2 Co1 N1 81.7(2) 3_656 4_765 ?
F2 Co1 C1 108.6(3) 3_656 1_555 ?
F2 Co1 C1 71.4(3) 3_656 3_656 ?
F2 Co1 F2 88.90(19) 13_666 15_565 ?
F2 Co1 N1 93.4(3) 13_666 1_555 ?
F2 Co1 N1 98.3(2) 13_666 2_466 ?
F2 Co1 N1 86.6(3) 13_666 3_656 ?
F2 Co1 N1 81.7(2) 13_666 4_765 ?
F2 Co1 C1 108.6(3) 13_666 1_555 ?
F2 Co1 C1 71.4(3) 13_666 3_656 ?
F2 Co1 N1 86.6(3) 15_565 1_555 ?
F2 Co1 N1 81.7(2) 15_565 2_466 ?
F2 Co1 N1 93.4(3) 15_565 3_656 ?
F2 Co1 N1 98.3(2) 15_565 4_765 ?
F2 Co1 C1 71.4(3) 15_565 1_555 ?
F2 Co1 C1 108.6(3) 15_565 3_656 ?
N1 Co1 N1 163.2(4) 1_555 2_466 ?
N1 Co1 N1 180.0(5) 1_555 3_656 ?
N1 Co1 C1 157.8(5) 1_555 3_656 ?
N1 Co1 N1 180.0(3) 2_466 4_765 ?
N1 Co1 C1 141.0(4) 2_466 1_555 ?
N1 Co1 N1 163.2(4) 3_656 4_765 ?
N1 Co1 C1 157.8(5) 3_656 1_555 ?
N1 Co1 C1 141.0(4) 4_765 3_656 ?
C1 Co1 C1 180.0(5) 1_555 3_656 ?
F1 V1 F1 180.00(19) 1_555 5_666 ?
F1 V1 F2 92.3(2) 1_555 1_555 ?
F1 V1 F2 87.68(16) 1_555 5_666 ?
F1 V1 F2 87.68(16) 1_555 10_566 ?
F1 V1 F2 92.3(2) 1_555 14_655 ?
F1 V1 F2 87.68(16) 5_666 1_555 ?
F1 V1 F2 92.3(2) 5_666 5_666 ?
F1 V1 F2 92.3(2) 5_666 10_566 ?
F1 V1 F2 87.68(16) 5_666 14_655 ?
F2 V1 F2 180.0(3) 1_555 5_666 ?
F2 V1 F2 90.1(2) 1_555 10_566 ?
F2 V1 F2 89.9(2) 1_555 14_655 ?
F2 V1 F2 89.9(2) 5_666 10_566 ?
F2 V1 F2 90.1(2) 5_666 14_655 ?
F2 V1 F2 180.0(3) 10_566 14_655 ?
V1 F1 V1 137.47(8) 1_555 4_665 ?
V1 F1 F2 102.80(16) 1_555 4_665 ?
V1 F1 F2 149.36(17) 1_555 8_556 ?
V1 F1 F2 149.36(17) 1_555 11_656 ?
V1 F1 F2 102.80(16) 1_555 15_565 ?
V1 F1 N2 111.3(4) 1_555 2_465 ?
V1 F1 C1 88.38(6) 1_555 1_555 ?
V1 F1 C1 88.4(3) 1_555 4_665 ?
V1 F1 F2 102.80(16) 4_665 1_555 ?
V1 F1 F2 149.36(17) 4_665 5_666 ?
V1 F1 F2 149.36(17) 4_665 10_566 ?
V1 F1 F2 102.80(16) 4_665 14_655 ?
V1 F1 N2 111.3(4) 4_665 2_465 ?
V1 F1 C1 88.4(3) 4_665 1_555 ?
V1 F1 C1 88.4(3) 4_665 4_665 ?
F2 F1 F2 89.14(18) 1_555 4_665 ?
F2 F1 F2 87.04(17) 1_555 5_666 ?
F2 F1 F2 110.09(19) 1_555 8_556 ?
F2 F1 F2 58.32(15) 1_555 10_566 ?
F2 F1 F2 144.8(2) 1_555 11_656 ?
F2 F1 F2 56.96(16) 1_555 14_655 ?
F2 F1 F2 61.98(17) 1_555 15_565 ?
F2 F1 N2 135.4(4) 1_555 2_465 ?
F2 F1 C1 57.9(2) 1_555 1_555 ?
F2 F1 C1 114.8(3) 1_555 4_665 ?
F2 F1 F2 110.09(19) 4_665 5_666 ?
F2 F1 F2 87.04(17) 4_665 8_556 ?
F2 F1 F2 144.8(2) 4_665 10_566 ?
F2 F1 F2 58.32(15) 4_665 11_656 ?
F2 F1 F2 61.98(17) 4_665 14_655 ?
F2 F1 F2 56.96(16) 4_665 15_565 ?
F2 F1 N2 135.4(4) 4_665 2_465 ?
F2 F1 C1 114.8(3) 4_665 1_555 ?
F2 F1 C1 57.9(2) 4_665 4_665 ?
F2 F1 F2 156.35(20) 5_666 8_556 ?
F2 F1 F2 59.54(12) 5_666 10_566 ?
F2 F1 F2 115.02(18) 5_666 11_656 ?
F2 F1 F2 58.32(15) 5_666 14_655 ?
F2 F1 F2 144.8(2) 5_666 15_565 ?
F2 F1 N2 78.2(3) 5_666 2_465 ?
F2 F1 C1 120.7(3) 5_666 1_555 ?
F2 F1 C1 61.38(20) 5_666 4_665 ?
F2 F1 F2 115.02(18) 8_556 10_566 ?
F2 F1 F2 59.54(12) 8_556 11_656 ?
F2 F1 F2 144.8(2) 8_556 14_655 ?
F2 F1 F2 58.32(15) 8_556 15_565 ?
F2 F1 N2 78.2(3) 8_556 2_465 ?
F2 F1 C1 61.38(20) 8_556 1_555 ?
F2 F1 C1 120.7(3) 8_556 4_665 ?
F2 F1 F2 156.35(20) 10_566 11_656 ?
F2 F1 F2 87.04(17) 10_566 14_655 ?
F2 F1 F2 110.09(19) 10_566 15_565 ?
F2 F1 N2 78.2(3) 10_566 2_465 ?
F2 F1 C1 61.38(20) 10_566 1_555 ?
F2 F1 C1 120.7(3) 10_566 4_665 ?
F2 F1 F2 110.09(19) 11_656 14_655 ?
F2 F1 F2 87.04(17) 11_656 15_565 ?
F2 F1 N2 78.2(3) 11_656 2_465 ?
F2 F1 C1 120.7(3) 11_656 1_555 ?
F2 F1 C1 61.38(20) 11_656 4_665 ?
F2 F1 F2 89.14(18) 14_655 15_565 ?
F2 F1 N2 135.4(4) 14_655 2_465 ?
F2 F1 C1 114.8(3) 14_655 1_555 ?
F2 F1 C1 57.9(2) 14_655 4_665 ?
F2 F1 N2 135.4(4) 15_565 2_465 ?
F2 F1 C1 57.9(2) 15_565 1_555 ?
F2 F1 C1 114.8(3) 15_565 4_665 ?
N2 F1 C1 94.5(4) 2_465 1_555 ?
N2 F1 C1 94.5(4) 2_465 4_665 ?
C1 F1 C1 171.1(4) 1_555 4_665 ?
Co1 F2 V1 146.71(12) 1_555 1_555 ?
Co1 F2 F1 103.2(2) 1_555 1_555 ?
Co1 F2 F1 159.61(14) 1_555 5_666 ?
Co1 F2 F2 45.55(13) 1_555 3_656 ?
Co1 F2 F2 136.57(18) 1_555 10_566 ?
Co1 F2 F2 117.11(16) 1_555 14_655 ?
Co1 F2 N1 49.96(19) 1_555 1_555 ?
Co1 F2 N1 46.19(19) 1_555 3_656 ?
Co1 F2 N2 108.47(15) 1_555 6_645 ?
Co1 F2 C1 69.84(14) 1_555 1_555 ?
Co1 F2 C1 110.4(2) 1_555 8_546 ?
V1 F2 F1 45.26(14) 1_555 1_555 ?
V1 F2 F1 47.70(12) 1_555 5_666 ?
V1 F2 F2 166.13(18) 1_555 3_656 ?
V1 F2 F2 45.06(13) 1_555 14_655 ?
V1 F2 F2 102.63(17) 1_555 15_565 ?
V1 F2 N1 126.0(3) 1_555 1_555 ?
V1 F2 N1 122.1(3) 1_555 3_656 ?
V1 F2 N2 90.3(3) 1_555 6_645 ?
V1 F2 C1 101.6(3) 1_555 1_555 ?
V1 F2 C1 97.5(3) 1_555 8_546 ?
F1 F2 F1 92.96(15) 1_555 5_666 ?
F1 F2 F2 148.3(2) 1_555 3_656 ?
F1 F2 F2 58.77(15) 1_555 10_566 ?
F1 F2 F2 61.52(17) 1_555 14_655 ?
F1 F2 F2 59.01(16) 1_555 15_565 ?
F1 F2 N1 91.4(2) 1_555 1_555 ?
F1 F2 N1 105.9(3) 1_555 3_656 ?
F1 F2 N2 127.4(3) 1_555 6_645 ?
F1 F2 C1 71.2(3) 1_555 1_555 ?
F1 F2 C1 119.7(2) 1_555 8_546 ?
F1 F2 F2 118.60(18) 5_666 3_656 ?
F1 F2 F2 62.91(15) 5_666 10_566 ?
F1 F2 F2 60.23(13) 5_666 14_655 ?
F1 F2 F2 147.51(16) 5_666 15_565 ?
F1 F2 N1 143.21(20) 5_666 1_555 ?
F1 F2 N1 117.5(2) 5_666 3_656 ?
F1 F2 N2 51.2(2) 5_666 6_645 ?
F1 F2 C1 128.2(3) 5_666 1_555 ?
F1 F2 C1 70.7(2) 5_666 8_546 ?
F2 F2 F2 136.24(19) 3_656 10_566 ?
F2 F2 F2 130.60(19) 3_656 14_655 ?
F2 F2 F2 90.00(16) 3_656 15_565 ?
F2 F2 N1 65.33(19) 3_656 1_555 ?
F2 F2 N1 58.94(18) 3_656 3_656 ?
F2 F2 N2 76.90(14) 3_656 6_645 ?
F2 F2 C1 89.3(3) 3_656 1_555 ?
F2 F2 C1 76.8(2) 3_656 8_546 ?
F2 F2 F2 90.00(17) 10_566 14_655 ?
F2 F2 F2 107.99(18) 10_566 15_565 ?
F2 F2 N1 88.9(2) 10_566 1_555 ?
F2 F2 N1 164.1(3) 10_566 3_656 ?
F2 F2 N2 113.4(3) 10_566 6_645 ?
F2 F2 C1 66.9(2) 10_566 1_555 ?
F2 F2 C1 62.3(2) 10_566 8_546 ?
F2 F2 F2 90.00(17) 14_655 15_565 ?
F2 F2 N1 148.4(3) 14_655 1_555 ?
F2 F2 N1 77.8(2) 14_655 3_656 ?
F2 F2 N2 66.92(19) 14_655 6_645 ?
F2 F2 C1 132.6(3) 14_655 1_555 ?
F2 F2 C1 130.7(3) 14_655 8_546 ?
F2 F2 N1 60.54(17) 15_565 1_555 ?
F2 F2 N1 62.38(19) 15_565 3_656 ?
F2 F2 N2 131.76(20) 15_565 6_645 ?
F2 F2 C1 61.9(2) 15_565 1_555 ?
F2 F2 C1 135.5(2) 15_565 8_546 ?
N1 F2 N1 96.1(3) 1_555 3_656 ?
N1 F2 N2 140.9(3) 1_555 6_645 ?
N1 F2 C1 75.48(16) 1_555 8_546 ?
N1 F2 N2 71.33(16) 3_656 6_645 ?
N1 F2 C1 114.2(4) 3_656 1_555 ?
N1 F2 C1 133.6(3) 3_656 8_546 ?
N2 F2 C1 159.7(3) 6_645 1_555 ?
N2 F2 C1 86.8(3) 6_645 8_546 ?
C1 F2 C1 75.49(19) 1_555 8_546 ?
Co1 N1 Co1 105.90(18) 1_555 2_566 ?
Co1 N1 N1 134.5(5) 1_555 4_765 ?
Co1 N1 N2 154.2(5) 1_555 1_555 ?
Co1 N1 C1 116.0(7) 1_555 1_555 ?
Co1 N1 C1 168.5(5) 1_555 4_765 ?
Co1 N1 F2 131.39(17) 2_566 1_555 ?
Co1 N1 F2 76.87(17) 2_566 3_656 ?
Co1 N1 F2 76.87(17) 2_566 13_666 ?
Co1 N1 F2 131.39(17) 2_566 15_565 ?
Co1 N1 N2 99.9(4) 2_566 1_555 ?
Co1 N1 C1 138.1(7) 2_566 1_555 ?
Co1 N1 C1 62.6(3) 2_566 4_765 ?
F2 N1 F2 55.74(17) 1_555 3_656 ?
F2 N1 F2 83.85(19) 1_555 13_666 ?
F2 N1 F2 58.92(17) 1_555 15_565 ?
F2 N1 N1 148.4(5) 1_555 4_765 ?
F2 N1 N2 116.4(4) 1_555 1_555 ?
F2 N1 C1 83.4(6) 1_555 1_555 ?
F2 N1 C1 143.8(5) 1_555 4_765 ?
F2 N1 F2 55.24(18) 3_656 13_666 ?
F2 N1 F2 83.85(19) 3_656 15_565 ?
F2 N1 N1 102.2(5) 3_656 4_765 ?
F2 N1 N2 152.0(5) 3_656 1_555 ?
F2 N1 C1 137.8(6) 3_656 1_555 ?
F2 N1 C1 131.0(4) 3_656 4_765 ?
F2 N1 F2 55.74(17) 13_666 15_565 ?
F2 N1 N1 102.2(5) 13_666 4_765 ?
F2 N1 N2 152.0(5) 13_666 1_555 ?
F2 N1 C1 137.8(6) 13_666 1_555 ?
F2 N1 C1 131.0(4) 13_666 4_765 ?
F2 N1 N1 148.4(5) 15_565 4_765 ?
F2 N1 N2 116.4(4) 15_565 1_555 ?
F2 N1 C1 83.4(6) 15_565 1_555 ?
F2 N1 C1 143.8(5) 15_565 4_765 ?
N1 N1 N2 71.3(6) 4_765 1_555 ?
N1 N1 C1 109.5(9) 4_765 1_555 ?
C1 N1 C1 75.6(7) 1_555 4_765 ?
F1 N2 F2 50.6(2) 2_565 6_654 ?
F1 N2 F2 50.6(2) 2_565 7_564 ?
F1 N2 F2 50.6(2) 2_565 9_554 ?
F1 N2 F2 50.6(2) 2_565 12_664 ?
F1 N2 N1 161.3(5) 2_565 1_555 ?
F1 N2 N1 161.3(5) 2_565 4_765 ?
F1 N2 C1 126.1(7) 2_565 1_555 ?
F1 N2 C1 126.1(7) 2_565 4_765 ?
F2 N2 F2 101.23(18) 6_654 7_564 ?
F2 N2 F2 46.17(15) 6_654 9_554 ?
F2 N2 F2 83.53(17) 6_654 12_664 ?
F2 N2 N1 118.4(4) 6_654 1_555 ?
F2 N2 N1 136.6(4) 6_654 4_765 ?
F2 N2 C1 93.3(5) 6_654 1_555 ?
F2 N2 C1 133.7(6) 6_654 4_765 ?
F2 N2 F2 83.53(17) 7_564 9_554 ?
F2 N2 F2 46.17(15) 7_564 12_664 ?
F2 N2 N1 136.6(4) 7_564 1_555 ?
F2 N2 N1 118.4(4) 7_564 4_765 ?
F2 N2 C1 133.7(6) 7_564 1_555 ?
F2 N2 C1 93.3(5) 7_564 4_765 ?
F2 N2 F2 101.23(18) 9_554 12_664 ?
F2 N2 N1 136.6(4) 9_554 1_555 ?
F2 N2 N1 118.4(4) 9_554 4_765 ?
F2 N2 C1 133.7(6) 9_554 1_555 ?
F2 N2 C1 93.3(5) 9_554 4_765 ?
F2 N2 N1 118.4(4) 12_664 1_555 ?
F2 N2 N1 136.6(4) 12_664 4_765 ?
F2 N2 C1 93.3(5) 12_664 1_555 ?
F2 N2 C1 133.7(6) 12_664 4_765 ?
N1 N2 C1 72.6(6) 1_555 4_765 ?
N1 N2 C1 72.6(6) 4_765 1_555 ?
C1 N2 C1 107.8(10) 1_555 4_765 ?
Co1 C1 F1 72.1(2) 1_555 1_555 ?
Co1 C1 F2 89.42(20) 1_555 8_556 ?
Co1 C1 F2 89.42(20) 1_555 10_566 ?
Co1 C1 N1 78.4(3) 1_555 4_765 ?
Co1 C1 N2 148.4(6) 1_555 1_555 ?
Co1 C1 C1 112.4(4) 1_555 4_765 ?
F1 C1 F2 50.9(2) 1_555 1_555 ?
F1 C1 F2 47.94(18) 1_555 8_556 ?
F1 C1 F2 47.94(18) 1_555 10_566 ?
F1 C1 F2 50.9(2) 1_555 15_565 ?
F1 C1 N1 114.0(6) 1_555 1_555 ?
F1 C1 N1 150.5(4) 1_555 4_765 ?
F1 C1 N2 139.4(4) 1_555 1_555 ?
F1 C1 C1 175.5(5) 1_555 4_765 ?
F2 C1 F2 92.3(2) 1_555 8_556 ?
F2 C1 F2 50.77(19) 1_555 10_566 ?
F2 C1 F2 56.2(2) 1_555 15_565 ?
F2 C1 N1 72.2(5) 1_555 1_555 ?
F2 C1 N1 104.3(4) 1_555 4_765 ?
F2 C1 N2 151.66(11) 1_555 1_555 ?
F2 C1 C1 132.6(5) 1_555 4_765 ?
F2 C1 F2 91.03(19) 8_556 10_566 ?
F2 C1 F2 50.77(19) 8_556 15_565 ?
F2 C1 N1 117.4(6) 8_556 1_555 ?
F2 C1 N1 133.2(4) 8_556 4_765 ?
F2 C1 N2 112.0(4) 8_556 1_555 ?
F2 C1 C1 130.7(4) 8_556 4_765 ?
F2 C1 F2 92.3(2) 10_566 15_565 ?
F2 C1 N1 117.4(6) 10_566 1_555 ?
F2 C1 N1 133.2(4) 10_566 4_765 ?
F2 C1 N2 112.0(4) 10_566 1_555 ?
F2 C1 C1 130.7(4) 10_566 4_765 ?
F2 C1 N1 72.2(5) 15_565 1_555 ?
F2 C1 N1 104.3(4) 15_565 4_765 ?
F2 C1 N2 151.7(5) 15_565 1_555 ?
F2 C1 C1 132.6(5) 15_565 4_765 ?
N1 C1 N2 106.6(9) 1_555 1_555 ?
N1 C1 C1 70.5(7) 1_555 4_765 ?
N1 C1 N2 70.0(6) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_ZnVF5Htaz
_database_code_depnum_ccdc_archive 'CCDC 1527752'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 F5 N3 V Zn'
_chemical_formula_weight         277.38
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Zn Zn 0.284 1.430 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.301 O.529 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.0595(4)
_cell_length_b                   7.4628(3)
_cell_length_c                   9.4321(4)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     637.70(5)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5582
_pd_meas_2theta_range_min        5.11700
_pd_meas_2theta_range_max        99.99400
_pd_meas_2theta_range_inc        0.017001

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        3.4604
_pd_proc_ls_prof_wR_factor       5.9722
_pd_proc_ls_prof_wR_expected     1.7205

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       11.2260
_pd_proc_ls_prof_cwR_factor      12.8987
_pd_proc_ls_prof_cwR_expected    3.7159

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            12.0491
_pd_proc_ls_prof_echi2           12.5317
_refine_ls_goodness_of_fit_all   3.4712

#  Items related to LS refinement

_refine_ls_R_I_factor            3.8384
_refine_ls_number_reflns         416
_refine_ls_number_parameters     50
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        5.1230
_pd_proc_2theta_range_max        100.0000
_pd_proc_2theta_range_inc        0.017001
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Zn1 0.75000 0.75000 0.75000 0.0288(7) 1.00000 Uiso Zn
V1 0.50000 0.50000 0.50000 0.0199(10) 1.00000 Uiso V
F1 0.50000 0.75000 0.4245(6) 0.0239(11) 1.00000 Uiso F
F2 0.6470(3) 0.5563(4) 0.6332(3) 0.0239(11) 1.00000 Uiso F
N1 0.9250(5) 0.75000 0.5796(6) 0.0155(19) 1.00000 Uiso N
N2 1.00000 0.75000 0.3704(9) 0.0155(19) 1.00000 Uiso N
C1 0.8750(8) 0.75000 0.4509(8) 0.0155(19) 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn1 F2 2.043(3) 1_555 ?
Zn1 F2 2.043(3) 3_656 ?
Zn1 F2 2.043(3) 13_666 ?
Zn1 F2 2.043(3) 15_565 ?
Zn1 N1 2.258(5) 1_555 ?
Zn1 N1 3.354(5) 2_466 ?
Zn1 N1 2.258(5) 3_656 ?
Zn1 N1 3.354(5) 4_765 ?
Zn1 C1 3.040(8) 1_555 ?
Zn1 C1 3.040(8) 3_656 ?
V1 F1 1.997(2) 1_555 ?
V1 F1 1.997(2) 5_666 ?
V1 F2 1.878(3) 1_555 ?
V1 F2 1.878(3) 5_666 ?
V1 F2 1.878(3) 10_566 ?
V1 F2 1.878(3) 14_655 ?
F1 V1 1.997(2) 1_555 ?
F1 V1 1.997(2) 4_665 ?
F1 F2 2.782(5) 1_555 ?
F1 F2 2.782(5) 4_665 ?
F1 F2 2.701(3) 5_666 ?
F1 F2 2.701(3) 8_556 ?
F1 F2 2.701(3) 10_566 ?
F1 F2 2.701(3) 11_656 ?
F1 F2 2.782(5) 14_655 ?
F1 F2 2.782(5) 15_565 ?
F1 N2 2.782(10) 2_465 ?
F1 C1 3.406(7) 1_555 ?
F1 C1 3.406(7) 4_665 ?
F2 Zn1 2.043(3) 1_555 ?
F2 V1 1.878(3) 1_555 ?
F2 F1 2.782(5) 1_555 ?
F2 F1 2.701(3) 5_666 ?
F2 F2 2.887(4) 3_656 ?
F2 F2 2.649(4) 10_566 ?
F2 F2 2.663(4) 14_655 ?
F2 F2 2.891(4) 15_565 ?
F2 N1 2.948(5) 1_555 ?
F2 N1 3.139(6) 3_656 ?
F2 N2 3.465(6) 6_645 ?
F2 C1 3.052(7) 1_555 ?
F2 C1 3.181(6) 8_546 ?
N1 Zn1 2.258(5) 1_555 ?
N1 Zn1 3.354(5) 2_566 ?
N1 F2 2.948(5) 1_555 ?
N1 F2 3.139(6) 3_656 ?
N1 F2 3.139(6) 13_666 ?
N1 F2 2.948(5) 15_565 ?
N1 N1 1.359(6) 4_765 ?
N1 N2 2.087(10) 1_555 ?
N1 C1 1.296(9) 1_555 ?
N1 C1 2.181(9) 4_765 ?
N2 F1 2.782(10) 2_565 ?
N2 F2 3.465(6) 6_654 ?
N2 F2 3.465(6) 7_564 ?
N2 F2 3.465(6) 9_554 ?
N2 F2 3.465(6) 12_664 ?
N2 N1 2.087(10) 1_555 ?
N2 N1 2.087(10) 4_765 ?
N2 C1 1.363(9) 1_555 ?
N2 C1 1.363(9) 4_765 ?
C1 Zn1 3.040(8) 1_555 ?
C1 F1 3.406(7) 1_555 ?
C1 F2 3.052(7) 1_555 ?
C1 F2 3.181(6) 8_556 ?
C1 F2 3.181(6) 10_566 ?
C1 F2 3.052(7) 15_565 ?
C1 N1 1.296(9) 1_555 ?
C1 N1 2.181(9) 4_765 ?
C1 N2 1.363(9) 1_555 ?
C1 C1 2.265(10) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Zn1 F2 89.93(19) 1_555 3_656 ?
F2 Zn1 F2 180.0(3) 1_555 13_666 ?
F2 Zn1 F2 90.1(2) 1_555 15_565 ?
F2 Zn1 N1 86.4(2) 1_555 1_555 ?
F2 Zn1 N1 81.8(2) 1_555 2_466 ?
F2 Zn1 N1 93.6(3) 1_555 3_656 ?
F2 Zn1 N1 98.2(2) 1_555 4_765 ?
F2 Zn1 C1 70.71(12) 1_555 1_555 ?
F2 Zn1 C1 109.3(3) 1_555 3_656 ?
F2 Zn1 F2 90.1(2) 3_656 13_666 ?
F2 Zn1 F2 180.0(3) 3_656 15_565 ?
F2 Zn1 N1 93.6(3) 3_656 1_555 ?
F2 Zn1 N1 98.2(2) 3_656 2_466 ?
F2 Zn1 N1 86.4(2) 3_656 3_656 ?
F2 Zn1 N1 81.8(2) 3_656 4_765 ?
F2 Zn1 C1 109.3(3) 3_656 1_555 ?
F2 Zn1 C1 70.7(3) 3_656 3_656 ?
F2 Zn1 F2 89.93(19) 13_666 15_565 ?
F2 Zn1 N1 93.6(3) 13_666 1_555 ?
F2 Zn1 N1 98.2(2) 13_666 2_466 ?
F2 Zn1 N1 86.4(2) 13_666 3_656 ?
F2 Zn1 N1 81.8(2) 13_666 4_765 ?
F2 Zn1 C1 109.3(3) 13_666 1_555 ?
F2 Zn1 C1 70.7(3) 13_666 3_656 ?
F2 Zn1 N1 86.4(2) 15_565 1_555 ?
F2 Zn1 N1 81.8(2) 15_565 2_466 ?
F2 Zn1 N1 93.6(3) 15_565 3_656 ?
F2 Zn1 N1 98.2(2) 15_565 4_765 ?
F2 Zn1 C1 70.7(3) 15_565 1_555 ?
F2 Zn1 C1 109.3(3) 15_565 3_656 ?
N1 Zn1 N1 163.2(3) 1_555 2_466 ?
N1 Zn1 N1 180.0(4) 1_555 3_656 ?
N1 Zn1 C1 157.3(4) 1_555 3_656 ?
N1 Zn1 N1 180.0(3) 2_466 4_765 ?
N1 Zn1 C1 140.5(3) 2_466 1_555 ?
N1 Zn1 N1 163.2(3) 3_656 4_765 ?
N1 Zn1 C1 157.3(4) 3_656 1_555 ?
N1 Zn1 C1 140.5(3) 4_765 3_656 ?
C1 Zn1 C1 180.0(4) 1_555 3_656 ?
F1 V1 F1 180.00(18) 1_555 5_666 ?
F1 V1 F2 91.7(2) 1_555 1_555 ?
F1 V1 F2 88.31(17) 1_555 5_666 ?
F1 V1 F2 88.31(17) 1_555 10_566 ?
F1 V1 F2 91.7(2) 1_555 14_655 ?
F1 V1 F2 88.31(17) 5_666 1_555 ?
F1 V1 F2 91.7(2) 5_666 5_666 ?
F1 V1 F2 91.7(2) 5_666 10_566 ?
F1 V1 F2 88.31(17) 5_666 14_655 ?
F2 V1 F2 180.0(3) 1_555 5_666 ?
F2 V1 F2 89.7(2) 1_555 10_566 ?
F2 V1 F2 90.3(2) 1_555 14_655 ?
F2 V1 F2 90.3(2) 5_666 10_566 ?
F2 V1 F2 89.7(2) 5_666 14_655 ?
F2 V1 F2 180.0(3) 10_566 14_655 ?
V1 F1 V1 138.22(8) 1_555 4_665 ?
V1 F1 F2 103.48(16) 1_555 4_665 ?
V1 F1 F2 149.60(17) 1_555 8_556 ?
V1 F1 F2 149.60(17) 1_555 11_656 ?
V1 F1 F2 103.48(16) 1_555 15_565 ?
V1 F1 N2 110.9(4) 1_555 2_465 ?
V1 F1 C1 88.51(6) 1_555 1_555 ?
V1 F1 C1 88.5(2) 1_555 4_665 ?
V1 F1 F2 103.48(16) 4_665 1_555 ?
V1 F1 F2 149.60(17) 4_665 5_666 ?
V1 F1 F2 149.60(17) 4_665 10_566 ?
V1 F1 F2 103.48(16) 4_665 14_655 ?
V1 F1 N2 110.9(4) 4_665 2_465 ?
V1 F1 C1 88.5(2) 4_665 1_555 ?
V1 F1 C1 88.5(2) 4_665 4_665 ?
F2 F1 F2 89.91(19) 1_555 4_665 ?
F2 F1 F2 86.49(17) 1_555 5_666 ?
F2 F1 F2 110.26(19) 1_555 8_556 ?
F2 F1 F2 57.77(15) 1_555 10_566 ?
F2 F1 F2 144.9(2) 1_555 11_656 ?
F2 F1 F2 57.21(16) 1_555 14_655 ?
F2 F1 F2 62.62(17) 1_555 15_565 ?
F2 F1 N2 135.0(4) 1_555 2_465 ?
F2 F1 C1 58.0(2) 1_555 1_555 ?
F2 F1 C1 115.2(3) 1_555 4_665 ?
F2 F1 F2 110.26(19) 4_665 5_666 ?
F2 F1 F2 86.49(17) 4_665 8_556 ?
F2 F1 F2 144.9(2) 4_665 10_566 ?
F2 F1 F2 57.77(15) 4_665 11_656 ?
F2 F1 F2 62.62(17) 4_665 14_655 ?
F2 F1 F2 57.21(16) 4_665 15_565 ?
F2 F1 N2 135.0(4) 4_665 2_465 ?
F2 F1 C1 115.2(3) 4_665 1_555 ?
F2 F1 C1 58.0(2) 4_665 4_665 ?
F2 F1 F2 156.75(20) 5_666 8_556 ?
F2 F1 F2 59.09(12) 5_666 10_566 ?
F2 F1 F2 115.63(18) 5_666 11_656 ?
F2 F1 F2 57.77(15) 5_666 14_655 ?
F2 F1 F2 144.9(2) 5_666 15_565 ?
F2 F1 N2 78.4(3) 5_666 2_465 ?
F2 F1 C1 120.4(3) 5_666 1_555 ?
F2 F1 C1 61.51(18) 5_666 4_665 ?
F2 F1 F2 115.63(18) 8_556 10_566 ?
F2 F1 F2 59.09(12) 8_556 11_656 ?
F2 F1 F2 144.9(2) 8_556 14_655 ?
F2 F1 F2 57.77(15) 8_556 15_565 ?
F2 F1 N2 78.4(3) 8_556 2_465 ?
F2 F1 C1 61.51(18) 8_556 1_555 ?
F2 F1 C1 120.4(3) 8_556 4_665 ?
F2 F1 F2 156.75(20) 10_566 11_656 ?
F2 F1 F2 86.49(17) 10_566 14_655 ?
F2 F1 F2 110.26(19) 10_566 15_565 ?
F2 F1 N2 78.4(3) 10_566 2_465 ?
F2 F1 C1 61.51(18) 10_566 1_555 ?
F2 F1 C1 120.4(3) 10_566 4_665 ?
F2 F1 F2 110.26(19) 11_656 14_655 ?
F2 F1 F2 86.49(17) 11_656 15_565 ?
F2 F1 N2 78.4(3) 11_656 2_465 ?
F2 F1 C1 120.4(3) 11_656 1_555 ?
F2 F1 C1 61.51(18) 11_656 4_665 ?
F2 F1 F2 89.91(19) 14_655 15_565 ?
F2 F1 N2 135.0(4) 14_655 2_465 ?
F2 F1 C1 115.2(3) 14_655 1_555 ?
F2 F1 C1 58.0(2) 14_655 4_665 ?
F2 F1 N2 135.0(4) 15_565 2_465 ?
F2 F1 C1 58.0(2) 15_565 1_555 ?
F2 F1 C1 115.2(3) 15_565 4_665 ?
N2 F1 C1 94.2(4) 2_465 1_555 ?
N2 F1 C1 94.2(4) 2_465 4_665 ?
C1 F1 C1 171.6(4) 1_555 4_665 ?
Zn1 F2 V1 147.43(12) 1_555 1_555 ?
Zn1 F2 F1 103.4(2) 1_555 1_555 ?
Zn1 F2 F1 158.86(14) 1_555 5_666 ?
Zn1 F2 F2 45.04(13) 1_555 3_656 ?
Zn1 F2 F2 137.37(18) 1_555 10_566 ?
Zn1 F2 F2 117.18(16) 1_555 14_655 ?
Zn1 F2 N1 49.85(17) 1_555 1_555 ?
Zn1 F2 N1 45.87(17) 1_555 3_656 ?
Zn1 F2 N2 107.11(15) 1_555 6_645 ?
Zn1 F2 C1 70.09(14) 1_555 1_555 ?
Zn1 F2 C1 110.26(20) 1_555 8_546 ?
V1 F2 F1 45.85(14) 1_555 1_555 ?
V1 F2 F1 47.65(12) 1_555 5_666 ?
V1 F2 F2 165.60(18) 1_555 3_656 ?
V1 F2 F2 45.15(14) 1_555 10_566 ?
V1 F2 F2 102.92(17) 1_555 15_565 ?
V1 F2 N1 126.9(2) 1_555 1_555 ?
V1 F2 N1 122.2(3) 1_555 3_656 ?
V1 F2 N2 90.7(3) 1_555 6_645 ?
V1 F2 C1 102.1(3) 1_555 1_555 ?
V1 F2 C1 97.6(3) 1_555 8_546 ?
F1 F2 F1 93.51(15) 1_555 5_666 ?
F1 F2 F2 148.1(2) 1_555 3_656 ?
F1 F2 F2 59.58(15) 1_555 10_566 ?
F1 F2 F2 61.40(17) 1_555 14_655 ?
F1 F2 F2 58.69(16) 1_555 15_565 ?
F1 F2 N1 91.9(2) 1_555 1_555 ?
F1 F2 N1 105.8(3) 1_555 3_656 ?
F1 F2 N2 128.0(3) 1_555 6_645 ?
F1 F2 C1 71.3(2) 1_555 1_555 ?
F1 F2 C1 120.5(2) 1_555 8_546 ?
F1 F2 F2 118.19(18) 5_666 3_656 ?
F1 F2 F2 62.64(15) 5_666 10_566 ?
F1 F2 F2 60.46(13) 5_666 14_655 ?
F1 F2 F2 147.81(16) 5_666 15_565 ?
F1 F2 N1 143.30(17) 5_666 1_555 ?
F1 F2 N1 117.5(2) 5_666 3_656 ?
F1 F2 N2 51.8(2) 5_666 6_645 ?
F1 F2 C1 128.4(2) 5_666 1_555 ?
F1 F2 C1 70.2(2) 5_666 8_546 ?
F2 F2 F2 136.36(19) 3_656 10_566 ?
F2 F2 F2 130.27(18) 3_656 14_655 ?
F2 F2 F2 90.00(16) 3_656 15_565 ?
F2 F2 N1 65.08(17) 3_656 1_555 ?
F2 F2 N1 58.39(16) 3_656 3_656 ?
F2 F2 N2 75.86(14) 3_656 6_645 ?
F2 F2 C1 89.6(3) 3_656 1_555 ?
F2 F2 C1 76.7(2) 3_656 8_546 ?
F2 F2 F2 90.00(17) 10_566 14_655 ?
F2 F2 F2 108.49(18) 10_566 15_565 ?
F2 F2 N1 89.59(19) 10_566 1_555 ?
F2 F2 N1 164.7(3) 10_566 3_656 ?
F2 F2 N2 113.8(3) 10_566 6_645 ?
F2 F2 C1 67.4(2) 10_566 1_555 ?
F2 F2 C1 62.3(2) 10_566 8_546 ?
F2 F2 F2 90.00(17) 14_655 15_565 ?
F2 F2 N1 148.7(2) 14_655 1_555 ?
F2 F2 N1 78.01(19) 14_655 3_656 ?
F2 F2 N2 67.40(19) 14_655 6_645 ?
F2 F2 C1 132.6(3) 14_655 1_555 ?
F2 F2 C1 130.5(3) 14_655 8_546 ?
F2 F2 N1 60.63(16) 15_565 1_555 ?
F2 F2 N1 62.58(18) 15_565 3_656 ?
F2 F2 N2 131.28(20) 15_565 6_645 ?
F2 F2 C1 61.7(2) 15_565 1_555 ?
F2 F2 C1 135.93(20) 15_565 8_546 ?
N1 F2 N1 95.7(2) 1_555 3_656 ?
N1 F2 N2 139.7(2) 1_555 6_645 ?
N1 F2 C1 75.81(14) 1_555 8_546 ?
N1 F2 N2 70.53(15) 3_656 6_645 ?
N1 F2 C1 114.1(3) 3_656 1_555 ?
N1 F2 C1 132.9(3) 3_656 8_546 ?
N2 F2 C1 159.5(3) 6_645 1_555 ?
N2 F2 C1 86.4(3) 6_645 8_546 ?
C1 F2 C1 76.14(18) 1_555 8_546 ?
Zn1 N1 Zn1 105.98(15) 1_555 2_566 ?
Zn1 N1 N1 134.6(4) 1_555 4_765 ?
Zn1 N1 N2 154.4(5) 1_555 1_555 ?
Zn1 N1 C1 114.9(6) 1_555 1_555 ?
Zn1 N1 C1 168.4(5) 1_555 4_765 ?
Zn1 N1 F2 131.90(16) 2_566 1_555 ?
Zn1 N1 F2 76.64(15) 2_566 3_656 ?
Zn1 N1 F2 76.64(15) 2_566 13_666 ?
Zn1 N1 F2 131.90(16) 2_566 15_565 ?
Zn1 N1 N2 99.6(4) 2_566 1_555 ?
Zn1 N1 C1 139.1(6) 2_566 1_555 ?
Zn1 N1 C1 62.4(3) 2_566 4_765 ?
F2 N1 F2 56.54(16) 1_555 3_656 ?
F2 N1 F2 84.28(17) 1_555 13_666 ?
F2 N1 F2 58.74(16) 1_555 15_565 ?
F2 N1 N1 148.7(4) 1_555 4_765 ?
F2 N1 N2 116.1(4) 1_555 1_555 ?
F2 N1 C1 82.1(5) 1_555 1_555 ?
F2 N1 C1 143.6(4) 1_555 4_765 ?
F2 N1 F2 54.84(16) 3_656 13_666 ?
F2 N1 F2 84.28(17) 3_656 15_565 ?
F2 N1 N1 102.0(4) 3_656 4_765 ?
F2 N1 N2 152.1(5) 3_656 1_555 ?
F2 N1 C1 137.4(6) 3_656 1_555 ?
F2 N1 C1 130.8(4) 3_656 4_765 ?
F2 N1 F2 56.54(16) 13_666 15_565 ?
F2 N1 N1 102.0(4) 13_666 4_765 ?
F2 N1 N2 152.1(5) 13_666 1_555 ?
F2 N1 C1 137.4(6) 13_666 1_555 ?
F2 N1 C1 130.8(4) 13_666 4_765 ?
F2 N1 N1 148.7(4) 15_565 4_765 ?
F2 N1 N2 116.1(4) 15_565 1_555 ?
F2 N1 C1 82.1(5) 15_565 1_555 ?
F2 N1 C1 143.6(4) 15_565 4_765 ?
N1 N1 N2 71.0(6) 4_765 1_555 ?
N1 N1 C1 110.5(8) 4_765 1_555 ?
C1 N1 C1 76.6(7) 1_555 4_765 ?
F1 N2 F2 49.8(2) 2_565 6_654 ?
F1 N2 F2 49.8(2) 2_565 7_564 ?
F1 N2 F2 49.8(2) 2_565 9_554 ?
F1 N2 F2 49.8(2) 2_565 12_664 ?
F1 N2 N1 161.0(5) 2_565 1_555 ?
F1 N2 N1 161.0(5) 2_565 4_765 ?
F1 N2 C1 123.8(7) 2_565 1_555 ?
F1 N2 C1 123.8(7) 2_565 4_765 ?
F2 N2 F2 99.56(18) 6_654 7_564 ?
F2 N2 F2 45.21(15) 6_654 9_554 ?
F2 N2 F2 82.56(17) 6_654 12_664 ?
F2 N2 N1 119.0(4) 6_654 1_555 ?
F2 N2 N1 137.4(4) 6_654 4_765 ?
F2 N2 C1 92.3(5) 6_654 1_555 ?
F2 N2 C1 132.8(5) 6_654 4_765 ?
F2 N2 F2 82.56(17) 7_564 9_554 ?
F2 N2 F2 45.21(15) 7_564 12_664 ?
F2 N2 N1 137.4(4) 7_564 1_555 ?
F2 N2 N1 119.0(4) 7_564 4_765 ?
F2 N2 C1 132.8(5) 7_564 1_555 ?
F2 N2 C1 92.3(5) 7_564 4_765 ?
F2 N2 F2 99.56(18) 9_554 12_664 ?
F2 N2 N1 137.4(4) 9_554 1_555 ?
F2 N2 N1 119.0(4) 9_554 4_765 ?
F2 N2 C1 132.8(5) 9_554 1_555 ?
F2 N2 C1 92.3(5) 9_554 4_765 ?
F2 N2 N1 119.0(4) 12_664 1_555 ?
F2 N2 N1 137.4(4) 12_664 4_765 ?
F2 N2 C1 92.3(5) 12_664 1_555 ?
F2 N2 C1 132.8(5) 12_664 4_765 ?
N1 N2 C1 75.2(6) 1_555 4_765 ?
N1 N2 C1 75.2(6) 4_765 1_555 ?
C1 N2 C1 112.3(9) 1_555 4_765 ?
Zn1 C1 F1 72.3(2) 1_555 1_555 ?
Zn1 C1 F2 89.40(19) 1_555 8_556 ?
Zn1 C1 F2 89.40(19) 1_555 10_566 ?
Zn1 C1 N1 78.1(3) 1_555 4_765 ?
Zn1 C1 N2 145.7(6) 1_555 1_555 ?
Zn1 C1 C1 111.9(4) 1_555 4_765 ?
F1 C1 F2 50.66(20) 1_555 1_555 ?
F1 C1 F2 48.26(17) 1_555 8_556 ?
F1 C1 F2 48.26(17) 1_555 10_566 ?
F1 C1 F2 50.66(20) 1_555 15_565 ?
F1 C1 N1 114.7(5) 1_555 1_555 ?
F1 C1 N1 150.4(3) 1_555 4_765 ?
F1 C1 N2 142.0(4) 1_555 1_555 ?
F1 C1 C1 175.8(4) 1_555 4_765 ?
F2 C1 F2 92.4(2) 1_555 8_556 ?
F2 C1 F2 50.26(18) 1_555 10_566 ?
F2 C1 F2 56.5(2) 1_555 15_565 ?
F2 C1 N1 73.1(5) 1_555 1_555 ?
F2 C1 N1 104.4(3) 1_555 4_765 ?
F2 C1 N2 151.16(13) 1_555 1_555 ?
F2 C1 C1 132.6(4) 1_555 4_765 ?
F2 C1 F2 91.86(18) 8_556 10_566 ?
F2 C1 F2 50.26(18) 8_556 15_565 ?
F2 C1 N1 117.4(5) 8_556 1_555 ?
F2 C1 N1 132.7(3) 8_556 4_765 ?
F2 C1 N2 113.6(4) 8_556 1_555 ?
F2 C1 C1 130.5(4) 8_556 4_765 ?
F2 C1 F2 92.4(2) 10_566 15_565 ?
F2 C1 N1 117.4(5) 10_566 1_555 ?
F2 C1 N1 132.7(3) 10_566 4_765 ?
F2 C1 N2 113.6(4) 10_566 1_555 ?
F2 C1 C1 130.5(4) 10_566 4_765 ?
F2 C1 N1 73.1(5) 15_565 1_555 ?
F2 C1 N1 104.4(3) 15_565 4_765 ?
F2 C1 N2 151.2(5) 15_565 1_555 ?
F2 C1 C1 132.6(4) 15_565 4_765 ?
N1 C1 N2 103.4(9) 1_555 1_555 ?
N1 C1 C1 69.5(6) 1_555 4_765 ?
N1 C1 N2 67.7(6) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_FeGaF5Htaz
_database_code_depnum_ccdc_archive 'CCDC 1527803'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 F5 Fe1.39 Ga0.61 N3'
_chemical_formula_weight         281.21
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe Fe 0.346 0.972 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.231 1.608 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.1404(4)
_cell_length_b                   7.4753(3)
_cell_length_c                   9.4629(4)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     646.58(5)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5582
_pd_meas_2theta_range_min        5.11700
_pd_meas_2theta_range_max        99.99400
_pd_meas_2theta_range_inc        0.017001

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.9214
_pd_proc_ls_prof_wR_factor       1.3013
_pd_proc_ls_prof_wR_expected     0.9838

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       21.2371
_pd_proc_ls_prof_cwR_factor      10.8660
_pd_proc_ls_prof_cwR_expected    8.2152

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            1.7495
_pd_proc_ls_prof_echi2           1.9040
_refine_ls_goodness_of_fit_all   1.3227

#  Items related to LS refinement

_refine_ls_R_I_factor            5.2000
_refine_ls_number_reflns         417
_refine_ls_number_parameters     47
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        5.0934
_pd_proc_2theta_range_max        99.9704
_pd_proc_2theta_range_inc        0.017001
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Fe1 0.75000 0.75000 0.75000 0.0199(11) 1.00000 Uiso Fe
Ga2 0.50000 0.50000 0.50000 0.0415(14) 0.61000 Uiso Ga
Fe2 0.50000 0.50000 0.50000 0.0415(14) 0.39000 Uiso Fe
F1 0.50000 0.75000 0.4329(8) 0.0180(15) 1.00000 Uiso F
F2 0.6504(4) 0.5568(5) 0.6385(3) 0.0180(15) 1.00000 Uiso F
N1 0.9218(8) 0.75000 0.5812(8) 0.014(3) 1.00000 Uiso N
N2 1.00000 0.75000 0.3682(10) 0.014(3) 1.00000 Uiso N
C1 0.8843(10) 0.75000 0.4504(11) 0.014(3) 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 F2 2.007(3) 1_555 ?
Fe1 F2 2.007(3) 3_656 ?
Fe1 F2 2.007(3) 13_666 ?
Fe1 F2 2.007(3) 15_565 ?
Fe1 N1 2.240(7) 1_555 ?
Fe1 N1 3.399(7) 2_466 ?
Fe1 N1 2.240(7) 3_656 ?
Fe1 N1 3.399(7) 4_765 ?
Fe1 C1 3.089(10) 1_555 ?
Fe1 C1 3.089(10) 3_656 ?
Ga2 F1 1.974(2) 1_555 ?
Ga2 F1 1.974(2) 5_666 ?
Ga2 F2 1.946(3) 1_555 ?
Ga2 F2 1.946(3) 5_666 ?
Ga2 F2 1.946(3) 10_566 ?
Ga2 F2 1.946(3) 14_655 ?
Fe2 F1 1.974(2) 1_555 ?
Fe2 F1 1.974(2) 5_666 ?
Fe2 F2 1.946(3) 1_555 ?
Fe2 F2 1.946(3) 5_666 ?
Fe2 F2 1.946(3) 10_566 ?
Fe2 F2 1.946(3) 14_655 ?
F1 Ga2 1.974(2) 1_555 ?
F1 Ga2 1.974(2) 4_665 ?
F1 Fe2 1.974(2) 1_555 ?
F1 Fe2 1.974(2) 4_665 ?
F1 F2 2.786(6) 1_555 ?
F1 F2 2.786(6) 4_665 ?
F1 F2 2.758(4) 5_666 ?
F1 F2 2.758(4) 8_556 ?
F1 F2 2.758(4) 10_566 ?
F1 F2 2.758(4) 11_656 ?
F1 F2 2.786(6) 14_655 ?
F1 F2 2.786(6) 15_565 ?
F1 N2 2.849(12) 2_465 ?
F2 Fe1 2.007(3) 1_555 ?
F2 Ga2 1.946(3) 1_555 ?
F2 Fe2 1.946(3) 1_555 ?
F2 F1 2.786(6) 1_555 ?
F2 F1 2.758(4) 5_666 ?
F2 F2 2.787(5) 3_656 ?
F2 F2 2.755(4) 10_566 ?
F2 F2 2.749(5) 14_655 ?
F2 F2 2.888(5) 15_565 ?
F2 N1 2.921(7) 1_555 ?
F2 N1 3.091(7) 3_656 ?
F2 N2 3.446(7) 6_645 ?
F2 C1 3.134(9) 1_555 ?
F2 C1 3.246(8) 8_546 ?
N1 Fe1 2.240(7) 1_555 ?
N1 Fe1 3.399(7) 2_566 ?
N1 F2 2.921(7) 1_555 ?
N1 F2 3.091(7) 3_656 ?
N1 F2 3.091(7) 13_666 ?
N1 F2 2.921(7) 15_565 ?
N1 N1 1.430(10) 4_765 ?
N1 N2 2.139(12) 1_555 ?
N1 C1 1.284(13) 1_555 ?
N1 C1 2.162(12) 4_765 ?
N2 F1 2.849(12) 2_565 ?
N2 F2 3.446(7) 6_654 ?
N2 F2 3.446(7) 7_564 ?
N2 F2 3.446(7) 9_554 ?
N2 F2 3.446(7) 12_664 ?
N2 N1 2.139(12) 1_555 ?
N2 N1 2.139(12) 4_765 ?
N2 C1 1.313(11) 1_555 ?
N2 C1 1.313(11) 4_765 ?
C1 Fe1 3.089(10) 1_555 ?
C1 F2 3.134(9) 1_555 ?
C1 F2 3.246(8) 8_556 ?
C1 F2 3.246(8) 10_566 ?
C1 F2 3.134(9) 15_565 ?
C1 N1 1.284(13) 1_555 ?
C1 N1 2.162(12) 4_765 ?
C1 N2 1.313(11) 1_555 ?
C1 C1 2.115(13) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Fe1 F2 88.0(2) 1_555 3_656 ?
F2 Fe1 F2 180.0(3) 1_555 13_666 ?
F2 Fe1 F2 92.0(3) 1_555 15_565 ?
F2 Fe1 N1 86.7(3) 1_555 1_555 ?
F2 Fe1 N1 81.2(3) 1_555 2_466 ?
F2 Fe1 N1 93.3(4) 1_555 3_656 ?
F2 Fe1 N1 98.8(3) 1_555 4_765 ?
F2 Fe1 C1 72.4(3) 1_555 1_555 ?
F2 Fe1 C1 107.6(4) 1_555 3_656 ?
F2 Fe1 F2 92.0(3) 3_656 13_666 ?
F2 Fe1 F2 180.0(3) 3_656 15_565 ?
F2 Fe1 N1 93.3(4) 3_656 1_555 ?
F2 Fe1 N1 98.8(3) 3_656 2_466 ?
F2 Fe1 N1 86.7(3) 3_656 3_656 ?
F2 Fe1 N1 81.2(3) 3_656 4_765 ?
F2 Fe1 C1 107.6(4) 3_656 1_555 ?
F2 Fe1 C1 72.4(3) 3_656 3_656 ?
F2 Fe1 F2 88.0(2) 13_666 15_565 ?
F2 Fe1 N1 93.3(4) 13_666 1_555 ?
F2 Fe1 N1 98.8(3) 13_666 2_466 ?
F2 Fe1 N1 86.7(3) 13_666 3_656 ?
F2 Fe1 N1 81.2(3) 13_666 4_765 ?
F2 Fe1 C1 107.6(4) 13_666 1_555 ?
F2 Fe1 C1 72.4(3) 13_666 3_656 ?
F2 Fe1 N1 86.7(3) 15_565 1_555 ?
F2 Fe1 N1 81.2(3) 15_565 2_466 ?
F2 Fe1 N1 93.3(4) 15_565 3_656 ?
F2 Fe1 N1 98.8(3) 15_565 4_765 ?
F2 Fe1 C1 72.4(3) 15_565 1_555 ?
F2 Fe1 C1 107.6(4) 15_565 3_656 ?
N1 Fe1 N1 162.5(5) 1_555 2_466 ?
N1 Fe1 N1 180.0(6) 1_555 3_656 ?
N1 Fe1 C1 158.9(6) 1_555 3_656 ?
N1 Fe1 N1 180.0(4) 2_466 4_765 ?
N1 Fe1 C1 141.4(5) 2_466 1_555 ?
N1 Fe1 N1 162.5(5) 3_656 4_765 ?
N1 Fe1 C1 158.9(6) 3_656 1_555 ?
N1 Fe1 C1 141.4(5) 4_765 3_656 ?
C1 Fe1 C1 180.0(6) 1_555 3_656 ?
F1 Ga2 F1 180.0(2) 1_555 5_666 ?
F1 Ga2 F2 90.6(3) 1_555 1_555 ?
F1 Ga2 F2 89.4(2) 1_555 5_666 ?
F1 Ga2 F2 89.4(2) 1_555 10_566 ?
F1 Ga2 F2 90.6(3) 1_555 14_655 ?
F1 Ga2 F2 89.4(2) 5_666 1_555 ?
F1 Ga2 F2 90.6(3) 5_666 5_666 ?
F1 Ga2 F2 90.6(3) 5_666 10_566 ?
F1 Ga2 F2 89.4(2) 5_666 14_655 ?
F2 Ga2 F2 180.0(3) 1_555 5_666 ?
F2 Ga2 F2 90.1(2) 1_555 10_566 ?
F2 Ga2 F2 89.9(3) 1_555 14_655 ?
F2 Ga2 F2 89.9(3) 5_666 10_566 ?
F2 Ga2 F2 90.1(2) 5_666 14_655 ?
F2 Ga2 F2 180.0(3) 10_566 14_655 ?
F1 Fe2 F1 180.0(2) 1_555 5_666 ?
F1 Fe2 F2 90.6(3) 1_555 1_555 ?
F1 Fe2 F2 89.4(2) 1_555 5_666 ?
F1 Fe2 F2 89.4(2) 1_555 10_566 ?
F1 Fe2 F2 90.6(3) 1_555 14_655 ?
F1 Fe2 F2 89.4(2) 5_666 1_555 ?
F1 Fe2 F2 90.6(3) 5_666 5_666 ?
F1 Fe2 F2 90.6(3) 5_666 10_566 ?
F1 Fe2 F2 89.4(2) 5_666 14_655 ?
F2 Fe2 F2 180.0(3) 1_555 5_666 ?
F2 Fe2 F2 90.1(2) 1_555 10_566 ?
F2 Fe2 F2 89.9(3) 1_555 14_655 ?
F2 Fe2 F2 89.9(3) 5_666 10_566 ?
F2 Fe2 F2 90.1(2) 5_666 14_655 ?
F2 Fe2 F2 180.0(3) 10_566 14_655 ?
Ga2 F1 Ga2 142.47(10) 1_555 4_665 ?
Ga2 F1 Fe2 142.47(10) 1_555 4_665 ?
Ga2 F1 F2 105.4(2) 1_555 4_665 ?
Ga2 F1 F2 150.0(2) 1_555 8_556 ?
Ga2 F1 F2 150.0(2) 1_555 11_656 ?
Ga2 F1 F2 105.4(2) 1_555 15_565 ?
Ga2 F1 N2 108.8(4) 1_555 2_465 ?
Ga2 F1 Fe2 142.47(10) 4_665 1_555 ?
Ga2 F1 F2 105.4(2) 4_665 1_555 ?
Ga2 F1 F2 150.0(2) 4_665 5_666 ?
Ga2 F1 F2 150.0(2) 4_665 10_566 ?
Ga2 F1 F2 105.4(2) 4_665 14_655 ?
Ga2 F1 N2 108.8(4) 4_665 2_465 ?
Fe2 F1 Fe2 142.47(10) 1_555 4_665 ?
Fe2 F1 F2 105.4(2) 1_555 4_665 ?
Fe2 F1 F2 150.0(2) 1_555 8_556 ?
Fe2 F1 F2 150.0(2) 1_555 11_656 ?
Fe2 F1 F2 105.4(2) 1_555 15_565 ?
Fe2 F1 N2 108.8(4) 1_555 2_465 ?
Fe2 F1 F2 105.4(2) 4_665 1_555 ?
Fe2 F1 F2 150.0(2) 4_665 5_666 ?
Fe2 F1 F2 150.0(2) 4_665 10_566 ?
Fe2 F1 F2 105.4(2) 4_665 14_655 ?
Fe2 F1 N2 108.8(4) 4_665 2_465 ?
F2 F1 F2 91.4(2) 1_555 4_665 ?
F2 F1 F2 89.2(2) 1_555 5_666 ?
F2 F1 F2 110.9(2) 1_555 8_556 ?
F2 F1 F2 59.60(18) 1_555 10_566 ?
F2 F1 F2 148.0(3) 1_555 11_656 ?
F2 F1 F2 59.1(2) 1_555 14_655 ?
F2 F1 F2 62.5(2) 1_555 15_565 ?
F2 F1 N2 134.3(4) 1_555 2_465 ?
F2 F1 F2 110.9(2) 4_665 5_666 ?
F2 F1 F2 89.2(2) 4_665 8_556 ?
F2 F1 F2 148.0(3) 4_665 10_566 ?
F2 F1 F2 59.60(18) 4_665 11_656 ?
F2 F1 F2 62.5(2) 4_665 14_655 ?
F2 F1 F2 59.1(2) 4_665 15_565 ?
F2 F1 N2 134.3(4) 4_665 2_465 ?
F2 F1 F2 151.6(2) 5_666 8_556 ?
F2 F1 F2 59.80(16) 5_666 10_566 ?
F2 F1 F2 112.5(2) 5_666 11_656 ?
F2 F1 F2 59.60(18) 5_666 14_655 ?
F2 F1 F2 148.0(3) 5_666 15_565 ?
F2 F1 N2 75.8(3) 5_666 2_465 ?
F2 F1 F2 112.5(2) 8_556 10_566 ?
F2 F1 F2 59.80(16) 8_556 11_656 ?
F2 F1 F2 148.0(3) 8_556 14_655 ?
F2 F1 F2 59.60(18) 8_556 15_565 ?
F2 F1 N2 75.8(3) 8_556 2_465 ?
F2 F1 F2 151.6(2) 10_566 11_656 ?
F2 F1 F2 89.2(2) 10_566 14_655 ?
F2 F1 F2 110.9(2) 10_566 15_565 ?
F2 F1 N2 75.8(3) 10_566 2_465 ?
F2 F1 F2 110.9(2) 11_656 14_655 ?
F2 F1 F2 89.2(2) 11_656 15_565 ?
F2 F1 N2 75.8(3) 11_656 2_465 ?
F2 F1 F2 91.4(2) 14_655 15_565 ?
F2 F1 N2 134.3(4) 14_655 2_465 ?
F2 F1 N2 134.3(4) 15_565 2_465 ?
Fe1 F2 Ga2 146.25(14) 1_555 1_555 ?
Fe1 F2 Fe2 146.25(14) 1_555 1_555 ?
Fe1 F2 F1 102.6(3) 1_555 1_555 ?
Fe1 F2 F1 162.42(19) 1_555 5_666 ?
Fe1 F2 F2 46.02(15) 1_555 3_656 ?
Fe1 F2 F2 136.21(20) 1_555 10_566 ?
Fe1 F2 F2 117.0(2) 1_555 14_655 ?
Fe1 F2 N1 50.0(2) 1_555 1_555 ?
Fe1 F2 N1 46.3(2) 1_555 3_656 ?
Fe1 F2 N2 109.16(18) 1_555 6_645 ?
Fe1 F2 C1 70.0(3) 1_555 1_555 ?
Fe1 F2 C1 110.2(3) 1_555 8_546 ?
Ga2 F2 F1 45.11(17) 1_555 1_555 ?
Ga2 F2 F1 45.69(14) 1_555 5_666 ?
Ga2 F2 F2 166.2(2) 1_555 3_656 ?
Ga2 F2 F2 45.06(16) 1_555 14_655 ?
Ga2 F2 F2 102.6(2) 1_555 15_565 ?
Ga2 F2 N1 125.6(3) 1_555 1_555 ?
Ga2 F2 N1 121.9(3) 1_555 3_656 ?
Ga2 F2 N2 89.9(3) 1_555 6_645 ?
Ga2 F2 C1 101.5(4) 1_555 1_555 ?
Ga2 F2 C1 97.8(3) 1_555 8_546 ?
Fe2 F2 F1 45.11(17) 1_555 1_555 ?
Fe2 F2 F1 45.69(14) 1_555 5_666 ?
Fe2 F2 F2 166.2(2) 1_555 3_656 ?
Fe2 F2 F2 45.06(16) 1_555 14_655 ?
Fe2 F2 F2 102.6(2) 1_555 15_565 ?
Fe2 F2 N1 125.6(3) 1_555 1_555 ?
Fe2 F2 N1 121.9(3) 1_555 3_656 ?
Fe2 F2 N2 89.9(3) 1_555 6_645 ?
Fe2 F2 C1 101.5(4) 1_555 1_555 ?
Fe2 F2 C1 97.8(3) 1_555 8_546 ?
F1 F2 F1 90.80(18) 1_555 5_666 ?
F1 F2 F2 148.3(3) 1_555 3_656 ?
F1 F2 F2 59.69(18) 1_555 10_566 ?
F1 F2 F2 60.4(2) 1_555 14_655 ?
F1 F2 F2 58.8(2) 1_555 15_565 ?
F1 F2 N1 91.9(3) 1_555 1_555 ?
F1 F2 N1 104.6(4) 1_555 3_656 ?
F1 F2 N2 126.1(3) 1_555 6_645 ?
F1 F2 C1 72.6(3) 1_555 1_555 ?
F1 F2 C1 120.7(3) 1_555 8_546 ?
F1 F2 F2 120.7(2) 5_666 3_656 ?
F1 F2 F2 60.70(18) 5_666 10_566 ?
F1 F2 F2 60.10(16) 5_666 14_655 ?
F1 F2 F2 146.3(2) 5_666 15_565 ?
F1 F2 N1 142.1(3) 5_666 1_555 ?
F1 F2 N1 119.5(3) 5_666 3_656 ?
F1 F2 N2 53.3(3) 5_666 6_645 ?
F1 F2 C1 125.7(3) 5_666 1_555 ?
F1 F2 C1 71.2(3) 5_666 8_546 ?
F2 F2 F2 136.1(2) 3_656 10_566 ?
F2 F2 F2 130.8(2) 3_656 14_655 ?
F2 F2 F2 90.00(20) 3_656 15_565 ?
F2 F2 N1 65.5(2) 3_656 1_555 ?
F2 F2 N1 59.3(2) 3_656 3_656 ?
F2 F2 N2 77.47(17) 3_656 6_645 ?
F2 F2 C1 89.1(3) 3_656 1_555 ?
F2 F2 C1 76.5(3) 3_656 8_546 ?
F2 F2 F2 90.00(20) 10_566 14_655 ?
F2 F2 F2 108.0(2) 10_566 15_565 ?
F2 F2 N1 88.6(3) 10_566 1_555 ?
F2 F2 N1 163.8(3) 10_566 3_656 ?
F2 F2 N2 113.3(3) 10_566 6_645 ?
F2 F2 C1 66.5(2) 10_566 1_555 ?
F2 F2 C1 62.3(2) 10_566 8_546 ?
F2 F2 F2 90.0(2) 14_655 15_565 ?
F2 F2 N1 148.1(4) 14_655 1_555 ?
F2 F2 N1 77.7(3) 14_655 3_656 ?
F2 F2 N2 66.5(2) 14_655 6_645 ?
F2 F2 C1 133.0(4) 14_655 1_555 ?
F2 F2 C1 131.2(4) 14_655 8_546 ?
F2 F2 N1 60.4(2) 15_565 1_555 ?
F2 F2 N1 62.1(2) 15_565 3_656 ?
F2 F2 N2 131.7(2) 15_565 6_645 ?
F2 F2 C1 62.6(3) 15_565 1_555 ?
F2 F2 C1 134.9(2) 15_565 8_546 ?
N1 F2 N1 96.3(4) 1_555 3_656 ?
N1 F2 N2 141.7(3) 1_555 6_645 ?
N1 F2 C1 75.04(20) 1_555 8_546 ?
N1 F2 N2 71.61(18) 3_656 6_645 ?
N1 F2 C1 114.7(4) 3_656 1_555 ?
N1 F2 C1 133.9(4) 3_656 8_546 ?
N2 F2 C1 159.5(4) 6_645 1_555 ?
N2 F2 C1 87.5(3) 6_645 8_546 ?
C1 F2 C1 74.3(2) 1_555 8_546 ?
Fe1 N1 Fe1 106.5(2) 1_555 2_566 ?
Fe1 N1 N1 134.5(6) 1_555 4_765 ?
Fe1 N1 N2 155.0(5) 1_555 1_555 ?
Fe1 N1 C1 120.0(9) 1_555 1_555 ?
Fe1 N1 C1 169.4(6) 1_555 4_765 ?
Fe1 N1 F2 131.5(2) 2_566 1_555 ?
Fe1 N1 F2 77.6(2) 2_566 3_656 ?
Fe1 N1 F2 77.6(2) 2_566 13_666 ?
Fe1 N1 F2 131.5(2) 2_566 15_565 ?
Fe1 N1 N2 98.5(4) 2_566 1_555 ?
Fe1 N1 C1 133.5(8) 2_566 1_555 ?
Fe1 N1 C1 63.0(4) 2_566 4_765 ?
F2 N1 F2 55.1(2) 1_555 3_656 ?
F2 N1 F2 83.7(2) 1_555 13_666 ?
F2 N1 F2 59.3(2) 1_555 15_565 ?
F2 N1 N1 148.1(6) 1_555 4_765 ?
F2 N1 N2 117.3(4) 1_555 1_555 ?
F2 N1 C1 87.3(7) 1_555 1_555 ?
F2 N1 C1 143.4(5) 1_555 4_765 ?
F2 N1 F2 55.7(2) 3_656 13_666 ?
F2 N1 F2 83.7(2) 3_656 15_565 ?
F2 N1 N1 102.3(6) 3_656 4_765 ?
F2 N1 N2 151.6(5) 3_656 1_555 ?
F2 N1 C1 140.3(8) 3_656 1_555 ?
F2 N1 C1 131.8(5) 3_656 4_765 ?
F2 N1 F2 55.1(2) 13_666 15_565 ?
F2 N1 N1 102.3(6) 13_666 4_765 ?
F2 N1 N2 151.6(5) 13_666 1_555 ?
F2 N1 C1 140.3(8) 13_666 1_555 ?
F2 N1 C1 131.8(5) 13_666 4_765 ?
F2 N1 N1 148.1(6) 15_565 4_765 ?
F2 N1 N2 117.3(4) 15_565 1_555 ?
F2 N1 C1 87.3(7) 15_565 1_555 ?
F2 N1 C1 143.4(5) 15_565 4_765 ?
N1 N1 N2 70.5(7) 4_765 1_555 ?
N1 N1 C1 105.5(11) 4_765 1_555 ?
C1 N1 C1 70.5(9) 1_555 4_765 ?
F1 N2 F2 50.9(3) 2_565 6_654 ?
F1 N2 F2 50.9(3) 2_565 7_564 ?
F1 N2 F2 50.9(3) 2_565 9_554 ?
F1 N2 F2 50.9(3) 2_565 12_664 ?
F1 N2 N1 160.5(6) 2_565 1_555 ?
F1 N2 N1 160.5(6) 2_565 4_765 ?
F1 N2 C1 126.3(9) 2_565 1_555 ?
F1 N2 C1 126.3(9) 2_565 4_765 ?
F2 N2 F2 101.8(2) 6_654 7_564 ?
F2 N2 F2 47.02(18) 6_654 9_554 ?
F2 N2 F2 83.45(20) 6_654 12_664 ?
F2 N2 N1 117.5(4) 6_654 1_555 ?
F2 N2 N1 136.7(4) 6_654 4_765 ?
F2 N2 C1 93.0(7) 6_654 1_555 ?
F2 N2 C1 134.0(7) 6_654 4_765 ?
F2 N2 F2 83.45(20) 7_564 9_554 ?
F2 N2 F2 47.02(18) 7_564 12_664 ?
F2 N2 N1 136.7(4) 7_564 1_555 ?
F2 N2 N1 117.5(4) 7_564 4_765 ?
F2 N2 C1 134.0(7) 7_564 1_555 ?
F2 N2 C1 93.0(7) 7_564 4_765 ?
F2 N2 F2 101.8(2) 9_554 12_664 ?
F2 N2 N1 136.7(4) 9_554 1_555 ?
F2 N2 N1 117.5(4) 9_554 4_765 ?
F2 N2 C1 134.0(7) 9_554 1_555 ?
F2 N2 C1 93.0(7) 9_554 4_765 ?
F2 N2 N1 117.5(4) 12_664 1_555 ?
F2 N2 N1 136.7(4) 12_664 4_765 ?
F2 N2 C1 93.0(7) 12_664 1_555 ?
F2 N2 C1 134.0(7) 12_664 4_765 ?
N1 N2 C1 73.2(8) 1_555 4_765 ?
N1 N2 C1 73.2(8) 4_765 1_555 ?
C1 N2 C1 107.3(11) 1_555 4_765 ?
Fe1 C1 F2 88.6(2) 1_555 8_556 ?
Fe1 C1 F2 88.6(2) 1_555 10_566 ?
Fe1 C1 N1 78.5(4) 1_555 4_765 ?
Fe1 C1 N2 149.7(7) 1_555 1_555 ?
Fe1 C1 C1 113.4(5) 1_555 4_765 ?
F2 C1 F2 91.3(2) 1_555 8_556 ?
F2 C1 F2 51.1(2) 1_555 10_566 ?
F2 C1 F2 54.9(3) 1_555 15_565 ?
F2 C1 N1 68.6(7) 1_555 1_555 ?
F2 C1 N1 103.5(5) 1_555 4_765 ?
F2 C1 N2 152.37(13) 1_555 1_555 ?
F2 C1 C1 133.0(6) 1_555 4_765 ?
F2 C1 F2 89.9(2) 8_556 10_566 ?
F2 C1 F2 51.1(2) 8_556 15_565 ?
F2 C1 N1 115.2(7) 8_556 1_555 ?
F2 C1 N1 133.5(5) 8_556 4_765 ?
F2 C1 N2 112.1(5) 8_556 1_555 ?
F2 C1 C1 131.2(5) 8_556 4_765 ?
F2 C1 F2 91.3(2) 10_566 15_565 ?
F2 C1 N1 115.2(7) 10_566 1_555 ?
F2 C1 N1 133.5(5) 10_566 4_765 ?
F2 C1 N2 112.1(5) 10_566 1_555 ?
F2 C1 C1 131.2(5) 10_566 4_765 ?
F2 C1 N1 68.6(7) 15_565 1_555 ?
F2 C1 N1 103.5(5) 15_565 4_765 ?
F2 C1 N2 152.4(6) 15_565 1_555 ?
F2 C1 C1 133.0(6) 15_565 4_765 ?
N1 C1 N2 110.9(11) 1_555 1_555 ?
N1 C1 C1 74.5(9) 1_555 4_765 ?
N1 C1 N2 71.3(8) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Fe2F5Htaz
_database_code_depnum_ccdc_archive 'CCDC 1527832'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 F5 Fe2 N3'
_chemical_formula_weight         272.75
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Fe Fe 0.346 0.844 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.1583(3)
_cell_length_b                   7.4912(2)
_cell_length_c                   9.4607(3)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     649.06(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5582
_pd_meas_2theta_range_min        5.11700
_pd_meas_2theta_range_max        99.99400
_pd_meas_2theta_range_inc        0.017001

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.7216
_pd_proc_ls_prof_wR_factor       0.9176
_pd_proc_ls_prof_wR_expected     0.9264

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       19.0754
_pd_proc_ls_prof_cwR_factor      8.5043
_pd_proc_ls_prof_cwR_expected    8.5860

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            0.9811
_pd_proc_ls_prof_echi2           1.0152
_refine_ls_goodness_of_fit_all   0.9905

#  Items related to LS refinement

_refine_ls_R_I_factor            4.8167
_refine_ls_number_reflns         418
_refine_ls_number_parameters     44
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        4.9918
_pd_proc_2theta_range_max        99.8688
_pd_proc_2theta_range_inc        0.017001
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Fe1 0.75000 0.75000 0.75000 0.0223(9) 1.00000 Uiso Fe
Fe2 0.50000 0.50000 0.50000 0.0164(10) 1.00000 Uiso Fe
F1 0.50000 0.75000 0.4291(5) 0.0194(11) 1.00000 Uiso F
F2 0.6473(3) 0.5507(4) 0.6363(2) 0.0194(11) 1.00000 Uiso F
N1 0.9256(6) 0.75000 0.5778(6) 0.01267 1.00000 Uiso N
N2 1.00000 0.75000 0.3671(7) 0.01267 1.00000 Uiso N
C1 0.8800(7) 0.75000 0.4540(7) 0.01267 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 F2 2.067(3) 1_555 ?
Fe1 F2 2.067(3) 3_656 ?
Fe1 F2 2.067(3) 13_666 ?
Fe1 F2 2.067(3) 15_565 ?
Fe1 N1 2.289(6) 1_555 ?
Fe1 N1 3.388(6) 2_466 ?
Fe1 N1 2.289(6) 3_656 ?
Fe1 N1 3.388(6) 4_765 ?
Fe1 C1 3.043(7) 1_555 ?
Fe1 C1 3.043(7) 3_656 ?
Fe2 F1 1.9893(16) 1_555 ?
Fe2 F1 1.9893(16) 5_666 ?
Fe2 F2 1.904(2) 1_555 ?
Fe2 F2 1.904(2) 5_666 ?
Fe2 F2 1.904(2) 10_566 ?
Fe2 F2 1.904(2) 14_655 ?
F1 Fe2 1.9893(16) 1_555 ?
F1 Fe2 1.9893(16) 4_665 ?
F1 F2 2.809(4) 1_555 ?
F1 F2 2.809(4) 4_665 ?
F1 F2 2.698(3) 5_666 ?
F1 F2 2.698(3) 8_556 ?
F1 F2 2.698(3) 10_566 ?
F1 F2 2.698(3) 11_656 ?
F1 F2 2.809(4) 14_655 ?
F1 F2 2.809(4) 15_565 ?
F1 N2 2.802(8) 2_465 ?
F1 C1 3.488(6) 1_555 ?
F1 C1 3.488(6) 4_665 ?
F2 Fe1 2.067(3) 1_555 ?
F2 Fe2 1.904(2) 1_555 ?
F2 F1 2.809(4) 1_555 ?
F2 F1 2.698(3) 5_666 ?
F2 F2 2.858(3) 3_656 ?
F2 F2 2.689(3) 10_566 ?
F2 F2 2.698(4) 14_655 ?
F2 F2 2.986(4) 15_565 ?
F2 N1 3.005(6) 1_555 ?
F2 N1 3.161(5) 3_656 ?
F2 N2 3.415(5) 6_645 ?
F2 C1 3.122(6) 1_555 ?
F2 C1 3.216(5) 8_546 ?
N1 Fe1 2.289(6) 1_555 ?
N1 Fe1 3.388(6) 2_566 ?
N1 F2 3.005(6) 1_555 ?
N1 F2 3.161(5) 3_656 ?
N1 F2 3.161(5) 13_666 ?
N1 F2 3.005(6) 15_565 ?
N1 N1 1.363(8) 4_765 ?
N1 N2 2.107(8) 1_555 ?
N1 C1 1.243(9) 1_555 ?
N1 C1 2.131(9) 4_765 ?
N2 F1 2.802(8) 2_565 ?
N2 F2 3.415(5) 6_654 ?
N2 F2 3.415(5) 7_564 ?
N2 F2 3.415(5) 9_554 ?
N2 F2 3.415(5) 12_664 ?
N2 N1 2.107(8) 1_555 ?
N2 N1 2.107(8) 4_765 ?
N2 C1 1.372(8) 1_555 ?
N2 C1 1.372(8) 4_765 ?
C1 Fe1 3.043(7) 1_555 ?
C1 F1 3.488(6) 1_555 ?
C1 F2 3.122(6) 1_555 ?
C1 F2 3.216(5) 8_556 ?
C1 F2 3.216(5) 10_566 ?
C1 F2 3.122(6) 15_565 ?
C1 N1 1.243(9) 1_555 ?
C1 N1 2.131(9) 4_765 ?
C1 N2 1.372(8) 1_555 ?
C1 C1 2.198(9) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Fe1 F2 87.49(16) 1_555 3_656 ?
F2 Fe1 F2 180.0(2) 1_555 13_666 ?
F2 Fe1 F2 92.51(20) 1_555 15_565 ?
F2 Fe1 N1 87.09(12) 1_555 1_555 ?
F2 Fe1 N1 81.4(2) 1_555 2_466 ?
F2 Fe1 N1 92.9(3) 1_555 3_656 ?
F2 Fe1 N1 98.6(2) 1_555 4_765 ?
F2 Fe1 C1 72.5(2) 1_555 1_555 ?
F2 Fe1 C1 107.5(3) 1_555 3_656 ?
F2 Fe1 F2 92.51(20) 3_656 13_666 ?
F2 Fe1 F2 180.0(2) 3_656 15_565 ?
F2 Fe1 N1 92.9(3) 3_656 1_555 ?
F2 Fe1 N1 98.6(2) 3_656 2_466 ?
F2 Fe1 N1 87.1(3) 3_656 3_656 ?
F2 Fe1 N1 81.4(2) 3_656 4_765 ?
F2 Fe1 C1 107.5(3) 3_656 1_555 ?
F2 Fe1 C1 72.5(2) 3_656 3_656 ?
F2 Fe1 F2 87.49(16) 13_666 15_565 ?
F2 Fe1 N1 92.9(3) 13_666 1_555 ?
F2 Fe1 N1 98.6(2) 13_666 2_466 ?
F2 Fe1 N1 87.1(3) 13_666 3_656 ?
F2 Fe1 N1 81.4(2) 13_666 4_765 ?
F2 Fe1 C1 107.5(3) 13_666 1_555 ?
F2 Fe1 C1 72.5(2) 13_666 3_656 ?
F2 Fe1 N1 87.1(3) 15_565 1_555 ?
F2 Fe1 N1 81.4(2) 15_565 2_466 ?
F2 Fe1 N1 92.9(3) 15_565 3_656 ?
F2 Fe1 N1 98.6(2) 15_565 4_765 ?
F2 Fe1 C1 72.5(2) 15_565 1_555 ?
F2 Fe1 C1 107.5(3) 15_565 3_656 ?
N1 Fe1 N1 163.4(4) 1_555 2_466 ?
N1 Fe1 N1 180.0(4) 1_555 3_656 ?
N1 Fe1 C1 158.4(4) 1_555 3_656 ?
N1 Fe1 N1 180.0(3) 2_466 4_765 ?
N1 Fe1 C1 141.8(3) 2_466 1_555 ?
N1 Fe1 N1 163.4(4) 3_656 4_765 ?
N1 Fe1 C1 158.4(4) 3_656 1_555 ?
N1 Fe1 C1 141.8(3) 4_765 3_656 ?
C1 Fe1 C1 180.0(4) 1_555 3_656 ?
F1 Fe2 F1 179.97(15) 1_555 5_666 ?
F1 Fe2 F2 92.32(19) 1_555 1_555 ?
F1 Fe2 F2 87.68(15) 1_555 5_666 ?
F1 Fe2 F2 87.68(15) 1_555 10_566 ?
F1 Fe2 F2 92.32(19) 1_555 14_655 ?
F1 Fe2 F2 87.68(15) 5_666 1_555 ?
F1 Fe2 F2 92.32(19) 5_666 5_666 ?
F1 Fe2 F2 92.32(19) 5_666 10_566 ?
F1 Fe2 F2 87.68(15) 5_666 14_655 ?
F2 Fe2 F2 180.0(2) 1_555 5_666 ?
F2 Fe2 F2 89.80(16) 1_555 10_566 ?
F2 Fe2 F2 90.20(19) 1_555 14_655 ?
F2 Fe2 F2 90.20(19) 5_666 10_566 ?
F2 Fe2 F2 89.80(16) 5_666 14_655 ?
F2 Fe2 F2 180.0(2) 10_566 14_655 ?
Fe2 F1 Fe2 140.59(7) 1_555 4_665 ?
Fe2 F1 F2 105.37(15) 1_555 4_665 ?
Fe2 F1 F2 149.71(16) 1_555 8_556 ?
Fe2 F1 F2 149.71(16) 1_555 11_656 ?
Fe2 F1 F2 105.37(15) 1_555 15_565 ?
Fe2 F1 N2 109.7(3) 1_555 2_465 ?
Fe2 F1 C1 88.70(5) 1_555 1_555 ?
Fe2 F1 C1 88.7(2) 1_555 4_665 ?
Fe2 F1 F2 105.37(15) 4_665 1_555 ?
Fe2 F1 F2 149.71(16) 4_665 5_666 ?
Fe2 F1 F2 149.71(16) 4_665 10_566 ?
Fe2 F1 F2 105.37(15) 4_665 14_655 ?
Fe2 F1 N2 109.7(3) 4_665 2_465 ?
Fe2 F1 C1 88.7(2) 4_665 1_555 ?
Fe2 F1 C1 88.7(2) 4_665 4_665 ?
F2 F1 F2 91.50(17) 1_555 4_665 ?
F2 F1 F2 87.50(14) 1_555 5_666 ?
F2 F1 F2 111.33(17) 1_555 8_556 ?
F2 F1 F2 58.41(12) 1_555 10_566 ?
F2 F1 F2 147.57(19) 1_555 11_656 ?
F2 F1 F2 57.40(14) 1_555 14_655 ?
F2 F1 F2 64.21(15) 1_555 15_565 ?
F2 F1 N2 134.3(3) 1_555 2_465 ?
F2 F1 C1 58.25(18) 1_555 1_555 ?
F2 F1 C1 115.6(2) 1_555 4_665 ?
F2 F1 F2 111.33(17) 4_665 5_666 ?
F2 F1 F2 87.50(14) 4_665 8_556 ?
F2 F1 F2 147.57(19) 4_665 10_566 ?
F2 F1 F2 58.41(12) 4_665 11_656 ?
F2 F1 F2 64.21(15) 4_665 14_655 ?
F2 F1 F2 57.40(14) 4_665 15_565 ?
F2 F1 N2 134.3(3) 4_665 2_465 ?
F2 F1 C1 115.6(2) 4_665 1_555 ?
F2 F1 C1 58.25(18) 4_665 4_665 ?
F2 F1 F2 153.48(19) 5_666 8_556 ?
F2 F1 F2 60.01(12) 5_666 10_566 ?
F2 F1 F2 113.24(18) 5_666 11_656 ?
F2 F1 F2 58.41(12) 5_666 14_655 ?
F2 F1 F2 147.57(19) 5_666 15_565 ?
F2 F1 N2 76.7(2) 5_666 2_465 ?
F2 F1 C1 121.0(2) 5_666 1_555 ?
F2 F1 C1 61.09(16) 5_666 4_665 ?
F2 F1 F2 113.24(18) 8_556 10_566 ?
F2 F1 F2 60.01(12) 8_556 11_656 ?
F2 F1 F2 147.57(19) 8_556 14_655 ?
F2 F1 F2 58.41(12) 8_556 15_565 ?
F2 F1 N2 76.7(2) 8_556 2_465 ?
F2 F1 C1 61.09(16) 8_556 1_555 ?
F2 F1 C1 121.0(2) 8_556 4_665 ?
F2 F1 F2 153.48(19) 10_566 11_656 ?
F2 F1 F2 87.50(14) 10_566 14_655 ?
F2 F1 F2 111.33(17) 10_566 15_565 ?
F2 F1 N2 76.7(2) 10_566 2_465 ?
F2 F1 C1 61.09(16) 10_566 1_555 ?
F2 F1 C1 121.0(2) 10_566 4_665 ?
F2 F1 F2 111.33(17) 11_656 14_655 ?
F2 F1 F2 87.50(14) 11_656 15_565 ?
F2 F1 N2 76.7(2) 11_656 2_465 ?
F2 F1 C1 121.0(2) 11_656 1_555 ?
F2 F1 C1 61.09(16) 11_656 4_665 ?
F2 F1 F2 91.50(17) 14_655 15_565 ?
F2 F1 N2 134.3(3) 14_655 2_465 ?
F2 F1 C1 115.6(2) 14_655 1_555 ?
F2 F1 C1 58.25(18) 14_655 4_665 ?
F2 F1 N2 134.3(3) 15_565 2_465 ?
F2 F1 C1 58.25(18) 15_565 1_555 ?
F2 F1 C1 115.6(2) 15_565 4_665 ?
N2 F1 C1 93.9(3) 2_465 1_555 ?
N2 F1 C1 93.9(3) 2_465 4_665 ?
C1 F1 C1 172.3(3) 1_555 4_665 ?
Fe1 F2 Fe2 144.98(10) 1_555 1_555 ?
Fe1 F2 F1 101.41(18) 1_555 1_555 ?
Fe1 F2 F1 161.85(13) 1_555 5_666 ?
Fe1 F2 F2 46.26(11) 1_555 3_656 ?
Fe1 F2 F2 134.70(14) 1_555 10_566 ?
Fe1 F2 F2 117.07(16) 1_555 14_655 ?
Fe1 F2 N1 49.53(17) 1_555 1_555 ?
Fe1 F2 N1 46.33(17) 1_555 3_656 ?
Fe1 F2 N2 108.88(13) 1_555 6_645 ?
Fe1 F2 C1 68.4(2) 1_555 1_555 ?
Fe1 F2 C1 110.04(18) 1_555 8_546 ?
Fe2 F2 F1 45.04(12) 1_555 1_555 ?
Fe2 F2 F1 47.46(10) 1_555 5_666 ?
Fe2 F2 F2 167.42(15) 1_555 3_656 ?
Fe2 F2 F2 45.10(11) 1_555 10_566 ?
Fe2 F2 F2 101.50(16) 1_555 15_565 ?
Fe2 F2 N1 125.11(14) 1_555 1_555 ?
Fe2 F2 N1 121.6(3) 1_555 3_656 ?
Fe2 F2 N2 91.2(2) 1_555 6_645 ?
Fe2 F2 C1 101.82(14) 1_555 1_555 ?
Fe2 F2 C1 98.6(2) 1_555 8_546 ?
F1 F2 F1 92.50(13) 1_555 5_666 ?
F1 F2 F2 147.29(20) 1_555 3_656 ?
F1 F2 F2 58.72(12) 1_555 10_566 ?
F1 F2 F2 61.30(15) 1_555 14_655 ?
F1 F2 F2 57.90(14) 1_555 15_565 ?
F1 F2 N1 90.8(2) 1_555 1_555 ?
F1 F2 N1 104.2(3) 1_555 3_656 ?
F1 F2 N2 127.4(2) 1_555 6_645 ?
F1 F2 C1 71.8(2) 1_555 1_555 ?
F1 F2 C1 120.33(20) 1_555 8_546 ?
F1 F2 F2 120.12(16) 5_666 3_656 ?
F1 F2 F2 62.87(13) 5_666 10_566 ?
F1 F2 F2 59.99(12) 5_666 14_655 ?
F1 F2 F2 146.62(16) 5_666 15_565 ?
F1 F2 N1 142.82(20) 5_666 1_555 ?
F1 F2 N1 119.0(2) 5_666 3_656 ?
F1 F2 N2 53.01(18) 5_666 6_645 ?
F1 F2 C1 127.9(2) 5_666 1_555 ?
F1 F2 C1 71.68(19) 5_666 8_546 ?
F2 F2 F2 136.23(14) 3_656 10_566 ?
F2 F2 F2 131.17(17) 3_656 14_655 ?
F2 F2 F2 90.00(15) 3_656 15_565 ?
F2 F2 N1 65.19(17) 3_656 1_555 ?
F2 F2 N1 59.66(16) 3_656 3_656 ?
F2 F2 N2 77.21(12) 3_656 6_645 ?
F2 F2 C1 88.1(2) 3_656 1_555 ?
F2 F2 C1 76.34(18) 3_656 8_546 ?
F2 F2 F2 90.00(14) 10_566 14_655 ?
F2 F2 F2 106.41(16) 10_566 15_565 ?
F2 F2 N1 87.92(19) 10_566 1_555 ?
F2 F2 N1 162.6(2) 10_566 3_656 ?
F2 F2 N2 115.3(2) 10_566 6_645 ?
F2 F2 C1 66.74(18) 10_566 1_555 ?
F2 F2 C1 63.09(17) 10_566 8_546 ?
F2 F2 F2 90.00(16) 14_655 15_565 ?
F2 F2 N1 148.0(3) 14_655 1_555 ?
F2 F2 N1 77.81(19) 14_655 3_656 ?
F2 F2 N2 66.73(16) 14_655 6_645 ?
F2 F2 C1 133.1(3) 14_655 1_555 ?
F2 F2 C1 131.5(3) 14_655 8_546 ?
F2 F2 N1 60.21(17) 15_565 1_555 ?
F2 F2 N1 61.81(17) 15_565 3_656 ?
F2 F2 N2 131.27(17) 15_565 6_645 ?
F2 F2 C1 61.43(19) 15_565 1_555 ?
F2 F2 C1 134.45(18) 15_565 8_546 ?
N1 F2 N1 95.9(3) 1_555 3_656 ?
N1 F2 N2 141.3(2) 1_555 6_645 ?
N1 F2 C1 74.76(15) 1_555 8_546 ?
N1 F2 N2 71.40(13) 3_656 6_645 ?
N1 F2 C1 113.0(3) 3_656 1_555 ?
N1 F2 C1 134.3(3) 3_656 8_546 ?
N2 F2 C1 159.8(3) 6_645 1_555 ?
N2 F2 C1 88.3(2) 6_645 8_546 ?
C1 F2 C1 74.69(16) 1_555 8_546 ?
Fe1 N1 Fe1 105.89(17) 1_555 2_566 ?
Fe1 N1 N1 134.6(5) 1_555 4_765 ?
Fe1 N1 N2 154.2(4) 1_555 1_555 ?
Fe1 N1 C1 115.7(6) 1_555 1_555 ?
Fe1 N1 C1 168.0(4) 1_555 4_765 ?
Fe1 N1 F2 130.93(17) 2_566 1_555 ?
Fe1 N1 F2 76.92(15) 2_566 3_656 ?
Fe1 N1 F2 76.92(15) 2_566 13_666 ?
Fe1 N1 F2 130.93(17) 2_566 15_565 ?
Fe1 N1 N2 99.9(3) 2_566 1_555 ?
Fe1 N1 C1 138.4(6) 2_566 1_555 ?
Fe1 N1 C1 62.1(3) 2_566 4_765 ?
F2 N1 F2 55.15(16) 1_555 3_656 ?
F2 N1 F2 84.14(17) 1_555 13_666 ?
F2 N1 F2 59.58(17) 1_555 15_565 ?
F2 N1 N1 148.0(5) 1_555 4_765 ?
F2 N1 N2 116.7(3) 1_555 1_555 ?
F2 N1 C1 83.6(5) 1_555 1_555 ?
F2 N1 C1 144.1(4) 1_555 4_765 ?
F2 N1 F2 56.37(16) 3_656 13_666 ?
F2 N1 F2 84.14(17) 3_656 15_565 ?
F2 N1 N1 102.2(4) 3_656 4_765 ?
F2 N1 N2 151.4(4) 3_656 1_555 ?
F2 N1 C1 137.3(6) 3_656 1_555 ?
F2 N1 C1 130.3(4) 3_656 4_765 ?
F2 N1 F2 55.15(16) 13_666 15_565 ?
F2 N1 N1 102.2(4) 13_666 4_765 ?
F2 N1 N2 151.4(4) 13_666 1_555 ?
F2 N1 C1 137.3(6) 13_666 1_555 ?
F2 N1 C1 130.3(4) 13_666 4_765 ?
F2 N1 N1 148.0(5) 15_565 4_765 ?
F2 N1 N2 116.7(3) 15_565 1_555 ?
F2 N1 C1 83.6(5) 15_565 1_555 ?
F2 N1 C1 144.1(4) 15_565 4_765 ?
N1 N1 N2 71.1(5) 4_765 1_555 ?
N1 N1 C1 109.6(8) 4_765 1_555 ?
C1 N1 C1 76.3(6) 1_555 4_765 ?
F1 N2 F2 50.25(19) 2_565 6_654 ?
F1 N2 F2 50.25(19) 2_565 7_564 ?
F1 N2 F2 50.25(19) 2_565 9_554 ?
F1 N2 F2 50.25(19) 2_565 12_664 ?
F1 N2 N1 161.1(4) 2_565 1_555 ?
F1 N2 N1 161.1(4) 2_565 4_765 ?
F1 N2 C1 126.8(6) 2_565 1_555 ?
F1 N2 C1 126.8(6) 2_565 4_765 ?
F2 N2 F2 100.51(16) 6_654 7_564 ?
F2 N2 F2 46.54(13) 6_654 9_554 ?
F2 N2 F2 82.54(15) 6_654 12_664 ?
F2 N2 N1 118.5(3) 6_654 1_555 ?
F2 N2 N1 137.1(3) 6_654 4_765 ?
F2 N2 C1 93.8(4) 6_654 1_555 ?
F2 N2 C1 134.4(5) 6_654 4_765 ?
F2 N2 F2 82.54(15) 7_564 9_554 ?
F2 N2 F2 46.54(13) 7_564 12_664 ?
F2 N2 N1 137.1(3) 7_564 1_555 ?
F2 N2 N1 118.5(3) 7_564 4_765 ?
F2 N2 C1 134.4(5) 7_564 1_555 ?
F2 N2 C1 93.8(4) 7_564 4_765 ?
F2 N2 F2 100.51(16) 9_554 12_664 ?
F2 N2 N1 137.1(3) 9_554 1_555 ?
F2 N2 N1 118.5(3) 9_554 4_765 ?
F2 N2 C1 134.4(5) 9_554 1_555 ?
F2 N2 C1 93.8(4) 9_554 4_765 ?
F2 N2 N1 118.5(3) 12_664 1_555 ?
F2 N2 N1 137.1(3) 12_664 4_765 ?
F2 N2 C1 93.8(4) 12_664 1_555 ?
F2 N2 C1 134.4(5) 12_664 4_765 ?
N1 N2 C1 72.1(5) 1_555 4_765 ?
N1 N2 C1 72.1(5) 4_765 1_555 ?
C1 N2 C1 106.4(8) 1_555 4_765 ?
Fe1 C1 F1 70.84(18) 1_555 1_555 ?
Fe1 C1 F2 89.15(17) 1_555 8_556 ?
Fe1 C1 F2 89.15(17) 1_555 10_566 ?
Fe1 C1 N1 79.7(3) 1_555 4_765 ?
Fe1 C1 N2 149.8(5) 1_555 1_555 ?
Fe1 C1 C1 113.0(4) 1_555 4_765 ?
F1 C1 F2 49.92(17) 1_555 1_555 ?
F1 C1 F2 47.24(15) 1_555 8_556 ?
F1 C1 F2 47.24(15) 1_555 10_566 ?
F1 C1 F2 49.92(17) 1_555 15_565 ?
F1 C1 N1 113.5(5) 1_555 1_555 ?
F1 C1 N1 150.5(3) 1_555 4_765 ?
F1 C1 N2 139.3(3) 1_555 1_555 ?
F1 C1 C1 176.1(4) 1_555 4_765 ?
F2 C1 F2 91.68(18) 1_555 8_556 ?
F2 C1 F2 50.17(16) 1_555 10_566 ?
F2 C1 F2 57.14(18) 1_555 15_565 ?
F2 C1 N1 73.1(5) 1_555 1_555 ?
F2 C1 N1 105.5(3) 1_555 4_765 ?
F2 C1 N2 151.35(8) 1_555 1_555 ?
F2 C1 C1 133.1(4) 1_555 4_765 ?
F2 C1 F2 88.91(17) 8_556 10_566 ?
F2 C1 F2 50.17(16) 8_556 15_565 ?
F2 C1 N1 118.2(5) 8_556 1_555 ?
F2 C1 N1 134.4(3) 8_556 4_765 ?
F2 C1 N2 111.8(4) 8_556 1_555 ?
F2 C1 C1 131.5(4) 8_556 4_765 ?
F2 C1 F2 91.68(18) 10_566 15_565 ?
F2 C1 N1 118.2(5) 10_566 1_555 ?
F2 C1 N1 134.4(3) 10_566 4_765 ?
F2 C1 N2 111.8(4) 10_566 1_555 ?
F2 C1 C1 131.5(4) 10_566 4_765 ?
F2 C1 N1 73.1(5) 15_565 1_555 ?
F2 C1 N1 105.5(3) 15_565 4_765 ?
F2 C1 N2 151.4(4) 15_565 1_555 ?
F2 C1 C1 133.1(4) 15_565 4_765 ?
N1 C1 N2 107.2(8) 1_555 1_555 ?
N1 C1 C1 70.4(6) 1_555 4_765 ?
N1 C1 N2 70.1(5) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_MnFeF5Htaz_1
_database_code_depnum_ccdc_archive 'CCDC 1527829'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 F5 Fe1.17 Mn0.83 N3'
_chemical_formula_weight         271.99
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mn Mn 0.337 0.728 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.346 0.844 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.2723(3)
_cell_length_b                   7.5057(2)
_cell_length_c                   9.5831(3)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     666.93(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5582
_pd_meas_2theta_range_min        5.11700
_pd_meas_2theta_range_max        99.99400
_pd_meas_2theta_range_inc        0.017001

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.9659
_pd_proc_ls_prof_wR_factor       1.2667
_pd_proc_ls_prof_wR_expected     1.0743

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       15.8470
_pd_proc_ls_prof_cwR_factor      8.5072
_pd_proc_ls_prof_cwR_expected    7.2147

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            1.3904
_pd_proc_ls_prof_echi2           1.4682
_refine_ls_goodness_of_fit_all   1.1791

#  Items related to LS refinement

_refine_ls_R_I_factor            4.6888
_refine_ls_number_reflns         440
_refine_ls_number_parameters     60
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        5.1537
_pd_proc_2theta_range_max        100.0307
_pd_proc_2theta_range_inc        0.017001
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Mn1 0.75000 0.75000 0.75000 0.0159(8) 0.83000 Uiso Mn
Fe1 0.75000 0.75000 0.75000 0.0159(8) 0.17000 Uiso Fe
Fe2 0.50000 0.50000 0.50000 0.0130(9) 1.00000 Uiso Fe
F1 0.50000 0.75000 0.4264(5) 0.0221(12) 1.00000 Uiso F
F2 0.6462(2) 0.5512(3) 0.6338(2) 0.0221(12) 1.00000 Uiso F
N1 0.9286(5) 0.75000 0.5729(5) 0.01267 1.00000 Uiso N
N2 1.00000 0.75000 0.3614(7) 0.01267 1.00000 Uiso N
C1 0.8862(7) 0.75000 0.4492(7) 0.01267 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mn1 F2 2.096(2) 1_555 ?
Mn1 F2 2.096(2) 3_656 ?
Mn1 F2 2.096(2) 13_666 ?
Mn1 F2 2.096(2) 15_565 ?
Mn1 N1 2.371(5) 1_555 ?
Mn1 N1 3.430(5) 2_466 ?
Mn1 N1 2.371(5) 3_656 ?
Mn1 N1 3.430(5) 4_765 ?
Mn1 C1 3.147(7) 1_555 ?
Mn1 C1 3.147(7) 3_656 ?
Fe1 F2 2.096(2) 1_555 ?
Fe1 F2 2.096(2) 3_656 ?
Fe1 F2 2.096(2) 13_666 ?
Fe1 F2 2.096(2) 15_565 ?
Fe1 N1 2.371(5) 1_555 ?
Fe1 N1 3.430(5) 2_466 ?
Fe1 N1 2.371(5) 3_656 ?
Fe1 N1 3.430(5) 4_765 ?
Fe1 C1 3.147(7) 1_555 ?
Fe1 C1 3.147(7) 3_656 ?
Fe2 F1 2.0046(17) 1_555 ?
Fe2 F1 2.0046(17) 5_666 ?
Fe2 F2 1.9051(19) 1_555 ?
Fe2 F2 1.9051(19) 5_666 ?
Fe2 F2 1.9051(19) 10_566 ?
Fe2 F2 1.9051(19) 14_655 ?
F1 Fe2 2.0046(17) 1_555 ?
F1 Fe2 2.0046(17) 4_665 ?
F1 F2 2.831(4) 1_555 ?
F1 F2 2.831(4) 4_665 ?
F1 F2 2.698(2) 5_666 ?
F1 F2 2.698(2) 8_556 ?
F1 F2 2.698(2) 10_566 ?
F1 F2 2.698(2) 11_656 ?
F1 F2 2.831(4) 14_655 ?
F1 F2 2.831(4) 15_565 ?
F1 N2 2.758(8) 2_465 ?
F2 Mn1 2.096(2) 1_555 ?
F2 Fe1 2.096(2) 1_555 ?
F2 Fe2 1.9051(19) 1_555 ?
F2 F1 2.831(4) 1_555 ?
F2 F1 2.698(2) 5_666 ?
F2 F2 2.944(3) 3_656 ?
F2 F2 2.677(3) 10_566 ?
F2 F2 2.711(3) 14_655 ?
F2 F2 2.984(3) 15_565 ?
F2 N1 3.070(5) 1_555 ?
F2 N1 3.257(5) 3_656 ?
F2 N2 3.421(5) 6_645 ?
F2 C1 3.211(6) 1_555 ?
F2 C1 3.270(5) 8_546 ?
N1 Mn1 2.371(5) 1_555 ?
N1 Mn1 3.430(5) 2_566 ?
N1 Fe1 2.371(5) 1_555 ?
N1 Fe1 3.430(5) 2_566 ?
N1 F2 3.070(5) 1_555 ?
N1 F2 3.257(5) 3_656 ?
N1 F2 3.257(5) 13_666 ?
N1 F2 3.070(5) 15_565 ?
N1 N1 1.324(7) 4_765 ?
N1 N2 2.132(8) 1_555 ?
N1 C1 1.249(8) 1_555 ?
N1 C1 2.087(8) 4_765 ?
N2 F1 2.758(8) 2_565 ?
N2 F2 3.421(5) 6_654 ?
N2 F2 3.421(5) 7_564 ?
N2 F2 3.421(5) 9_554 ?
N2 F2 3.421(5) 12_664 ?
N2 N1 2.132(8) 1_555 ?
N2 N1 2.132(8) 4_765 ?
N2 C1 1.350(8) 1_555 ?
N2 C1 1.350(8) 4_765 ?
C1 Mn1 3.147(7) 1_555 ?
C1 Fe1 3.147(7) 1_555 ?
C1 F2 3.211(6) 1_555 ?
C1 F2 3.270(5) 8_556 ?
C1 F2 3.270(5) 10_566 ?
C1 F2 3.211(6) 15_565 ?
C1 N1 1.249(8) 1_555 ?
C1 N1 2.087(8) 4_765 ?
C1 N2 1.350(8) 1_555 ?
C1 C1 2.110(9) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Mn1 F2 89.22(13) 1_555 3_656 ?
F2 Mn1 F2 180.00(18) 1_555 13_666 ?
F2 Mn1 F2 90.78(15) 1_555 15_565 ?
F2 Mn1 N1 86.6(2) 1_555 1_555 ?
F2 Mn1 N1 82.18(17) 1_555 2_466 ?
F2 Mn1 N1 93.4(2) 1_555 3_656 ?
F2 Mn1 N1 97.82(19) 1_555 4_765 ?
F2 Mn1 C1 72.4(2) 1_555 1_555 ?
F2 Mn1 C1 107.6(3) 1_555 3_656 ?
F2 Mn1 F2 90.78(15) 3_656 13_666 ?
F2 Mn1 F2 180.00(18) 3_656 15_565 ?
F2 Mn1 N1 93.4(2) 3_656 1_555 ?
F2 Mn1 N1 97.82(19) 3_656 2_466 ?
F2 Mn1 N1 86.6(2) 3_656 3_656 ?
F2 Mn1 N1 82.18(17) 3_656 4_765 ?
F2 Mn1 C1 107.6(3) 3_656 1_555 ?
F2 Mn1 C1 72.4(2) 3_656 3_656 ?
F2 Mn1 F2 89.22(13) 13_666 15_565 ?
F2 Mn1 N1 93.4(2) 13_666 1_555 ?
F2 Mn1 N1 97.82(19) 13_666 2_466 ?
F2 Mn1 N1 86.6(2) 13_666 3_656 ?
F2 Mn1 N1 82.18(17) 13_666 4_765 ?
F2 Mn1 C1 107.6(3) 13_666 1_555 ?
F2 Mn1 C1 72.4(2) 13_666 3_656 ?
F2 Mn1 N1 86.6(2) 15_565 1_555 ?
F2 Mn1 N1 82.18(17) 15_565 2_466 ?
F2 Mn1 N1 93.4(2) 15_565 3_656 ?
F2 Mn1 N1 97.82(19) 15_565 4_765 ?
F2 Mn1 C1 72.4(2) 15_565 1_555 ?
F2 Mn1 C1 107.6(3) 15_565 3_656 ?
N1 Mn1 N1 164.0(3) 1_555 2_466 ?
N1 Mn1 N1 180.0(4) 1_555 3_656 ?
N1 Mn1 C1 159.4(4) 1_555 3_656 ?
N1 Mn1 N1 180.0(2) 2_466 4_765 ?
N1 Mn1 C1 143.3(3) 2_466 1_555 ?
N1 Mn1 N1 164.0(3) 3_656 4_765 ?
N1 Mn1 C1 159.4(4) 3_656 1_555 ?
N1 Mn1 C1 143.3(3) 4_765 3_656 ?
C1 Mn1 C1 180.0(4) 1_555 3_656 ?
F2 Fe1 F2 89.22(13) 1_555 3_656 ?
F2 Fe1 F2 180.00(18) 1_555 13_666 ?
F2 Fe1 F2 90.78(15) 1_555 15_565 ?
F2 Fe1 N1 86.6(2) 1_555 1_555 ?
F2 Fe1 N1 82.18(17) 1_555 2_466 ?
F2 Fe1 N1 93.4(2) 1_555 3_656 ?
F2 Fe1 N1 97.82(19) 1_555 4_765 ?
F2 Fe1 C1 72.4(2) 1_555 1_555 ?
F2 Fe1 C1 107.6(3) 1_555 3_656 ?
F2 Fe1 F2 90.78(15) 3_656 13_666 ?
F2 Fe1 F2 180.00(18) 3_656 15_565 ?
F2 Fe1 N1 93.4(2) 3_656 1_555 ?
F2 Fe1 N1 97.82(19) 3_656 2_466 ?
F2 Fe1 N1 86.6(2) 3_656 3_656 ?
F2 Fe1 N1 82.18(17) 3_656 4_765 ?
F2 Fe1 C1 107.6(3) 3_656 1_555 ?
F2 Fe1 C1 72.4(2) 3_656 3_656 ?
F2 Fe1 F2 89.22(13) 13_666 15_565 ?
F2 Fe1 N1 93.4(2) 13_666 1_555 ?
F2 Fe1 N1 97.82(19) 13_666 2_466 ?
F2 Fe1 N1 86.6(2) 13_666 3_656 ?
F2 Fe1 N1 82.18(17) 13_666 4_765 ?
F2 Fe1 C1 107.6(3) 13_666 1_555 ?
F2 Fe1 C1 72.4(2) 13_666 3_656 ?
F2 Fe1 N1 86.6(2) 15_565 1_555 ?
F2 Fe1 N1 82.18(17) 15_565 2_466 ?
F2 Fe1 N1 93.4(2) 15_565 3_656 ?
F2 Fe1 N1 97.82(19) 15_565 4_765 ?
F2 Fe1 C1 72.4(2) 15_565 1_555 ?
F2 Fe1 C1 107.6(3) 15_565 3_656 ?
N1 Fe1 N1 164.0(3) 1_555 2_466 ?
N1 Fe1 N1 180.0(4) 1_555 3_656 ?
N1 Fe1 C1 159.4(4) 1_555 3_656 ?
N1 Fe1 N1 180.0(2) 2_466 4_765 ?
N1 Fe1 C1 143.3(3) 2_466 1_555 ?
N1 Fe1 N1 164.0(3) 3_656 4_765 ?
N1 Fe1 C1 159.4(4) 3_656 1_555 ?
N1 Fe1 C1 143.3(3) 4_765 3_656 ?
C1 Fe1 C1 180.0(4) 1_555 3_656 ?
F1 Fe2 F1 180.00(15) 1_555 5_666 ?
F1 Fe2 F2 92.75(18) 1_555 1_555 ?
F1 Fe2 F2 87.25(12) 1_555 5_666 ?
F1 Fe2 F2 87.25(12) 1_555 10_566 ?
F1 Fe2 F2 92.75(18) 1_555 14_655 ?
F1 Fe2 F2 87.25(12) 5_666 1_555 ?
F1 Fe2 F2 92.75(18) 5_666 5_666 ?
F1 Fe2 F2 92.75(18) 5_666 10_566 ?
F1 Fe2 F2 87.25(12) 5_666 14_655 ?
F2 Fe2 F2 180.00(18) 1_555 5_666 ?
F2 Fe2 F2 89.28(14) 1_555 10_566 ?
F2 Fe2 F2 90.72(14) 1_555 14_655 ?
F2 Fe2 F2 90.72(14) 5_666 10_566 ?
F2 Fe2 F2 89.28(14) 5_666 14_655 ?
F2 Fe2 F2 180.00(18) 10_566 14_655 ?
Fe2 F1 Fe2 138.80(7) 1_555 4_665 ?
Fe2 F1 F2 104.26(13) 1_555 4_665 ?
Fe2 F1 F2 149.26(13) 1_555 8_556 ?
Fe2 F1 F2 149.26(13) 1_555 11_656 ?
Fe2 F1 F2 104.26(13) 1_555 15_565 ?
Fe2 F1 N2 110.6(3) 1_555 2_465 ?
Fe2 F1 F2 104.26(13) 4_665 1_555 ?
Fe2 F1 F2 149.26(13) 4_665 5_666 ?
Fe2 F1 F2 149.26(13) 4_665 10_566 ?
Fe2 F1 F2 104.26(13) 4_665 14_655 ?
Fe2 F1 N2 110.6(3) 4_665 2_465 ?
F2 F1 F2 90.81(14) 1_555 4_665 ?
F2 F1 F2 87.08(12) 1_555 5_666 ?
F2 F1 F2 110.56(14) 1_555 8_556 ?
F2 F1 F2 57.86(11) 1_555 10_566 ?
F2 F1 F2 146.33(15) 1_555 11_656 ?
F2 F1 F2 57.22(12) 1_555 14_655 ?
F2 F1 F2 63.62(13) 1_555 15_565 ?
F2 F1 N2 134.6(3) 1_555 2_465 ?
F2 F1 F2 110.56(14) 4_665 5_666 ?
F2 F1 F2 87.08(12) 4_665 8_556 ?
F2 F1 F2 146.33(15) 4_665 10_566 ?
F2 F1 F2 57.86(11) 4_665 11_656 ?
F2 F1 F2 63.62(13) 4_665 14_655 ?
F2 F1 F2 57.22(12) 4_665 15_565 ?
F2 F1 N2 134.6(3) 4_665 2_465 ?
F2 F1 F2 155.31(15) 5_666 8_556 ?
F2 F1 F2 60.31(9) 5_666 10_566 ?
F2 F1 F2 113.82(13) 5_666 11_656 ?
F2 F1 F2 57.86(11) 5_666 14_655 ?
F2 F1 F2 146.33(15) 5_666 15_565 ?
F2 F1 N2 77.7(2) 5_666 2_465 ?
F2 F1 F2 113.82(13) 8_556 10_566 ?
F2 F1 F2 60.31(9) 8_556 11_656 ?
F2 F1 F2 146.33(15) 8_556 14_655 ?
F2 F1 F2 57.86(11) 8_556 15_565 ?
F2 F1 N2 77.7(2) 8_556 2_465 ?
F2 F1 F2 155.31(15) 10_566 11_656 ?
F2 F1 F2 87.08(12) 10_566 14_655 ?
F2 F1 F2 110.56(14) 10_566 15_565 ?
F2 F1 N2 77.7(2) 10_566 2_465 ?
F2 F1 F2 110.56(14) 11_656 14_655 ?
F2 F1 F2 87.08(12) 11_656 15_565 ?
F2 F1 N2 77.7(2) 11_656 2_465 ?
F2 F1 F2 90.81(14) 14_655 15_565 ?
F2 F1 N2 134.6(3) 14_655 2_465 ?
F2 F1 N2 134.6(3) 15_565 2_465 ?
Mn1 F2 Fe2 145.89(8) 1_555 1_555 ?
Mn1 F2 F1 102.57(17) 1_555 1_555 ?
Mn1 F2 F1 160.18(11) 1_555 5_666 ?
Mn1 F2 F2 45.39(9) 1_555 3_656 ?
Mn1 F2 F2 135.51(12) 1_555 10_566 ?
Mn1 F2 F2 117.34(11) 1_555 14_655 ?
Mn1 F2 N1 50.45(14) 1_555 1_555 ?
Mn1 F2 N1 46.62(14) 1_555 3_656 ?
Mn1 F2 N2 108.28(11) 1_555 6_645 ?
Mn1 F2 C1 69.1(2) 1_555 1_555 ?
Mn1 F2 C1 107.99(17) 1_555 8_546 ?
Fe1 F2 Fe2 145.89(8) 1_555 1_555 ?
Fe1 F2 F1 102.57(17) 1_555 1_555 ?
Fe1 F2 F1 160.18(11) 1_555 5_666 ?
Fe1 F2 F2 45.39(9) 1_555 3_656 ?
Fe1 F2 F2 135.51(12) 1_555 10_566 ?
Fe1 F2 F2 117.34(11) 1_555 14_655 ?
Fe1 F2 N1 50.45(14) 1_555 1_555 ?
Fe1 F2 N1 46.62(14) 1_555 3_656 ?
Fe1 F2 N2 108.28(11) 1_555 6_645 ?
Fe1 F2 C1 69.1(2) 1_555 1_555 ?
Fe1 F2 C1 107.99(17) 1_555 8_546 ?
Fe2 F2 F1 45.01(10) 1_555 1_555 ?
Fe2 F2 F1 47.90(9) 1_555 5_666 ?
Fe2 F2 F2 167.03(12) 1_555 3_656 ?
Fe2 F2 F2 45.36(9) 1_555 10_566 ?
Fe2 F2 F2 101.64(12) 1_555 15_565 ?
Fe2 F2 N1 125.2(2) 1_555 1_555 ?
Fe2 F2 N1 121.4(2) 1_555 3_656 ?
Fe2 F2 N2 90.8(2) 1_555 6_645 ?
Fe2 F2 C1 102.48(14) 1_555 1_555 ?
Fe2 F2 C1 100.4(2) 1_555 8_546 ?
F1 F2 F1 92.92(12) 1_555 5_666 ?
F1 F2 F2 147.60(18) 1_555 3_656 ?
F1 F2 F2 58.59(11) 1_555 10_566 ?
F1 F2 F2 61.39(13) 1_555 14_655 ?
F1 F2 F2 58.19(13) 1_555 15_565 ?
F1 F2 N1 91.08(18) 1_555 1_555 ?
F1 F2 N1 105.2(2) 1_555 3_656 ?
F1 F2 N2 127.3(2) 1_555 6_645 ?
F1 F2 C1 72.55(20) 1_555 1_555 ?
F1 F2 C1 121.29(20) 1_555 8_546 ?
F1 F2 F2 119.36(14) 5_666 3_656 ?
F1 F2 F2 63.56(12) 5_666 10_566 ?
F1 F2 F2 59.84(9) 5_666 14_655 ?
F1 F2 F2 146.91(12) 5_666 15_565 ?
F1 F2 N1 142.67(16) 5_666 1_555 ?
F1 F2 N1 117.47(18) 5_666 3_656 ?
F1 F2 N2 51.95(17) 5_666 6_645 ?
F1 F2 C1 128.3(2) 5_666 1_555 ?
F1 F2 C1 73.18(18) 5_666 8_546 ?
F2 F2 F2 136.45(13) 3_656 10_566 ?
F2 F2 F2 130.84(12) 3_656 14_655 ?
F2 F2 F2 90.00(11) 3_656 15_565 ?
F2 F2 N1 65.55(14) 3_656 1_555 ?
F2 F2 N1 59.09(13) 3_656 3_656 ?
F2 F2 N2 77.10(11) 3_656 6_645 ?
F2 F2 C1 87.9(2) 3_656 1_555 ?
F2 F2 C1 74.87(17) 3_656 8_546 ?
F2 F2 F2 90.00(11) 10_566 14_655 ?
F2 F2 F2 106.68(13) 10_566 15_565 ?
F2 F2 N1 87.56(16) 10_566 1_555 ?
F2 F2 N1 163.4(2) 10_566 3_656 ?
F2 F2 N2 114.9(2) 10_566 6_645 ?
F2 F2 C1 66.77(17) 10_566 1_555 ?
F2 F2 C1 64.44(17) 10_566 8_546 ?
F2 F2 F2 90.00(12) 14_655 15_565 ?
F2 F2 N1 148.5(2) 14_655 1_555 ?
F2 F2 N1 77.70(15) 14_655 3_656 ?
F2 F2 N2 66.66(14) 14_655 6_645 ?
F2 F2 C1 133.9(3) 14_655 1_555 ?
F2 F2 C1 132.9(2) 14_655 8_546 ?
F2 F2 N1 60.92(14) 15_565 1_555 ?
F2 F2 N1 62.73(14) 15_565 3_656 ?
F2 F2 N2 131.36(15) 15_565 6_645 ?
F2 F2 C1 62.31(17) 15_565 1_555 ?
F2 F2 C1 133.73(16) 15_565 8_546 ?
N1 F2 N1 97.1(2) 1_555 3_656 ?
N1 F2 N2 141.29(20) 1_555 6_645 ?
N1 F2 C1 73.10(12) 1_555 8_546 ?
N1 F2 N2 70.62(12) 3_656 6_645 ?
N1 F2 C1 114.2(3) 3_656 1_555 ?
N1 F2 C1 132.2(2) 3_656 8_546 ?
N2 F2 C1 158.9(3) 6_645 1_555 ?
N2 F2 C1 88.2(2) 6_645 8_546 ?
C1 F2 C1 73.48(15) 1_555 8_546 ?
Mn1 N1 Mn1 104.64(14) 1_555 2_566 ?
Mn1 N1 Fe1 104.64(14) 1_555 2_566 ?
Mn1 N1 N1 134.3(4) 1_555 4_765 ?
Mn1 N1 N2 153.8(4) 1_555 1_555 ?
Mn1 N1 C1 117.4(6) 1_555 1_555 ?
Mn1 N1 C1 168.9(4) 1_555 4_765 ?
Mn1 N1 Fe1 104.64(14) 2_566 1_555 ?
Mn1 N1 F2 130.33(13) 2_566 1_555 ?
Mn1 N1 F2 75.99(12) 2_566 3_656 ?
Mn1 N1 F2 75.99(12) 2_566 13_666 ?
Mn1 N1 F2 130.33(13) 2_566 15_565 ?
Mn1 N1 N2 101.6(3) 2_566 1_555 ?
Mn1 N1 C1 138.0(5) 2_566 1_555 ?
Mn1 N1 C1 64.3(3) 2_566 4_765 ?
Fe1 N1 Fe1 104.64(14) 1_555 2_566 ?
Fe1 N1 N1 134.3(4) 1_555 4_765 ?
Fe1 N1 N2 153.8(4) 1_555 1_555 ?
Fe1 N1 C1 117.4(6) 1_555 1_555 ?
Fe1 N1 C1 168.9(4) 1_555 4_765 ?
Fe1 N1 F2 130.33(13) 2_566 1_555 ?
Fe1 N1 F2 75.99(12) 2_566 3_656 ?
Fe1 N1 F2 75.99(12) 2_566 13_666 ?
Fe1 N1 F2 130.33(13) 2_566 15_565 ?
Fe1 N1 N2 101.6(3) 2_566 1_555 ?
Fe1 N1 C1 138.0(5) 2_566 1_555 ?
Fe1 N1 C1 64.3(3) 2_566 4_765 ?
F2 N1 F2 55.36(13) 1_555 3_656 ?
F2 N1 F2 82.93(14) 1_555 13_666 ?
F2 N1 F2 58.17(13) 1_555 15_565 ?
F2 N1 N1 148.5(4) 1_555 4_765 ?
F2 N1 N2 116.5(3) 1_555 1_555 ?
F2 N1 C1 84.9(5) 1_555 1_555 ?
F2 N1 C1 144.1(4) 1_555 4_765 ?
F2 N1 F2 54.53(13) 3_656 13_666 ?
F2 N1 F2 82.93(14) 3_656 15_565 ?
F2 N1 N1 102.3(4) 3_656 4_765 ?
F2 N1 N2 152.4(4) 3_656 1_555 ?
F2 N1 C1 138.8(6) 3_656 1_555 ?
F2 N1 C1 131.7(4) 3_656 4_765 ?
F2 N1 F2 55.36(13) 13_666 15_565 ?
F2 N1 N1 102.3(4) 13_666 4_765 ?
F2 N1 N2 152.4(4) 13_666 1_555 ?
F2 N1 C1 138.8(6) 13_666 1_555 ?
F2 N1 C1 131.7(4) 13_666 4_765 ?
F2 N1 N1 148.5(4) 15_565 4_765 ?
F2 N1 N2 116.5(3) 15_565 1_555 ?
F2 N1 C1 84.9(5) 15_565 1_555 ?
F2 N1 C1 144.1(4) 15_565 4_765 ?
N1 N1 N2 71.9(5) 4_765 1_555 ?
N1 N1 C1 108.3(7) 4_765 1_555 ?
C1 N1 C1 73.7(6) 1_555 4_765 ?
F1 N2 F2 50.39(19) 2_565 6_654 ?
F1 N2 F2 50.39(19) 2_565 7_564 ?
F1 N2 F2 50.39(19) 2_565 9_554 ?
F1 N2 F2 50.39(19) 2_565 12_664 ?
F1 N2 N1 161.9(4) 2_565 1_555 ?
F1 N2 N1 161.9(4) 2_565 4_765 ?
F1 N2 C1 128.6(6) 2_565 1_555 ?
F1 N2 C1 128.6(6) 2_565 4_765 ?
F2 N2 F2 100.79(14) 6_654 7_564 ?
F2 N2 F2 46.68(12) 6_654 9_554 ?
F2 N2 F2 82.72(13) 6_654 12_664 ?
F2 N2 N1 118.9(3) 6_654 1_555 ?
F2 N2 N1 136.8(3) 6_654 4_765 ?
F2 N2 C1 95.0(4) 6_654 1_555 ?
F2 N2 C1 135.0(5) 6_654 4_765 ?
F2 N2 F2 82.72(13) 7_564 9_554 ?
F2 N2 F2 46.68(12) 7_564 12_664 ?
F2 N2 N1 136.8(3) 7_564 1_555 ?
F2 N2 N1 118.9(3) 7_564 4_765 ?
F2 N2 C1 135.0(5) 7_564 1_555 ?
F2 N2 C1 95.0(4) 7_564 4_765 ?
F2 N2 F2 100.79(14) 9_554 12_664 ?
F2 N2 N1 136.8(3) 9_554 1_555 ?
F2 N2 N1 118.9(3) 9_554 4_765 ?
F2 N2 C1 135.0(5) 9_554 1_555 ?
F2 N2 C1 95.0(4) 9_554 4_765 ?
F2 N2 N1 118.9(3) 12_664 1_555 ?
F2 N2 N1 136.8(3) 12_664 4_765 ?
F2 N2 C1 95.0(4) 12_664 1_555 ?
F2 N2 C1 135.0(5) 12_664 4_765 ?
N1 N2 C1 69.5(5) 1_555 4_765 ?
N1 N2 C1 69.5(5) 4_765 1_555 ?
C1 N2 C1 102.9(8) 1_555 4_765 ?
Mn1 C1 F2 87.12(16) 1_555 8_556 ?
Mn1 C1 F2 87.12(16) 1_555 10_566 ?
Mn1 C1 N1 79.0(3) 1_555 4_765 ?
Mn1 C1 N2 152.2(5) 1_555 1_555 ?
Mn1 C1 C1 113.7(4) 1_555 4_765 ?
Fe1 C1 F2 87.12(16) 1_555 8_556 ?
Fe1 C1 F2 87.12(16) 1_555 10_566 ?
Fe1 C1 N1 79.0(3) 1_555 4_765 ?
Fe1 C1 N2 152.2(5) 1_555 1_555 ?
Fe1 C1 C1 113.7(4) 1_555 4_765 ?
F2 C1 F2 89.06(16) 1_555 8_556 ?
F2 C1 F2 48.79(15) 1_555 10_566 ?
F2 C1 F2 55.39(16) 1_555 15_565 ?
F2 C1 N1 72.3(4) 1_555 1_555 ?
F2 C1 N1 104.9(3) 1_555 4_765 ?
F2 C1 N2 152.31(7) 1_555 1_555 ?
F2 C1 C1 133.9(4) 1_555 4_765 ?
F2 C1 F2 87.46(15) 8_556 10_566 ?
F2 C1 F2 48.79(15) 8_556 15_565 ?
F2 C1 N1 116.4(5) 8_556 1_555 ?
F2 C1 N1 134.3(3) 8_556 4_765 ?
F2 C1 N2 112.4(4) 8_556 1_555 ?
F2 C1 C1 132.9(4) 8_556 4_765 ?
F2 C1 F2 89.06(16) 10_566 15_565 ?
F2 C1 N1 116.4(5) 10_566 1_555 ?
F2 C1 N1 134.3(3) 10_566 4_765 ?
F2 C1 N2 112.4(4) 10_566 1_555 ?
F2 C1 C1 132.9(4) 10_566 4_765 ?
F2 C1 N1 72.3(4) 15_565 1_555 ?
F2 C1 N1 104.9(3) 15_565 4_765 ?
F2 C1 N2 152.3(4) 15_565 1_555 ?
F2 C1 C1 133.9(4) 15_565 4_765 ?
N1 C1 N2 110.2(8) 1_555 1_555 ?
N1 C1 C1 71.7(6) 1_555 4_765 ?
N1 C1 N2 73.2(5) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_MnFeF5Htaz_2
_database_code_depnum_ccdc_archive 'CCDC 1527830'
_audit_update_record             
;
2017-01-16 deposited with the CCDC.
2017-03-20 downloaded from the CCDC.
;

#=============================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        
; ?
;
_chemical_name_common            ?
_chemical_formula_moiety         ?
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'C2 F5 Fe1.06 Mn0.94 N3'
_chemical_formula_weight         271.89
_chemical_melting_point          ?
_chemical_compound_source        ? # for minerals and 
# natural products

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mn Mn 0.337 0.728 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.346 0.844 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

#=============================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_symmetry_space_group_name_Hall  '-I 2b 2'

loop_
_symmetry_equiv_pos_as_xyz #<--must include 'x,y,z'
x,y,z
x+1/2,-y+1/2,-z+1/2
-x+1/2,y,-z+1/2
-x,-y+1/2,z
-x,-y,-z
-x+1/2,y+1/2,z+1/2
x+1/2,-y,z+1/2
x,y+1/2,-z
x+1/2,y+1/2,z+1/2
x,-y,-z
-x,y+1/2,-z
-x+1/2,-y,z+1/2
-x+1/2,-y+1/2,-z+1/2
-x,y,z
x,-y+1/2,z
x+1/2,y,-z+1/2

_cell_length_a                   9.2919(3)
_cell_length_b                   7.5003(2)
_cell_length_c                   9.6020(3)
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_volume                     669.18(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    296
_cell_special_details            
; ?
;
# The next three fields give the specimen dimensions in mm.  The equatorial
# plane contains the incident and diffracted beam.

_pd_spec_size_axial              ? # perpendicular to 
# equatorial plane
_pd_spec_size_equat              ? # parallel to 
# scattering vector
# in transmission
_pd_spec_size_thick              ? # parallel to 
# scattering vector
# in reflection

# The next five fields are character fields that describe the specimen.

_pd_spec_mounting                
# This field should be
# used to give details of the 
# container.
; ?
;
_pd_spec_mount_mode              ? # options are 'reflection'
# or 'transmission'
_pd_spec_shape                   ? # options are 'cylinder' 
# 'flat_sheet' or 'irregular'
_pd_char_particle_morphology     ?
_pd_char_colour                  ? # use ICDD colour descriptions

# The following three fields describe the preparation of the specimen.
# The cooling rate is in K/min.  The pressure at which the sample was 
# prepared is in kPa.  The temperature of preparation is in K.        

_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

# The next four fields are normally only needed for transmission experiments.

_exptl_absorpt_coefficient_mu    ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?

#=============================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           
; ?
;

# The following item is used to identify the equipment used to record 
# the powder pattern when the diffractogram was measured at a laboratory 
# other than the authors' home institution, e.g. when neutron or synchrotron
# radiation is used.

_pd_instr_location               
; ?
;
_pd_calibration_special_details  
# description of the method used
# to calibrate the instrument
; ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71069
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Xpert Panaltycal'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ? # Not in version 2.0.1
_diffrn_detector                 ?
_diffrn_detector_type            ? # make or model of detector
_pd_meas_scan_method             ? # options are 'step', 'cont',
# 'tof', 'fixed' or
# 'disp' (= dispersive)
_pd_meas_special_details         
;  ?
;

#  The following four items give details of the measured (not processed)
#  powder pattern.  Angles are in degrees.

_pd_meas_number_of_points        5679
_pd_meas_2theta_range_min        5.11462
_pd_meas_2theta_range_max        100.00121
_pd_meas_2theta_range_inc        0.016712

#=============================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

# Use the next field to give any special details about the fitting of the
# powder pattern.

_pd_proc_ls_special_details      
; ?
;

# The next three items are given as text.

_pd_proc_ls_profile_function     ?
_pd_proc_ls_background_function  ?
_pd_proc_ls_pref_orient_corr     
; ?
;

#  The following profile R-factors are NOT CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These are the current CIF standard

_pd_proc_ls_prof_R_factor        0.9515
_pd_proc_ls_prof_wR_factor       1.2402
_pd_proc_ls_prof_wR_expected     0.8840

#  The following profile R-factors are CORRECTED for background
#  The sum is extended to all non-excluded points.
#  These items are not in the current CIF standard, but are defined above

_pd_proc_ls_prof_cR_factor       16.2015
_pd_proc_ls_prof_cwR_factor      8.5859
_pd_proc_ls_prof_cwR_expected    6.1197

#  The following items are not in the CIF standard, but are defined above

_pd_proc_ls_prof_chi2            1.9684
_pd_proc_ls_prof_echi2           2.0383
_refine_ls_goodness_of_fit_all   1.4030

#  Items related to LS refinement

_refine_ls_R_I_factor            3.9602
_refine_ls_number_reflns         439
_refine_ls_number_parameters     67
_refine_ls_number_restraints     0

# The following four items apply to angular dispersive measurements.
# 2theta minimum, maximum and increment (in degrees) are for the 
# intensities used in the refinement.

_pd_proc_2theta_range_min        4.9098
_pd_proc_2theta_range_max        99.7964
_pd_proc_2theta_range_inc        0.016712
_pd_proc_wavelength              1.540560

_pd_block_diffractogram_id       ? # The id used for the block containing
# the powder pattern profile (section 11)

# Give appropriate details in the next two text fields.

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

# The following items are used to identify the programs used.

_computing_data_collection       ?
_computing_structure_solution    ?
_computing_structure_refinement  FULLPROF
_computing_molecular_graphics    ?
_computing_publication_material  ?

#=============================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type # Not in version 2.0.1
_atom_site_type_symbol
Mn1 0.75000 0.75000 0.75000 0.01267 0.94000 Uiso Mn
Fe1 0.75000 0.75000 0.75000 0.01267 0.06000 Uiso Fe
Fe2 0.50000 0.50000 0.50000 0.01267 1.00000 Uiso Fe
F1 0.50000 0.75000 0.4289(5) 0.01267 1.00000 Uiso F
F2 0.6456(2) 0.5505(3) 0.6354(2) 0.01267 1.00000 Uiso F
N1 0.9293(5) 0.75000 0.5708(6) 0.01267 1.00000 Uiso N
N2 1.00000 0.75000 0.3591(8) 0.01267 1.00000 Uiso N
C1 0.8844(7) 0.75000 0.4458(7) 0.01267 1.00000 Uiso C

# Note: if the displacement parameters were refined anisotropically
# the U matrices should be given as for single-crystal studies.

#=============================================================================

# 10. DISTANCES AND ANGLES / MOLECULAR GEOMETRY 

_geom_special_details            ?

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mn1 F2 2.095(2) 1_555 ?
Mn1 F2 2.095(2) 3_656 ?
Mn1 F2 2.095(2) 13_666 ?
Mn1 F2 2.095(2) 15_565 ?
Mn1 N1 2.395(5) 1_555 ?
Mn1 N1 3.441(5) 2_466 ?
Mn1 N1 2.395(5) 3_656 ?
Mn1 N1 3.441(5) 4_765 ?
Mn1 C1 3.177(7) 1_555 ?
Mn1 C1 3.177(7) 3_656 ?
Fe1 F2 2.095(2) 1_555 ?
Fe1 F2 2.095(2) 3_656 ?
Fe1 F2 2.095(2) 13_666 ?
Fe1 F2 2.095(2) 15_565 ?
Fe1 N1 2.395(5) 1_555 ?
Fe1 N1 3.441(5) 2_466 ?
Fe1 N1 2.395(5) 3_656 ?
Fe1 N1 3.441(5) 4_765 ?
Fe1 C1 3.177(7) 1_555 ?
Fe1 C1 3.177(7) 3_656 ?
Fe2 F1 1.9955(16) 1_555 ?
Fe2 F1 1.9955(16) 5_666 ?
Fe2 F2 1.9142(19) 1_555 ?
Fe2 F2 1.9142(19) 5_666 ?
Fe2 F2 1.9142(19) 10_566 ?
Fe2 F2 1.9142(19) 14_655 ?
F1 Fe2 1.9955(16) 1_555 ?
F1 Fe2 1.9955(16) 4_665 ?
F1 F2 2.829(4) 1_555 ?
F1 F2 2.829(4) 4_665 ?
F1 F2 2.700(2) 5_666 ?
F1 F2 2.700(2) 8_556 ?
F1 F2 2.700(2) 10_566 ?
F1 F2 2.700(2) 11_656 ?
F1 F2 2.829(4) 14_655 ?
F1 F2 2.829(4) 15_565 ?
F1 N2 2.765(9) 2_465 ?
F2 Mn1 2.095(2) 1_555 ?
F2 Fe1 2.095(2) 1_555 ?
F2 Fe2 1.9142(19) 1_555 ?
F2 F1 2.829(4) 1_555 ?
F2 F1 2.700(2) 5_666 ?
F2 F2 2.934(3) 3_656 ?
F2 F2 2.708(3) 10_566 ?
F2 F2 2.706(3) 14_655 ?
F2 F2 2.993(3) 15_565 ?
F2 N1 3.094(5) 1_555 ?
F2 N1 3.268(5) 3_656 ?
F2 N2 3.395(5) 6_645 ?
F2 C1 3.237(6) 1_555 ?
F2 C1 3.257(5) 8_546 ?
N1 Mn1 2.395(5) 1_555 ?
N1 Mn1 3.441(5) 2_566 ?
N1 Fe1 2.395(5) 1_555 ?
N1 Fe1 3.441(5) 2_566 ?
N1 F2 3.094(5) 1_555 ?
N1 F2 3.268(5) 3_656 ?
N1 F2 3.268(5) 13_666 ?
N1 F2 3.094(5) 15_565 ?
N1 N1 1.314(7) 4_765 ?
N1 N2 2.136(9) 1_555 ?
N1 C1 1.271(9) 1_555 ?
N1 C1 2.106(8) 4_765 ?
N2 F1 2.765(9) 2_565 ?
N2 F2 3.395(5) 6_654 ?
N2 F2 3.395(5) 7_564 ?
N2 F2 3.395(5) 9_554 ?
N2 F2 3.395(5) 12_664 ?
N2 N1 2.136(9) 1_555 ?
N2 N1 2.136(9) 4_765 ?
N2 C1 1.359(8) 1_555 ?
N2 C1 1.359(8) 4_765 ?
C1 Mn1 3.177(7) 1_555 ?
C1 Fe1 3.177(7) 1_555 ?
C1 F2 3.237(6) 1_555 ?
C1 F2 3.257(5) 8_556 ?
C1 F2 3.257(5) 10_566 ?
C1 F2 3.237(6) 15_565 ?
C1 N1 1.271(9) 1_555 ?
C1 N1 2.106(8) 4_765 ?
C1 N2 1.359(8) 1_555 ?
C1 C1 2.148(9) 4_765 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Mn1 F2 88.86(13) 1_555 3_656 ?
F2 Mn1 F2 180.00(18) 1_555 13_666 ?
F2 Mn1 F2 91.14(15) 1_555 15_565 ?
F2 Mn1 N1 86.8(2) 1_555 1_555 ?
F2 Mn1 N1 82.05(19) 1_555 2_466 ?
F2 Mn1 N1 93.2(2) 1_555 3_656 ?
F2 Mn1 N1 97.95(19) 1_555 4_765 ?
F2 Mn1 C1 72.5(2) 1_555 1_555 ?
F2 Mn1 C1 107.5(3) 1_555 3_656 ?
F2 Mn1 F2 91.14(15) 3_656 13_666 ?
F2 Mn1 F2 180.00(18) 3_656 15_565 ?
F2 Mn1 N1 93.2(2) 3_656 1_555 ?
F2 Mn1 N1 97.95(19) 3_656 2_466 ?
F2 Mn1 N1 86.8(2) 3_656 3_656 ?
F2 Mn1 N1 82.05(19) 3_656 4_765 ?
F2 Mn1 C1 107.5(3) 3_656 1_555 ?
F2 Mn1 C1 72.5(2) 3_656 3_656 ?
F2 Mn1 F2 88.86(13) 13_666 15_565 ?
F2 Mn1 N1 93.2(2) 13_666 1_555 ?
F2 Mn1 N1 97.95(19) 13_666 2_466 ?
F2 Mn1 N1 86.8(2) 13_666 3_656 ?
F2 Mn1 N1 82.05(19) 13_666 4_765 ?
F2 Mn1 C1 107.5(3) 13_666 1_555 ?
F2 Mn1 C1 72.5(2) 13_666 3_656 ?
F2 Mn1 N1 86.8(2) 15_565 1_555 ?
F2 Mn1 N1 82.05(19) 15_565 2_466 ?
F2 Mn1 N1 93.2(2) 15_565 3_656 ?
F2 Mn1 N1 97.95(19) 15_565 4_765 ?
F2 Mn1 C1 72.5(2) 15_565 1_555 ?
F2 Mn1 C1 107.5(3) 15_565 3_656 ?
N1 Mn1 N1 164.1(3) 1_555 2_466 ?
N1 Mn1 N1 180.0(4) 1_555 3_656 ?
N1 Mn1 C1 159.1(4) 1_555 3_656 ?
N1 Mn1 N1 180.0(3) 2_466 4_765 ?
N1 Mn1 C1 143.2(3) 2_466 1_555 ?
N1 Mn1 N1 164.1(3) 3_656 4_765 ?
N1 Mn1 C1 159.1(4) 3_656 1_555 ?
N1 Mn1 C1 143.2(3) 4_765 3_656 ?
C1 Mn1 C1 180.0(4) 1_555 3_656 ?
F2 Fe1 F2 88.86(13) 1_555 3_656 ?
F2 Fe1 F2 180.00(18) 1_555 13_666 ?
F2 Fe1 F2 91.14(15) 1_555 15_565 ?
F2 Fe1 N1 86.8(2) 1_555 1_555 ?
F2 Fe1 N1 82.05(19) 1_555 2_466 ?
F2 Fe1 N1 93.2(2) 1_555 3_656 ?
F2 Fe1 N1 97.95(19) 1_555 4_765 ?
F2 Fe1 C1 72.5(2) 1_555 1_555 ?
F2 Fe1 C1 107.5(3) 1_555 3_656 ?
F2 Fe1 F2 91.14(15) 3_656 13_666 ?
F2 Fe1 F2 180.00(18) 3_656 15_565 ?
F2 Fe1 N1 93.2(2) 3_656 1_555 ?
F2 Fe1 N1 97.95(19) 3_656 2_466 ?
F2 Fe1 N1 86.8(2) 3_656 3_656 ?
F2 Fe1 N1 82.05(19) 3_656 4_765 ?
F2 Fe1 C1 107.5(3) 3_656 1_555 ?
F2 Fe1 C1 72.5(2) 3_656 3_656 ?
F2 Fe1 F2 88.86(13) 13_666 15_565 ?
F2 Fe1 N1 93.2(2) 13_666 1_555 ?
F2 Fe1 N1 97.95(19) 13_666 2_466 ?
F2 Fe1 N1 86.8(2) 13_666 3_656 ?
F2 Fe1 N1 82.05(19) 13_666 4_765 ?
F2 Fe1 C1 107.5(3) 13_666 1_555 ?
F2 Fe1 C1 72.5(2) 13_666 3_656 ?
F2 Fe1 N1 86.8(2) 15_565 1_555 ?
F2 Fe1 N1 82.05(19) 15_565 2_466 ?
F2 Fe1 N1 93.2(2) 15_565 3_656 ?
F2 Fe1 N1 97.95(19) 15_565 4_765 ?
F2 Fe1 C1 72.5(2) 15_565 1_555 ?
F2 Fe1 C1 107.5(3) 15_565 3_656 ?
N1 Fe1 N1 164.1(3) 1_555 2_466 ?
N1 Fe1 N1 180.0(4) 1_555 3_656 ?
N1 Fe1 C1 159.1(4) 1_555 3_656 ?
N1 Fe1 N1 180.0(3) 2_466 4_765 ?
N1 Fe1 C1 143.2(3) 2_466 1_555 ?
N1 Fe1 N1 164.1(3) 3_656 4_765 ?
N1 Fe1 C1 159.1(4) 3_656 1_555 ?
N1 Fe1 C1 143.2(3) 4_765 3_656 ?
C1 Fe1 C1 180.0(4) 1_555 3_656 ?
F1 Fe2 F1 180.00(15) 1_555 5_666 ?
F1 Fe2 F2 92.66(18) 1_555 1_555 ?
F1 Fe2 F2 87.34(12) 1_555 5_666 ?
F1 Fe2 F2 87.34(12) 1_555 10_566 ?
F1 Fe2 F2 92.66(18) 1_555 14_655 ?
F1 Fe2 F2 87.34(12) 5_666 1_555 ?
F1 Fe2 F2 92.66(18) 5_666 5_666 ?
F1 Fe2 F2 92.66(18) 5_666 10_566 ?
F1 Fe2 F2 87.34(12) 5_666 14_655 ?
F2 Fe2 F2 180.00(18) 1_555 5_666 ?
F2 Fe2 F2 90.05(14) 1_555 10_566 ?
F2 Fe2 F2 89.95(14) 1_555 14_655 ?
F2 Fe2 F2 89.95(14) 5_666 10_566 ?
F2 Fe2 F2 90.05(14) 5_666 14_655 ?
F2 Fe2 F2 180.00(18) 10_566 14_655 ?
Fe2 F1 Fe2 139.99(7) 1_555 4_665 ?
Fe2 F1 F2 104.91(13) 1_555 4_665 ?
Fe2 F1 F2 45.08(8) 1_555 5_666 ?
Fe2 F1 F2 149.60(13) 1_555 8_556 ?
Fe2 F1 F2 45.08(8) 1_555 10_566 ?
Fe2 F1 F2 149.60(13) 1_555 11_656 ?
Fe2 F1 F2 104.91(13) 1_555 15_565 ?
Fe2 F1 N2 110.0(3) 1_555 2_465 ?
Fe2 F1 F2 104.91(13) 4_665 1_555 ?
Fe2 F1 F2 149.60(13) 4_665 5_666 ?
Fe2 F1 F2 45.08(8) 4_665 8_556 ?
Fe2 F1 F2 149.60(13) 4_665 10_566 ?
Fe2 F1 F2 45.08(8) 4_665 11_656 ?
Fe2 F1 F2 104.91(13) 4_665 14_655 ?
Fe2 F1 N2 110.0(3) 4_665 2_465 ?
F2 F1 F2 90.99(14) 1_555 4_665 ?
F2 F1 F2 87.61(12) 1_555 5_666 ?
F2 F1 F2 111.23(14) 1_555 8_556 ?
F2 F1 F2 58.61(11) 1_555 10_566 ?
F2 F1 F2 147.30(15) 1_555 11_656 ?
F2 F1 F2 57.15(12) 1_555 14_655 ?
F2 F1 F2 63.88(13) 1_555 15_565 ?
F2 F1 N2 134.5(3) 1_555 2_465 ?
F2 F1 F2 111.23(14) 4_665 5_666 ?
F2 F1 F2 87.61(12) 4_665 8_556 ?
F2 F1 F2 147.30(15) 4_665 10_566 ?
F2 F1 F2 58.61(11) 4_665 11_656 ?
F2 F1 F2 63.88(13) 4_665 14_655 ?
F2 F1 F2 57.15(12) 4_665 15_565 ?
F2 F1 N2 134.5(3) 4_665 2_465 ?
F2 F1 F2 153.56(15) 5_666 8_556 ?
F2 F1 F2 60.14(9) 5_666 10_566 ?
F2 F1 F2 113.16(13) 5_666 11_656 ?
F2 F1 F2 58.61(11) 5_666 14_655 ?
F2 F1 F2 147.30(15) 5_666 15_565 ?
F2 F1 N2 76.8(2) 5_666 2_465 ?
F2 F1 F2 113.16(13) 8_556 10_566 ?
F2 F1 F2 60.14(9) 8_556 11_656 ?
F2 F1 F2 147.30(15) 8_556 14_655 ?
F2 F1 F2 58.61(11) 8_556 15_565 ?
F2 F1 N2 76.8(2) 8_556 2_465 ?
F2 F1 F2 153.56(15) 10_566 11_656 ?
F2 F1 F2 87.61(12) 10_566 14_655 ?
F2 F1 F2 111.23(14) 10_566 15_565 ?
F2 F1 N2 76.8(2) 10_566 2_465 ?
F2 F1 F2 111.23(14) 11_656 14_655 ?
F2 F1 F2 87.61(12) 11_656 15_565 ?
F2 F1 N2 76.8(2) 11_656 2_465 ?
F2 F1 F2 90.99(14) 14_655 15_565 ?
F2 F1 N2 134.5(3) 14_655 2_465 ?
F2 F1 N2 134.5(3) 15_565 2_465 ?
Mn1 F2 Fe2 145.61(8) 1_555 1_555 ?
Mn1 F2 F1 102.23(17) 1_555 1_555 ?
Mn1 F2 F1 161.45(11) 1_555 5_666 ?
Mn1 F2 F2 45.57(9) 1_555 3_656 ?
Mn1 F2 F2 134.74(12) 1_555 10_566 ?
Mn1 F2 F2 117.58(11) 1_555 14_655 ?
Mn1 F2 N1 50.62(15) 1_555 1_555 ?
Mn1 F2 N1 47.03(15) 1_555 3_656 ?
Mn1 F2 N2 109.05(12) 1_555 6_645 ?
Mn1 F2 C1 69.4(2) 1_555 1_555 ?
Mn1 F2 C1 107.72(17) 1_555 8_546 ?
Fe1 F2 Fe2 145.61(8) 1_555 1_555 ?
Fe1 F2 F1 102.23(17) 1_555 1_555 ?
Fe1 F2 F1 161.45(11) 1_555 5_666 ?
Fe1 F2 F2 45.57(9) 1_555 3_656 ?
Fe1 F2 F2 134.74(12) 1_555 10_566 ?
Fe1 F2 F2 117.58(11) 1_555 14_655 ?
Fe1 F2 N1 50.62(15) 1_555 1_555 ?
Fe1 F2 N1 47.03(15) 1_555 3_656 ?
Fe1 F2 N2 109.05(12) 1_555 6_645 ?
Fe1 F2 C1 69.4(2) 1_555 1_555 ?
Fe1 F2 C1 107.72(17) 1_555 8_546 ?
Fe2 F2 F1 47.58(8) 1_555 5_666 ?
Fe2 F2 F2 167.65(12) 1_555 3_656 ?
Fe2 F2 F2 45.03(9) 1_555 14_655 ?
Fe2 F2 F2 101.41(12) 1_555 15_565 ?
Fe2 F2 N1 124.2(2) 1_555 1_555 ?
Fe2 F2 N1 121.8(2) 1_555 3_656 ?
Fe2 F2 N2 91.0(3) 1_555 6_645 ?
Fe2 F2 C1 101.2(2) 1_555 1_555 ?
Fe2 F2 C1 100.5(2) 1_555 8_546 ?
F1 F2 F1 92.39(12) 1_555 5_666 ?
F1 F2 F2 147.37(18) 1_555 3_656 ?
F1 F2 F2 58.33(11) 1_555 10_566 ?
F1 F2 F2 61.43(13) 1_555 14_655 ?
F1 F2 F2 58.06(13) 1_555 15_565 ?
F1 F2 N1 90.64(18) 1_555 1_555 ?
F1 F2 N1 105.1(3) 1_555 3_656 ?
F1 F2 N2 127.2(3) 1_555 6_645 ?
F1 F2 C1 71.88(20) 1_555 1_555 ?
F1 F2 C1 121.60(20) 1_555 8_546 ?
F1 F2 F2 120.19(14) 5_666 3_656 ?
F1 F2 F2 63.06(12) 5_666 10_566 ?
F1 F2 F2 59.93(9) 5_666 14_655 ?
F1 F2 F2 146.58(12) 5_666 15_565 ?
F1 F2 N1 141.69(16) 5_666 1_555 ?
F1 F2 N1 118.2(2) 5_666 3_656 ?
F1 F2 N2 52.47(19) 5_666 6_645 ?
F1 F2 C1 126.9(2) 5_666 1_555 ?
F1 F2 C1 73.09(18) 5_666 8_546 ?
F2 F2 F2 136.07(13) 3_656 10_566 ?
F2 F2 F2 131.40(12) 3_656 14_655 ?
F2 F2 F2 90.00(11) 3_656 15_565 ?
F2 F2 N1 65.60(15) 3_656 1_555 ?
F2 F2 N1 59.56(14) 3_656 3_656 ?
F2 F2 N2 77.81(11) 3_656 6_645 ?
F2 F2 C1 88.2(2) 3_656 1_555 ?
F2 F2 C1 74.28(17) 3_656 8_546 ?
F2 F2 F2 90.00(11) 10_566 14_655 ?
F2 F2 F2 106.24(13) 10_566 15_565 ?
F2 F2 N1 86.72(16) 10_566 1_555 ?
F2 F2 N1 163.1(2) 10_566 3_656 ?
F2 F2 N2 114.9(3) 10_566 6_645 ?
F2 F2 C1 65.75(17) 10_566 1_555 ?
F2 F2 C1 64.96(17) 10_566 8_546 ?
F2 F2 F2 90.00(12) 14_655 15_565 ?
F2 F2 N1 148.4(2) 14_655 1_555 ?
F2 F2 N1 77.71(17) 14_655 3_656 ?
F2 F2 N2 66.51(15) 14_655 6_645 ?
F2 F2 C1 133.3(3) 14_655 1_555 ?
F2 F2 C1 132.9(2) 14_655 8_546 ?
F2 F2 N1 61.08(14) 15_565 1_555 ?
F2 F2 N1 62.75(15) 15_565 3_656 ?
F2 F2 N2 131.60(16) 15_565 6_645 ?
F2 F2 C1 62.47(17) 15_565 1_555 ?
F2 F2 C1 133.78(16) 15_565 8_546 ?
N1 F2 N1 97.6(2) 1_555 3_656 ?
N1 F2 N2 142.0(2) 1_555 6_645 ?
N1 F2 C1 72.92(13) 1_555 8_546 ?
N1 F2 N2 70.91(14) 3_656 6_645 ?
N1 F2 C1 114.8(3) 3_656 1_555 ?
N1 F2 C1 131.9(2) 3_656 8_546 ?
N2 F2 C1 159.4(3) 6_645 1_555 ?
N2 F2 C1 87.9(2) 6_645 8_546 ?
C1 F2 C1 73.64(15) 1_555 8_546 ?
Mn1 N1 Mn1 104.07(15) 1_555 2_566 ?
Mn1 N1 Fe1 104.07(15) 1_555 2_566 ?
Mn1 N1 N1 134.1(4) 1_555 4_765 ?
Mn1 N1 N2 153.8(4) 1_555 1_555 ?
Mn1 N1 C1 116.8(6) 1_555 1_555 ?
Mn1 N1 C1 168.8(4) 1_555 4_765 ?
Mn1 N1 Fe1 104.07(15) 2_566 1_555 ?
Mn1 N1 F2 129.61(13) 2_566 1_555 ?
Mn1 N1 F2 75.69(13) 2_566 3_656 ?
Mn1 N1 F2 75.69(13) 2_566 13_666 ?
Mn1 N1 F2 129.61(13) 2_566 15_565 ?
Mn1 N1 N2 102.1(3) 2_566 1_555 ?
Mn1 N1 C1 139.2(6) 2_566 1_555 ?
Mn1 N1 C1 64.7(3) 2_566 4_765 ?
Fe1 N1 Fe1 104.07(15) 1_555 2_566 ?
Fe1 N1 N1 134.1(4) 1_555 4_765 ?
Fe1 N1 N2 153.8(4) 1_555 1_555 ?
Fe1 N1 C1 116.8(6) 1_555 1_555 ?
Fe1 N1 C1 168.8(4) 1_555 4_765 ?
Fe1 N1 F2 129.61(13) 2_566 1_555 ?
Fe1 N1 F2 75.69(13) 2_566 3_656 ?
Fe1 N1 F2 75.69(13) 2_566 13_666 ?
Fe1 N1 F2 129.61(13) 2_566 15_565 ?
Fe1 N1 N2 102.1(3) 2_566 1_555 ?
Fe1 N1 C1 139.2(6) 2_566 1_555 ?
Fe1 N1 C1 64.7(3) 2_566 4_765 ?
F2 N1 F2 54.84(14) 1_555 3_656 ?
F2 N1 F2 82.35(15) 1_555 13_666 ?
F2 N1 F2 57.84(13) 1_555 15_565 ?
F2 N1 N1 148.4(4) 1_555 4_765 ?
F2 N1 N2 116.9(3) 1_555 1_555 ?
F2 N1 C1 84.8(5) 1_555 1_555 ?
F2 N1 C1 144.5(4) 1_555 4_765 ?
F2 N1 F2 54.49(14) 3_656 13_666 ?
F2 N1 F2 82.35(15) 3_656 15_565 ?
F2 N1 N1 102.3(4) 3_656 4_765 ?
F2 N1 N2 152.5(4) 3_656 1_555 ?
F2 N1 C1 138.2(6) 3_656 1_555 ?
F2 N1 C1 131.8(4) 3_656 4_765 ?
F2 N1 F2 54.84(14) 13_666 15_565 ?
F2 N1 N1 102.3(4) 13_666 4_765 ?
F2 N1 N2 152.5(4) 13_666 1_555 ?
F2 N1 C1 138.2(6) 13_666 1_555 ?
F2 N1 C1 131.8(4) 13_666 4_765 ?
F2 N1 N1 148.4(4) 15_565 4_765 ?
F2 N1 N2 116.9(3) 15_565 1_555 ?
F2 N1 C1 84.8(5) 15_565 1_555 ?
F2 N1 C1 144.5(4) 15_565 4_765 ?
N1 N1 N2 72.1(6) 4_765 1_555 ?
N1 N1 C1 109.2(8) 4_765 1_555 ?
C1 N1 C1 74.4(6) 1_555 4_765 ?
F1 N2 F2 50.7(2) 2_565 6_654 ?
F1 N2 F2 50.7(2) 2_565 7_564 ?
F1 N2 F2 50.7(2) 2_565 9_554 ?
F1 N2 F2 50.7(2) 2_565 12_664 ?
F1 N2 N1 162.1(5) 2_565 1_555 ?
F1 N2 N1 162.1(5) 2_565 4_765 ?
F1 N2 C1 127.8(6) 2_565 1_555 ?
F1 N2 C1 127.8(6) 2_565 4_765 ?
F2 N2 F2 101.49(15) 6_654 7_564 ?
F2 N2 F2 46.97(13) 6_654 9_554 ?
F2 N2 F2 83.20(14) 6_654 12_664 ?
F2 N2 N1 118.7(3) 6_654 1_555 ?
F2 N2 N1 136.4(3) 6_654 4_765 ?
F2 N2 C1 94.2(4) 6_654 1_555 ?
F2 N2 C1 134.6(5) 6_654 4_765 ?
F2 N2 F2 83.20(14) 7_564 9_554 ?
F2 N2 F2 46.97(13) 7_564 12_664 ?
F2 N2 N1 136.4(3) 7_564 1_555 ?
F2 N2 N1 118.7(3) 7_564 4_765 ?
F2 N2 C1 134.6(5) 7_564 1_555 ?
F2 N2 C1 94.2(4) 7_564 4_765 ?
F2 N2 F2 101.49(15) 9_554 12_664 ?
F2 N2 N1 136.4(3) 9_554 1_555 ?
F2 N2 N1 118.7(3) 9_554 4_765 ?
F2 N2 C1 134.6(5) 9_554 1_555 ?
F2 N2 C1 94.2(4) 9_554 4_765 ?
F2 N2 N1 118.7(3) 12_664 1_555 ?
F2 N2 N1 136.4(3) 12_664 4_765 ?
F2 N2 C1 94.2(4) 12_664 1_555 ?
F2 N2 C1 134.6(5) 12_664 4_765 ?
N1 N2 C1 70.1(5) 1_555 4_765 ?
N1 N2 C1 70.1(5) 4_765 1_555 ?
C1 N2 C1 104.4(8) 1_555 4_765 ?
Mn1 C1 F2 87.27(16) 1_555 8_556 ?
Mn1 C1 F2 87.27(16) 1_555 10_566 ?
Mn1 C1 N1 78.4(3) 1_555 4_765 ?
Mn1 C1 N2 150.9(5) 1_555 1_555 ?
Mn1 C1 C1 113.1(4) 1_555 4_765 ?
Fe1 C1 F2 87.27(16) 1_555 8_556 ?
Fe1 C1 F2 87.27(16) 1_555 10_566 ?
Fe1 C1 N1 78.4(3) 1_555 4_765 ?
Fe1 C1 N2 150.9(5) 1_555 1_555 ?
Fe1 C1 C1 113.1(4) 1_555 4_765 ?
F2 C1 F2 89.28(16) 1_555 8_556 ?
F2 C1 F2 49.29(15) 1_555 10_566 ?
F2 C1 F2 55.07(16) 1_555 15_565 ?
F2 C1 N1 72.2(5) 1_555 1_555 ?
F2 C1 N1 104.1(3) 1_555 4_765 ?
F2 C1 N2 152.42(7) 1_555 1_555 ?
F2 C1 C1 133.3(4) 1_555 4_765 ?
F2 C1 F2 87.56(15) 8_556 10_566 ?
F2 C1 F2 49.29(15) 8_556 15_565 ?
F2 C1 N1 116.7(5) 8_556 1_555 ?
F2 C1 N1 134.1(3) 8_556 4_765 ?
F2 C1 N2 113.1(4) 8_556 1_555 ?
F2 C1 C1 132.9(4) 8_556 4_765 ?
F2 C1 F2 89.28(16) 10_566 15_565 ?
F2 C1 N1 116.7(5) 10_566 1_555 ?
F2 C1 N1 134.1(3) 10_566 4_765 ?
F2 C1 N2 113.1(4) 10_566 1_555 ?
F2 C1 C1 132.9(4) 10_566 4_765 ?
F2 C1 N1 72.2(5) 15_565 1_555 ?
F2 C1 N1 104.1(3) 15_565 4_765 ?
F2 C1 N2 152.4(5) 15_565 1_555 ?
F2 C1 C1 133.3(4) 15_565 4_765 ?
N1 C1 N2 108.6(8) 1_555 1_555 ?
N1 C1 C1 70.8(6) 1_555 4_765 ?
N1 C1 N2 72.5(6) 4_765 1_555 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?

#=============================================================================

#=============================================================================
# Additional structures (last six sections and associated data_? identifiers) 
# may be added at this point.                                                 
#=============================================================================

# The following lines are used to test the character set of files sent by     
# network email or other means. They are not part of the CIF data set.        
# abcdefghijklmnopqrstuvwxyzABCDEFGHIJKLMNOPQRSTUVWXYZ0123456789              
# !@#$%^&*()_+{}:"~<>?|\-=[];'`,./ 
